advertisement

IIW Collection A.F. Hobbacher Recommendations for Fatigue Design of Welded Joints and Components Second Edition IIW Collection Series editor Cécile Mayer, Villepinte, France About the Series The IIW Collection of Books is authored by experts from the 59 countries participating in the work of the 23 Technical Working Units of the International Institute of Welding, recognized as the largest worldwide network for welding and allied joining technologies. The IIW’s Mission is to operate as the global body for the science and application of joining technology, providing a forum for networking and knowledge exchange among scientists, researchers and industry. Published books, Best Practices, Recommendations or Guidelines are the outcome of collaborative work and technical discussions-they are truly validated by the IIW groups of experts in joining, cutting and surface treatment of metallic and non-metallic materials by such processes as welding, brazing, soldering, thermal cutting, thermal spraying, adhesive bonding and microjoining. IIW work also embraces allied ﬁelds including quality assurance, non-destructive testing, standardization, inspection, health and safety, education, training, qualiﬁcation, design and fabrication. More information about this series at http://www.springer.com/series/13906 A.F. Hobbacher Recommendations for Fatigue Design of Welded Joints and Components Second Edition IIW document IIW-2259-15 ex XIII-2460-13/XV-1440-13 This document is a revision of XIII-2151r4-07/XV-1254r4-07 123 A.F. Hobbacher University of Applied Sciences Wilhelmshaven Germany 1st edition: “Fatigue Design of Welded Joints and Components: Recommendations of IIW Joint Working Group XIII–XV”, Crc Press, 1996, ISBN: 978-1855733152 ISSN 2365-435X IIW Collection ISBN 978-3-319-23756-5 DOI 10.1007/978-3-319-23757-2 ISSN 2365-4368 (electronic) ISBN 978-3-319-23757-2 (eBook) Library of Congress Control Number: 2015950054 Springer Cham Heidelberg New York Dordrecht London © International Institute of Welding 1996 © Springer International Publishing Switzerland 2016 This work is subject to copyright. All rights are reserved by the Publisher, whether the whole or part of the material is concerned, speciﬁcally the rights of translation, reprinting, reuse of illustrations, recitation, broadcasting, reproduction on microﬁlms or in any other physical way, and transmission or information storage and retrieval, electronic adaptation, computer software, or by similar or dissimilar methodology now known or hereafter developed. The use of general descriptive names, registered names, trademarks, service marks, etc. in this publication does not imply, even in the absence of a speciﬁc statement, that such names are exempt from the relevant protective laws and regulations and therefore free for general use. The publisher, the authors and the editors are safe to assume that the advice and information in this book are believed to be true and accurate at the date of publication. Neither the publisher nor the authors or the editors give a warranty, express or implied, with respect to the material contained herein or for any errors or omissions that may have been made. Printed on acid-free paper Springer International Publishing AG Switzerland is part of Springer Science+Business Media (www.springer.com) The International Institute of Welding Mission “To act as the worldwide network for knowledge exchange of joining technologies to improve the global quality of life” The International Institute of Welding (IIW) was founded in 1948 by the welding institutes/societies of 13 countries who considered it crucial to make more rapid scientiﬁc and technical progress possible on a global level. Their vision was for the IIW to be the international vehicle by which innovation and best joining practices could be promoted, while providing an international platform for the exchange and dissemination of evolving welding technologies and applications. From its humble beginnings, the IIW is today a universal reference, recognized as the largest worldwide network for welding and allied joining technologies, boasting a current membership of 59 countries from the ﬁve continents. The IIW’s Mission is to operate as the global body for the science and application of joining technology, providing a forum for networking and knowledge exchange among scientists, researchers and industry. Through the work of its 23 Technical Commissions and Working Units, the organization’s technical focus encompasses the joining, cutting and surface treatment of metallic and non-metallic materials by such processes as welding, brazing, soldering, thermal cutting, thermal spraying, adhesive bonding and microjoining. IIW work also embraces allied ﬁelds including quality assurance, non-destructive testing, standardization, inspection, health and safety, education, training, qualiﬁcation, design and fabrication. Preface This document has been prepared as a result of an initiative by Commissions XIII and XV of the International Institute of Welding (IIW). The task was transferred to the Joint Working Group XIII–XV, where it was discussed and drafted in the years 1990–1996 and updated in the years 2002–2007. The recent version was updated in 2013–2014. The main points of that update were: Revision of the chapter on structural hot spot stress, consideration of aluminium at the effective notch stress method, a chapter on improvement techniques and a revision of the chapter on multi-axial loading. The update from 2014 contains, besides a continuous reﬁnement and adjustment to the most recent developments and completely revised chapters on fracture mechanics. vii Contents 1 General . . . . . . . . . . . . . . . . . . . . . . 1.1 Introduction . . . . . . . . . . . . . . . 1.2 Scope and Limitations . . . . . . . . 1.3 Deﬁnitions . . . . . . . . . . . . . . . . 1.4 Symbols. . . . . . . . . . . . . . . . . . 1.5 Basic Principles . . . . . . . . . . . . 1.6 Necessity of Fatigue Assessment . 1.7 Application of the Document . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1 1 1 2 5 7 7 8 2 Fatigue Actions (Loading). . . . . . . . . . . . . . . . . . . . . . . . . . 2.1 Basic Principles . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.1.1 Determination of Fatigue Actions (Loading) . . . . . 2.1.2 Stress Range . . . . . . . . . . . . . . . . . . . . . . . . . . 2.1.3 Types of Stress Concentrations and Notch Effects . 2.2 Determination of Stresses and Stress Intensity Factors . . . 2.2.1 Deﬁnition of Stress Components. . . . . . . . . . . . . 2.2.2 Nominal Stress . . . . . . . . . . . . . . . . . . . . . . . . . 2.2.3 Structural Hot Spot Stress . . . . . . . . . . . . . . . . . 2.2.4 Effective Notch Stress . . . . . . . . . . . . . . . . . . . . 2.2.5 Stress Intensity Factors . . . . . . . . . . . . . . . . . . . 2.3 Stress History . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.3.1 General . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.3.2 Cycle Counting Methods . . . . . . . . . . . . . . . . . . 2.3.3 Cumulative Frequency Diagram (Stress Spectrum) . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 11 11 11 12 12 12 12 15 18 27 30 34 34 35 36 ........ ........ ........ 37 37 38 ........ ........ ........ 60 60 60 3 Fatigue Resistance . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3.1 Basic Principles . . . . . . . . . . . . . . . . . . . . . . . . . . . 3.2 Fatigue Resistance of Classiﬁed Structural Details . . . . 3.3 Fatigue Resistance Assessed on the Basis of Structural Hot Spot Stress . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3.3.1 Fatigue Resistance Using Reference S-N Curve 3.3.2 Fatigue Resistance Using a Reference Detail . . . . . . . . . . ix x Contents 3.4 3.5 3.6 Fatigue Resistance Assessed on the Basis of the Effective Notch Stress . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3.4.1 Steel . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3.4.2 Aluminium. . . . . . . . . . . . . . . . . . . . . . . . . . . . Fatigue Strength Modiﬁcations . . . . . . . . . . . . . . . . . . . 3.5.1 Stress Ratio . . . . . . . . . . . . . . . . . . . . . . . . . . . 3.5.2 Wall Thickness. . . . . . . . . . . . . . . . . . . . . . . . . 3.5.3 Improvement Techniques . . . . . . . . . . . . . . . . . . 3.5.4 Effect of Elevated Temperatures . . . . . . . . . . . . . 3.5.5 Effect of Corrosion . . . . . . . . . . . . . . . . . . . . . . Fatigue Resistance Assessed on the Basis of Crack Propagation Analysis . . . . . . . . . . . . . . . . . . . . . . . . . . 3.6.1 Steel . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3.6.2 Aluminium. . . . . . . . . . . . . . . . . . . . . . . . . . . . 3.6.3 Correlation of Fracture Mechanics to Other Veriﬁcation Methods . . . . . . . . . . . . . . . . . . . . . Fatigue Resistance Determination by Testing . . . . . . . . . 3.7.1 General Considerations . . . . . . . . . . . . . . . . . . . 3.7.2 Evaluation of Test Data . . . . . . . . . . . . . . . . . . . 3.7.3 Evaluation of Data Collections . . . . . . . . . . . . . . Fatigue Resistance of Joints with Weld Imperfections . . . 3.8.1 General . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3.8.2 Misalignment . . . . . . . . . . . . . . . . . . . . . . . . . . 3.8.3 Undercut . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3.8.4 Porosity and Inclusions . . . . . . . . . . . . . . . . . . . 3.8.5 Crack-like Imperfections . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 62 62 62 63 63 64 66 71 72 ...... ...... ...... 73 73 74 . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 74 75 75 76 77 79 79 80 82 83 84 4 Fatigue Assessment. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 4.1 General Principles . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 4.2 Combination of Normal and Shear Stress . . . . . . . . . . . . . . 4.3 Fatigue Assessment Using S-N Curves. . . . . . . . . . . . . . . . 4.3.1 Linear Damage Calculation by the “Palmgren-Miner” Rule . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 4.3.2 Nonlinear Damage Calculation . . . . . . . . . . . . . . . . 4.4 Fatigue Assessment by Crack Propagation Calculation . . . . . 4.5 Fatigue Assessment on the Basis of Service Testing . . . . . . 4.5.1 General . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 4.5.2 Acceptance Criteria . . . . . . . . . . . . . . . . . . . . . . . . 4.5.3 Safe Life Assessment . . . . . . . . . . . . . . . . . . . . . . 4.5.4 Fail Safe Assessment. . . . . . . . . . . . . . . . . . . . . . . 4.5.5 Damage Tolerant Assessment . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 91 91 91 92 . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 96 99 100 102 102 103 104 104 105 3.7 3.8 Contents 5 Safety Considerations . . . . . . . . . . . . 5.1 Basic Principles . . . . . . . . . . . . 5.2 Fatigue Design Strategies . . . . . . 5.2.1 Inﬁnite Life Design . . . . . 5.2.2 Safe Life Design. . . . . . . 5.2.3 Fail Safe Design . . . . . . . 5.2.4 Damage Tolerant Design . 5.3 Partial Safety Factors . . . . . . . . . 5.4 Quality Assurance . . . . . . . . . . . 5.5 Repair of Components . . . . . . . . xi . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 107 107 108 108 108 108 108 109 110 110 6 Appendices. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 6.1 Loading History . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 6.1.1 Markov Transition Matrix . . . . . . . . . . . . . . . . . . 6.1.2 ‘Rainﬂow’ or ‘Reservoir’ Counting Method . . . . . . 6.2 Fracture Mechanics . . . . . . . . . . . . . . . . . . . . . . . . . . . . 6.2.1 Rapid Calculation of Stress Intensity Factors . . . . . 6.2.2 Dimensions of Cracks . . . . . . . . . . . . . . . . . . . . . 6.2.3 Interaction of Cracks . . . . . . . . . . . . . . . . . . . . . . 6.2.4 Formulae for Stress Intensity Factors. . . . . . . . . . . 6.2.5 Stress Distribution at a Weld Toe . . . . . . . . . . . . . 6.3 Formulae for Misalignment. . . . . . . . . . . . . . . . . . . . . . . 6.4 Statistical Considerations on Safety . . . . . . . . . . . . . . . . . 6.4.1 Statistical Evaluation of Fatigue Test Data . . . . . . . 6.4.2 Statistical Evaluation of Results from Component Testing . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 6.4.3 Statistical Considerations for Partial Safety Factors . 6.5 Fatigue Resistance of ISO 5817 Quality . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 113 113 113 113 115 115 115 116 117 126 127 129 129 . . . . . 130 . . . . . 132 . . . . . 133 References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 139 Contributors List The document contains contributions from: Prof. Dr. A.F. Hobbacher, Jade University of Applied Sciences Wilhelmshaven, Germany, as Chairman Prof. Dr. W. Fricke, Hamburg University of Technology (TUHH), Germany Prof. P.J. Haagensen, Institute of Technology, Trondheim, Norway Prof. Dr. A.F. Hobbacher, University of Applied Sciences, Wilhelmshaven, Germany Dr. M. Huther, Bureau Veritas, Paris France Prof. Dr. K. Iida, Institute of Technology, Shibaura, Japan Dr. H.P. Lieurade, CETIM, Senlis, France Dr. I. Lotsberg, DNV, Oslo, Norway Prof. S.J. Maddox, The Welding Institute, Cambridge, UK Prof. Dr. G. Marquis, Lappeenranta University of Technology, Finland Prof. Dr. Ch. Miki, Institute of Technology, Tokyo, Japan Prof. Erkki Niemi, Lappeenranta University of Technology, Finland Dr. A. Ohta, NRIM, Tokyo, Japan Mr. O. Ørjasæter, SINTEF, Trondheim, Norway Prof. Dr. H.J. Petershagen, Hamburg University of Technology (TUHH), Germany Prof. Dr. C.M. Sonsino, LBF Darmstadt, Germany Suggestions for a future reﬁnement of the document are welcome and should be addressed to the chairman: Prof. Dr. A.F. Hobbacher, Jade University of Applied Sciences, Friedrich-PaffrathStr. 101, D-26389 Wilhelmshaven, Germany, e-mail: hobbacher@t-online.de xiii Chapter 1 General The IIW, and every other body or person involved in the preparation and publication of this document, hereby expressly disclaim any liability or responsibility for loss or damage resulting from its use, for any violation of any mandatory regulation with which the document may conflict, or for the infringement of any patent resulting from the use of this document. It is the user’s responsibility to ensure that the recommendations given here are suitable for his/her intended purposes. 1.1 Introduction The aim of these recommendations is to provide a basis for the design and analysis of welded components loaded by fluctuating forces, to avoid failure by fatigue. In addition they may assist other bodies who are establishing fatigue design codes. It is assumed that the user has a working knowledge of the basics of fatigue and fracture mechanics [3–8]. The purpose of designing a structure against the limit state due to fatigue damage is to ensure that the performance is satisfactory during the design life with an adequate survival probability. The required survival probability is obtained by the use of appropriate partial safety factors. 1.2 Scope and Limitations The recommendations present general methods for the assessment of fatigue damage in welded components, which may affect the limit states of a structure, such as the ultimate and serviceability limit states [1]. The recommendations give fatigue resistance data for welded components made of wrought or extruded products of ferritic/pearlitic or bainitic structural steels up to fy = 960 MPa, of austenitic stainless steels and of aluminium alloys commonly used for welded structures. © Springer International Publishing Switzerland 2016 A.F. Hobbacher, Recommendations for Fatigue Design of Welded Joints and Components, IIW Collection, DOI 10.1007/978-3-319-23757-2_1 1 2 1 General The recommendations are not applicable to low cycle fatigue, where Δσnom > 1.5 · fy or maxσnom > fy, for corrosive conditions or for elevated temperature operation in the creep range. 1.3 Deﬁnitions Characteristic value Loads, forces or stresses, which vary statistically, at a speciﬁed fractile, here: 95 % survival probability referred to a two-sided conﬁdence level of the mean of 75 %, for details see Sect. 3.7 Classiﬁed or standard A structural detail containing a structural discontinuity structural detail including a weld or welds, for which the nominal stress approach is applicable, and which appear in the tables of these fatigue design recommendations. Also referred to as standard structural detail Concentrated load effect (i) A local stress ﬁeld in the vicinity of a point load or reaction force, (ii) membrane and shell bending stresses due to loads causing distortion of a cross section not sufﬁciently stiffened by a diaphragm Constant amplitude loading Crack propagation rate Crack propagation threshold Cut off limit Cycle counting Design value Effective notch stress Equivalent stress range A type of loading causing a regular stress fluctuation between constant maximum and minimum stress limits Amount of crack extension per stress cycle Limiting value of stress intensity factor range below which crack propagation can be considered as negligible Fatigue strength under variable amplitude loading, below which the stress cycles are considered to be non-damaging Procedure of converting the history of variable amplitude loading into an equivalent spectrum or transition matrix (e.g. ‘Rainflow’ or ‘Reservior’ methods) Characteristic value factored by a partial safety factor Notch stress calculated for a notch with a certain assumed notch radius Constant amplitude stress range which is equivalent in terms of fatigue damage to a variable stress history for the same number of applied stress cycles 1.3 Deﬁnitions Fatigue Fatigue action Fatigue damage ratio Fatigue life Fatigue limit Fatigue resistance Fatigue strength Fracture mechanics Hot spot Local or modiﬁed nominal stress Local notch Macro-geometric discontinuity Macro-geometric effect Membrane stress Miner sum Misalignment 3 Deterioration of a component caused by the crack initiation and/or by the growth of a crack Load effect causing fatigue, i.e. fluctuating load Ratio of fatigue damage sustained to fatigue damage required to cause failure, deﬁned as the ratio of the number of applied stress cycles and the corresponding fatigue life at constant amplitude loading Number of stress cycles of a particular magnitude required to cause fatigue failure of the component Fatigue strength under constant amplitude loading corresponding to a high number of cycles large enough to be considered as inﬁnite Structural detail’s resistance to fatigue actions expressed in terms of a S-N curve or crack propagation properties Magnitude of stress range leading to a particular fatigue life A branch of mechanics dealing with the behaviour and strength of components containing cracks A point in a structure where a fatigue crack may initiate due to the combined effect of structural stress fluctuation and the weld geometry or a similar notch Nominal stress including macro-geometric effects, concentrated load effects and misalignments, disregarding the stress raising effects of the welded joint itself A localised geometric feature, such as the toe of a weld, that causes stress concentration. The local notch does not alter the structural stress but generates a nonlinear stress peak A global discontinuity, the effect of which is usually not taken into account in the collection of standard structural details, such as a large opening, a curved part in a beam, a bend in a flange not supported by diaphragms or stiffeners, discontinuities in pressure containing shells, eccentricity in a lap joint (see Fig. 2.3) A stress raising effect due to macro-geometry in the vicinity of the welded joint, but not due to the welded joint itself Average normal stress across the thickness of a plate or shell Summation of individual fatigue damage ratios caused by each stress cycle or stress range block above a certain cut-off limit according to the Palmgren-Miner rule Axial and angular misalignments caused either by detail design or by poor fabrication or welding distortion 4 1 General Modiﬁed nominal stress See ‘Local nominal stress’ Nominal stress A stress in a component, resolved using general theories, e.g. beam theory. See also local nominal stress Nonlinear stress peak The stress component of a notch stress which exceeds the linearly distributed structural stress at a local notch Notch stress Total stress at the root of a notch taking into account the stress concentration caused by the local notch, consisting of the sum of structural stress and nonlinear stress peak Notch stress concentra- The ratio of notch stress to structural stress tion factor Paris-Erdogan law An experimentally determined relation between fatigue crack growth rate and stress intensity factor range Palmgren-Miner rule Method for estimating fatigue life under variable amplitude loading from the constant amplitude S-N curve (see Sect. 4.3.1). Often referred to as Miner’s rule Range counting A procedure of determining various stress cycles and their ranges from a stress history, preferably by rainflow counting method Shell bending stress Bending stress in a shell or plate-like part of a component, linearly distributed across the thickness as assumed in the theory of shells S-N curve Graph of the dependence of fatigue life N on applied stress range S (ΔσR or ΔτR), also known as Wöhler curve Stress cycle A part of a stress history containing a stress maximum and a stress minimum, usually determined by cycle counting Stress history A time-based presentation of a fluctuating stress, deﬁned by sequential stress peaks and troughs (valleys), either for the total life or for a certain period of time Stress intensity factor The fracture mechanics parameter, which is a function of applied stress, crack size and geometry Stress range The difference between the maximum and minimum stresses in a cycle Stress range block A part of the total spectrum of stress ranges which is discretized in a certain number of blocks Stress spectrum A tabular or graphical presentation of the cumulative frequency of stress range exceedence (e.g. the number of stress ranges exceeding a particular magnitude of stress range in a stress history, where frequency is the number of occurrences) Stress ratio Ratio of minimum to maximum algebraic value of the stress in a particular stress cycle Stress intensity factor Ratio of minimum to maximum algebraic value of the ratio stress intensity factor of a particular load cycle 1.3 Deﬁnitions 5 Structural discontinuity A geometric discontinuity due to the type of welded joint, usually to be found in the tables of classiﬁed structural details. The effects of a structural discontinuity are (i) concentration of the membrane stress and (ii) formation of secondary shell bending stresses (see Fig. 2.6) Structural or geometric A stress in a component, resolved to take into account stress the effects of a structural discontinuity, and consisting of membrane and shell bending stress components Structural stress concen- The ratio of structural stress to local or modiﬁed nominal tration factor stress Structural hot spot The value of structural stress on the surface at a hot spot stress Variable amplitude A type of loading causing irregular stress fluctuation with loading stress ranges (and amplitudes) of variable magnitude 1.4 Symbols Cross sectional area of loaded plate (a sufﬁx may be added) or weld throat size B Plate width C Constant in equation of S-N curve with exponent m CV Comparison value used in veriﬁcation procedure for assessing combined loading D Fatigue damage sum according to the Palmgren-Miner rule or mean diameter Dmax Maximum diameter Dmin Minimum diameter E Elastic modulus F Force or statistical safety factor FATx Classiﬁcation reference to S-N curve, in which x is the stress range in MPa at 2 × 106 cycles H Fillet weld leg length K Stress intensity factor Kmax Stress intensity factor caused by σmax Kmin Stress intensity factor caused by σmin L Attachment length in direction of loading considered M Bending moment Mk Magniﬁcation function for K due to nonlinear stress peak Mk,m Magniﬁcation function for K, concerning membrane stresses Mk,b Magniﬁcation function for K, concerning shell bending stresses N Fatigue life in cycles A 6 Ni R Stdv W Y Ym Yb a ao af b c d e fy km ks kt m n ni t ΔK ΔKS,d ΔKth Δσ ΔσS,d ΔσR,L Δτ γM ΓM σ σb σen σln σmax σm σmin σnl σnom σhs 1 General Constant amplitude fatigue life at the i-th stress range Stress ratio Standard deviation of logN Fillet weld leg length (see Table 6.4) Correction function for K, taking into account crack form, aspect ratio, relative crack size etc. Correction function for K, concerning membrane stress Correction function for K, concerning shell bending stress Weld throat size or depth of a surface crack or semi length of an embedded crack Initial depth of a surface crack Value of a at fatigue failure Distance between crack centre and nearest plate edge Half length of surface or embedded elliptical crack Deviation from the true circle due to angular misalignment Eccentricity, amount of offset misalignment Actual or speciﬁed yield strength of the material Stress magniﬁcation factor due to misalignment Stress concentration factor due to structural discontinuity Stress concentration factor due to local notch Exponent of S-N curve or Paris power law Exponent in thickness correction or number of data pairs Number of applied stress cycles at the i-th stress range Plate thickness, thickness parameter (crack centre to nearest surface) Stress intensity factor range Design value of stress intensity factor range caused by actions Threshold stress intensity factor range Stress range Design value of stress range caused by actions Characteristic value of stress range at knee point of S-N curve Shear stress range Partial safety factor for fatigue resistance in terms of stress Partial safety factor for fatigue resistance in terms of cycles Normal stress Shell bending stress Effective notch stress (Local) notch stress Stress maximum in stress history Membrane stress Stress minimum in stress history Nonlinear stress peak (Modiﬁed) nominal stress Structural hot spot stress 1.4 Symbols S R d k τ 7 Subscripts: Fatigue actions Fatigue resistance Design value Characteristic value Shear stress 1.5 Basic Principles According to the ISO format for veriﬁcation of structures [1], fatigue action and fatigue resistance are clearly separated. The main fatigue resistance data provided in this document are in the form of S-N or fatigue crack growth curves, based on constant amplitude test results. No speciﬁc recommendations are given for the fatigue load (action) side, or for the partial safety factors on fatigue resistance γM or actions γF. The different approaches for the fatigue assessment of welded joints and components considered are: nominal stress, structural hot-spot stress, effective notch stress, fracture mechanics and component testing. 1.6 Necessity of Fatigue Assessment Fatigue assessment is generally required for components subject to fluctuating loads. In the following cases, detailed fatigue assessment is not usually required. If there is any doubt that these criteria apply, a fatigue assessment is recommended: (a) The highest nominal design stress range satisﬁes Steel : DrS;d 36 MPa=cM Aluminium : DrS;d 12 MPa=cM ð1:1Þ ð1:2Þ γM should be taken from an applicable design code. This paragraph is not applicable to tubular joints. (b) The Miner sum D (Sect. 4.3.1) is less than or equal to D = 0.5 when evaluated using either fatigue class FAT 36 for steel or FAT 12 for aluminium (c) For a detail for which a constant amplitude fatigue limit ΔσR,L is speciﬁed and all design stress ranges are under an assumed or speciﬁed design resistance fatigue limit (Sect. 3.2) 8 1 General DrS;d DrR;L cM ð1:3Þ (d) For a crack, at which all design stress intensity factors are under an assumed or speciﬁed crack propagation threshold level ΔKth. DKS;d DKth =cM for steel ΔKth = 2.0 MPa√m = 63 N·mm−3/2 for aluminium ΔKth = 0.7 MPa√m = 21 N·mm−3/2 1.7 ð1:4Þ Application of the Document Various assessment procedures are presented of which the choice is depending on the initial information about the welded joint and the applied loading. Then, the fatigue action data (e.g. stress type) and the fatigue resistance data are determined according to the assessment procedure. The corresponding types of fatigue action and resistance are summarized in Tables 1.1 and 1.2. The chosen procedure may need to be performed using appropriate safety factors. Table 1.1 Presentation of fatigue actions and resistances versus assessment procedure Fatigue action Fatigue resistance Assessment procedure Forces on component Nominal stress in section Structural hot-spot stress at weld toe Effective notch stress in weld notch Stress intensity at crack tip Resistance determined by test of component Component testing Summation of cumulative damage Resistance given by tables of structural details in terms of a set of S-N curves Resistance against structural hot-spot stress in terms of S-N curves Resistance against effective notch stress in terms of a universal S-N curve Resistance against crack propagation in terms of the material parameters of the crack propagation law Summation of crack increments Table 1.2 General guidance for the application of the document 1.7 Application of the Document 9 Chapter 2 Fatigue Actions (Loading) All types of fluctuating load acting on the component and the resulting stresses at potential sites for fatigue have to be considered. Stresses or stress intensity factors then have to be determined according to the fatigue assessment procedure applied. The actions originate from live loads, dead weights, snow, wind, waves, pressure, accelerations, dynamic response etc. Actions due to transient temperature changes should also be considered. Improper knowledge of fatigue actions is one of the major sources of fatigue damage. Tensile residual stresses due to welding and other manufacturing processes decrease the fatigue resistance. However, the influence of high tensile residual stresses is already included in the fatigue resistance data given in Chap. 3. 2.1 2.1.1 Basic Principles Determination of Fatigue Actions (Loading) In assessing fatigue performance, a safe estimate of fatigue loading to be endured throughout the life of the structure or component under consideration is crucial. All types of varying loading should be considered. Fluctuating loading from different sources may be signiﬁcant at different phases of the life, e.g. construction, transportation, installation, in-service, and may involve different frequencies. The design load spectrum should be selected on the basis that it is an upper bound estimate of the accumulated service conditions over the full design life of the structure or component concerned. If relevant, this may be based on characteristic load data and partial safety factors γF speciﬁed in the application code giving design values for the fatigue loading. No guidance is given in this document for the establishing of design values for actions (loads), nor for partial safety factors γF on actions (loads). © Springer International Publishing Switzerland 2016 A.F. Hobbacher, Recommendations for Fatigue Design of Welded Joints and Components, IIW Collection, DOI 10.1007/978-3-319-23757-2_2 11 12 2 Fatigue Actions (Loading) 2.1.2 Stress Range Fatigue assessment is usually based on stress range or stress intensity factor range. Thus, the fatigue loading (actions) needs to be expressed in these terms. Dr ¼ rmax rmin ð2:1Þ DK ¼ Kmax Kmin ð2:2Þ The maximum and minimum stresses should be calculated from the superposition of all non permanent, i.e. fluctuating loads: (a) (b) (c) (d) (e) Fluctuations in the magnitudes of loads Movement of loads on the structure Changes in loading directions Structural vibrations due to loads and dynamic response Temperature transients Fatigue analysis is based on the cumulative effect of all stress range occurrences during the anticipated service life of the structure. 2.1.3 Types of Stress Concentrations and Notch Effects The stress required to assess the fatigue resistance of a particular stress concentration feature depends on the type and the fatigue assessment procedure used, see Table 2.1. Figure 2.1 shows an example of different stress deﬁnitions, such as gross nominal stress and modiﬁed or local nominal stress. Figure 2.2 shows the increase in stress in the vicinity of the notch, caused by the structural detail and the weld toe. 2.2 2.2.1 Determination of Stresses and Stress Intensity Factors Deﬁnition of Stress Components In the vicinity of a notch the stress distribution over the plate thickness is non-linear (Fig. 2.3). The stress components of the notch stress σnl are [2]: σm membrane stress σb shell bending stress σnl non-linear stress peak 2.2 Determination of Stresses and Stress Intensity Factors 13 Table 2.1 Stress concentrations and notch effects considered Type Stress concentrations Stress determined Assessment procedure A None B Macro-geometrical effects due to the design of the component, but excluding stress concentrations due to the welded joint itself. B + structural discontinuities due to the structural detail of the welded joint, but excluding the notch effect of the weld toe transition A + B + C + notch stress concentration due to the weld bead notches (a) actual notch stress (b) effective notch stress Gross average stress from sectional forces, calculated using general theories, e.g. beam theory Range of nominal stress (also modiﬁed or local nominal stress) Not applicable for fatigue analysis of joints, only for component testing Nominal stress approach Range of structural hot-spot stress Structural hot-spot stress approach Range of elastic notch stress (total stress) (a) Fracture mechanics approach (b) Effective notch stress approach C D Fig. 2.1 Modiﬁed or local nominal stress If a reﬁned stress analysis method is used, which gives a non-linear stress distribution, the stress components can be separated by the following method: The membrane stress σm is equal to the average stress calculated through the thickness of the plate. It is constant through the thickness. The shell bending stress σb is linearly distributed through the thickness of the plate. It is found by drawing a straight line through the point O in Fig. 2.3 where the membrane stress intersects the mid-plane of the plate. The gradient of the shell bending stress is chosen such that the remaining non-linearly distributed component is in equilibrium. 14 2 Fatigue Actions (Loading) Fig. 2.2 Notch stress and structural hot-spot stress The non-linear stress peak σnl is the remaining component of the stress. The stress components can be separated analytically for a given through thickness stress distribution σ(x) from x = 0 at the surface to x = t: 1 rm ¼ t Zx¼t rðxÞ dx ð2:3Þ t ðrðxÞ rm Þ ð xÞ dx 2 ð2:4Þ x¼0 6 rb ¼ 2 t Zx¼t x¼0 rnl ðxÞ ¼ rðxÞ rm ð1 2x Þ rb t ð2:5Þ Note: In Fig. 2.3 and at formulae (2.3)–(2.5) a linear distribution of bending stress according to the Bernoulli theory of beams was assumed. Prior to an application of the formulae, that condition should be checked. Fig. 2.3 Non-linear stress distribution separated to stress components 2.2 Determination of Stresses and Stress Intensity Factors 2.2.2 Nominal Stress 2.2.2.1 General 15 Nominal stress is the stress calculated in the sectional area under consideration, disregarding the local stress raising effects of the welded joint, but including the stress raising effects of the macro-geometric shape of the component in the vicinity of the joint, such as e.g. large cutouts. Overall elastic behaviour is assumed. The nominal stress may vary over the section under consideration. For example at a beam-like component, the modiﬁed (also local) nominal stress and the variation over the section can be calculated using simple beam theory. Here, the effect of a welded on attachment is ignored (Fig. 2.4). The effects of macro-geometric features of the component and stress ﬁelds in the vicinity of concentrated loads must be included in the nominal stress. Both may cause signiﬁcant redistribution of the membrane stresses across the section. Signiﬁcant shell bending stress may also be generated, as in curling of a flange, or distortion of a box section (Figs. 2.5, 2.6a, b). The secondary bending stress caused by axial or angular misalignment (e.g. as considered to be acceptable in the fabrication speciﬁcation) needs to be considered if the misalignment exceeds the amount which is already covered by the fatigue Fig. 2.4 Nominal stress in a beam-like component (a) (b) (c) (d) (e) (f) Fig. 2.5 Examples of macrogeometric effects. Stress concentrations at a cut-outs, b curved beams, c wide plates, d curved flanges, e concentrated loads, f excentricities 16 2 Fatigue Actions (Loading) resistance S-N curve for the structural detail. This is done by the application of an additional stress magniﬁcation factor km,eff (see Sect. 3.8.2). Either the applied stress is multiplied by km,eff or the fatigue resistance (stress) is divided by it. 2.2.2.2 Calculation of Nominal Stress In simple components the nominal stress can be determined using elementary theories of structural mechanics based on linear-elastic behaviour. Nominal stress is the average stress in the weld throat or in the plate at the weld toe as indicated in the tables of structural details. A possible misalignment shall be considered either in analysis or in resistance data (Fig. 2.7a) The weld throat is determined at (Fig. 2.7b) Butt welds Wall thickness of the plates, at dissimilar wall thicknesses, the smaller wall thickness has to be taken Fillet welds The smallest distance from the root or deepest point of penetration to the surface of the ﬁllet weld bead The stress σw or τw in weld throat a for a weld of length lw and a force in the weld F becomes F F rw or sw ¼ ¼ ð2:6Þ Aw a lw Fig. 2.6 a Modiﬁed (local) nominal stress near concentrated loads. b Modiﬁed (local) nominal stress at hard spots 2.2 Determination of Stresses and Stress Intensity Factors 17 Fig. 2.7 a Axial and angular misalignment. b Weld throat In other cases, ﬁnite element method (FEM) modelling may be used. This is primarily the case in (a) complex statically over-determined (hyperstatic) structures (b) structural components incorporating macro-geometric discontinuities, for which no analytical solutions are available If the ﬁnite element method is used, meshing can be simple and coarse. Care must be taken to ensure that all stress concentration effects from the structural detail of the welded joint are excluded when calculating the modiﬁed (local) nominal stress. If nominal stresses are calculated for ﬁllet welds by coarse ﬁnite element meshes, nodal forces rather than element stresses should be used in a section through the weld in order to avoid stress underestimation. When a nominal stress is intended to be calculated by ﬁnite elements, the more precise option of the structural hot spot stress determination should be considered. 2.2.2.3 Measurement of Nominal Stress The fatigue resistance S-N curves of classiﬁed structural details are based on nominal stress, disregarding the stress concentrations due to the welded joint. Therefore the measured nominal stress must exclude the stress or strain concentration due to the corresponding discontinuity in the structural component. Thus, strain gauges must be placed outside the stress concentration ﬁeld of the welded joint. In practice, it may be necessary ﬁrst to evaluate the extent and the stress gradient of the ﬁeld of stress concentration (see Sect. 2.2.3.4) due to the welded joint. For further measurements, simple strain gauge application outside this ﬁeld is sufﬁcient. 18 2 Fatigue Actions (Loading) When a nominal stress is intended to be measured by strain gauges, the more precise option of the structural hot spot stress measurement should be considered. 2.2.3 Structural Hot Spot Stress 2.2.3.1 General The structural or geometric stress σhs at the hot spot includes all stress raising effects of a structural detail excluding that due to the local weld proﬁle itself. So, the non-linear peak stress σnl caused by the local notch, i.e. the weld toe, is excluded from the structural stress. The structural stress is dependent on the global dimensional and loading parameters of the component in the vicinity of the joint (type C in Sect. 2.1.3 Table 2.1). It is determined on the surface at the hot spot of the component which is to be assessed. Structural hot spot stresses σhs are generally deﬁned for plate, shell and tubular structures. Figure 2.8 shows examples of structural discontinuities and details together with the structural stress distribution. The structural hot spot stress approach is typically used where there is no clearly deﬁned nominal stress due to complex geometric effects, or where the structural discontinuity is not comparable to a classiﬁed structural detail [9, 11–13]. The structural hot-spot stress can be determined using reference points by extrapolation to the weld toe under consideration from stresses at reference points (a) (b) (c) (d) (e) Fig. 2.8 Structural details and structural stress, e.g. at a end of longitudinal lateral attachment, b joint of plates with unequal width, c end of cover plate, d end of longitudinal attachment, e joint with unequal thickness 2.2 Determination of Stresses and Stress Intensity Factors 19 computed total stress reference points structural stress stress on surface F F hot spot Fig. 2.9 Deﬁnition of structural hot-spot stress (Fig. 2.9). Strictly speaking, the method as deﬁned here is limited to the assessment of the weld toe, i.e. cases a to e in Fig. 2.10. However, the approach may be extended to the assessment of other potential fatigue crack initiation sites including the weld root, by using the structural hot spot stress on the surface as an indication of that in the region of interest. The S-N curves or the stress concentration factors used for veriﬁcation in such cases depend largely on the geometric and dimensional parameters and are only valid in the range of these parameters. In the case of a biaxial stress state at the plate surface, it is recommended that the principal stress which acts approximately in line with the perpendicular to the weld toe, i.e. within ±60° (Fig. 2.11) is used. The other principal stress may need to be analysed, if necessary, using the fatigue class in the nominal stress approach for welds parallel to the stress. Fig. 2.10 Various locations of crack propagation in welded joints. a–e with weld toe cracks, f–j with weld root cracks 20 2 Fatigue Actions (Loading) Fig. 2.11 Biaxial stresses at weld toe, principle stress within (a) and without (b) an angle of 60° perpendicular to the weld 2.2.3.2 Types of Hot Spots Besides the deﬁnitions of structural hot spot stress as given above, two types of hot spots are deﬁned according to their location on the plate and their orientation in respect to the weld toe as deﬁned in Fig. 2.12, Table 2.2: The structural stress acts normal to the weld toe in each case and is determined either by a special FEA procedure or by extrapolation from measured stresses. Fig. 2.12 Types of hot spots Type Table 2.2 : Types of hot spots Type Description Determination a b Weld toe on plate surface Weld toe at plate edge FEA or measurement and extrapolation FEA or measurement and extrapolation 2.2 Determination of Stresses and Stress Intensity Factors 2.2.3.3 21 Determination of Structural Hot Spot Stress The structural hot spot stress can be determined either by measurement or by calculation. Here the non-linear peak stress is eliminated by linearization of the stress through the plate thickness (see Sect. 2.2.1) or by extrapolation of the stress at the surface to the weld toe. The following considerations focus on surface stress extrapolation procedures of the surface stress, which are essentially the same for both measurement and calculation. The procedure is ﬁrst to establish the reference points and then to determine the structural hot spot stress by extrapolation to the weld toe from the stresses of those reference points. Depending on the method, there may be two or three reference points. The reference point closest to the weld toe must be chosen to avoid any influence of the notch due to the weld itself (which leads to a non-linear stress peak). This is practically the case at a distance of 0.4 t from the weld toe, where t is plate thickness. The structural hot spot stress at the weld toe is then obtained by extrapolation. Identiﬁcation of the critical points (hot spots) can be made by: (a) Measuring several different points (b) Analysing the results of a prior FEM analysis (c) Experience of existing components, especially if they failed 2.2.3.4 Calculation of Structural Hot Spot Stress In general, analysis of structural discontinuities and details to obtain the structural hot spot stress is not possible using analytical methods. Parametric formulae are rarely available. Thus, ﬁnite element analysis (FEA) is generally applied. Usually, structural hot spot stress is calculated on the basis of an idealized, perfectly aligned welded joint. Consequently, any possible misalignment has to be taken explicitly into consideration explicitly in the FEA model or by applying an appropriate stress magniﬁcation factor km, see also Sect. 3.8.2. This applies particularly to butt welds, cruciform joints and one-sided transverse ﬁllet welded attachments on one side of an unsupported plate. The extent of the ﬁnite element model has to be chosen such that constraining boundary effects of the structural detail analysed are comparable to the actual structure. Models with either thin plate or shell elements or with solid elements may be used. It should be noted that on the one hand the arrangement and the type of the elements must allow for steep stress gradients and for the formation of plate bending, but on the other hand, only the linear stress distribution in the plate thickness direction needs to be evaluated with respect to the deﬁnition of the structural hot spot stress. The stresses should be determined at the speciﬁed reference points. 22 2 Fatigue Actions (Loading) Fig. 2.13 Typical meshes and stress evaluation paths for a welded detail A reasonably high level of expertise is required on the part of the FEA analyst. Guidance is given in [11]. In the following, only some rough recommendations are given: In a plate or shell element model (Fig. 2.13, left part), the elements are arranged in the mid-plane of the structural components. 8-noded elements are recommended particularly in regions of steep stress gradients. In simpliﬁed models, the welds are not modelled, except for cases where the results are affected by local bending, e. g. due to an offset between plates or due to a small distance between adjacent welds. Here, the welds may be included by vertical or inclined plate elements having appropriate stiffness or by introducing constraint equations or rigid links to couple node displacements. Thin-shell elements naturally provide a linear stress distribution through the shell thickness, suppressing the notch stress at weld toes. Nevertheless, the structural hot-spot stress is frequently determined by extrapolation from the reference points mentioned before, particularly at points showing an additional stress singularity such as stiffener ends. Alternatively, particularly for complex cases, prismatic solid elements which have a displacement function allowing steep stress gradients as well as plate bending with linear stress distribution in the plate thickness direction may be used. An example is isoparametric 20-node elements with mid-side nodes at the edges, which allow only one element to be arranged in the plate thickness direction due to the quadratic displacement function and the linear stress distribution. By reduced integration, the linear part of the stresses can be directly evaluated at the shell surface and extrapolated to the weld toe. Modelling of welds is generally recommended as shown in Fig. 2.13 (right part). The alternative with a multi-layer arrangement of solid elements allows to linearize the stresses over the plate thickness directly at the weld toe. Surface Stress Extrapolation Methods: If the structural hot-spot stress is determined by extrapolation, the element lengths are determined by the reference points selected for stress evaluation. In order to avoid an influence of the stress singularity, the stress closest to the hot spot is usually evaluated at the ﬁrst nodal point. Therefore, the length of the element at the hot spot corresponds to its distance from the ﬁrst reference point. If ﬁner meshes are used, the reﬁnement should be introduced in the thickness direction as well. 2.2 Determination of Stresses and Stress Intensity Factors 23 Fig. 2.14 Reference points at different types of meshing. Stress type “a” (a, b), type “b” (c, d) Coarser meshes are also possible with higher-order elements and ﬁxed lengths, as explained further below. Appropriate element widths are important, particularly in cases with steep stress gradients. The width of the solid element or the two shell elements in front of the attachment should not exceed the attachment width ‘w’, i. e. the attachment thickness plus two weld leg lengths as indicated in Fig. 2.13. Typical extrapolation paths for determining the structural hot spot stress components on the plate surface or edge are shown by arrows in Fig. 2.13. If the weld is not modelled, extrapolation to the structural intersection point is recommended in order to avoid stress underestimation due to the missing stiffness of the weld. Type “a” Hot Spots: The structural hot spot stress σhs is determined using the reference points and extrapolation equations as given below (see also Fig. 2.14). (1) Fine mesh with element length not more than 0.4 t at the hot spot: Evaluation of nodal stresses at two reference points 0.4 t and 1.0 t, and linear extrapolation (Eq. 2.7). rhs ¼ 1:67 r0:4t 0:67 r1:0t ð2:7Þ (2) Fine mesh as deﬁned in (1) above: Evaluation of nodal stresses at three reference points 0.4 t, 0.9 t and 1.4 t, and quadratic extrapolation (Eq. 2.8). This method is recommended for cases of pronounced non-linear structural stress increase towards the hot spot, at sharp changes of direction of the applied force or for thick-walled structures. rhs ¼ 2:52 r0:4t 2:24 r0:9t þ 0:72 r1:4t ð2:8Þ 24 2 Fatigue Actions (Loading) (3) Coarse mesh with higher-order elements having lengths equal to plate thickness at the hot spot: Evaluation of stresses at mid-side points or surface centres respectively, i.e. at two reference points 0.5 t and 1.5 t, and linear extrapolation (Eq. 2.9). rhs ¼ 1:50 r0:5t 0:50 r1:5t ð2:9Þ Application of the usual wall thickness correction, as given in Sect. 3.5.2 is required when the structural hot spot stress of type “a” is obtained by surface extrapolation. For circular tubular joints, the wall thickness correction exponent of n = 0.4 is recommended. Type “b” Hot Spots: The stress distribution is not dependent on plate thickness. Therefore, the reference points are given at absolute distances from the weld toe, or from the weld end if the weld does not continue around the end of the attached plate. (4) Fine mesh with element length of not more than 4 mm at the hot spot: Evaluation of nodal stresses at three reference points 4, 8 and 12 mm and quadratic extrapolation (Eq. 2.10). rhs ¼ 3 r4 mm 3 r8 mm þ r12 mm ð2:10Þ (5) Coarse mesh with higher-order elements having length of 10 mm at the hot spot: Evaluation of stresses at the mid-side points of the ﬁrst two elements and linear extrapolation (Eq. 2.11). rhs ¼ 1:5 r5 mm 0:5 r15 mm ð2:11Þ Table 2.3 Recommended meshing and extrapolation (see also Fig. 2.14) Type of model and weld toe Element size Extra-polation points a Relatively coarse models Type a Type b Shells txt max t x w/2a 10 × 10 mm Solids txt max t x w 10 × 10 mm Shells 0.5 t and 1.5 t mid-side pointsb 5 and 15 mm mid-side points Solids 0.5 and 1.5 t surface centre 5 and 15 mm surface centre Relatively ﬁne models Type a Type b ≤0.4 t x t or ≤0.4 t x w/2 ≤0.4 t x t or ≤0.4 t x w/2 0.4 t and 1.0 t nodal points 0.4 t and 1.0 t nodal points ≤4 × 4 mm ≤4 × 4 mm 4, 8 and 12 mm nodal points 4, 8 and 12 mm nodal points w = longitudinal attachment thickness +2 weld leg lengths surface centre at transverse welds, if the weld below the plate is not modelled (see left part of Fig. 2.13) b 2.2 Determination of Stresses and Stress Intensity Factors 25 In the case of type “b” hot spots obtained by surface stress extrapolation, the wall thickness correction (see Sect. 3.5.2) is applied with an exponent of n = 0.1 (Table 2.3). Alternative Methods: Alternative methods of estimation the structural hot spot stress may be useful in special cases. However, care is needed to ensure that they are compatible with the fatigue design resistance data recommended in this document. In the method after Haibach [15], the stress on the surface 2 mm away from the weld toe is determined. In the method after Xiao and Yamada [16], the stress 1 mm below the weld toe on the anticipated crack path is taken. Both methods are useful at sharp changes in the direction of the applied force or at thick-walled structures. In both methods no correction is required for wall thickness. The results from FEA can also be evaluated using nodal forces or through thickness integration to estimate the structural hot spot stress. A further alternative procedure after Dong and Hong [12] uses a special stress parameter based partly on structural hot spot stress and partly on fracture mechanics analysis, with a consideration of wall thickness and stress gradient. 2.2.3.5 Measurement of Structural Hot Spot Stress The recommended placement and number of strain gauges depends on the extent of shell bending stresses, the wall thickness and the type of structural stress. The centre point of the ﬁrst gauge, whose gauge length should not exceed 0.2 t, is located at a distance of 0.4 t from the weld toe. If this is not possible for example due to a small plate thickness, the leading edge of the gauge should be placed at a distance of 0.3 t from the weld toe. The following extrapolation procedure and number of gauges are recommended (Fig. 2.15): Type “a” Hot Spots: (a) Two gauges at reference points 0.4 t and 1.0 t and linear extrapolation (Eq. 2.12). 0.4t 0.6t t t 0.4t 0.5t 0.5t <1.5t Fig. 2.15 Examples of strain gauges in plate structures t 0.3t 26 2 Fatigue Actions (Loading) ehs ¼ 1:67 e0:4t 0:67 e1:0t ð2:12Þ (b) Three gauges at reference points 0.4 t, 0.9 t and 1.4 t, and quadratic extrapolation. This method is particularly suitable for cases of pronounced non-linear structural stress increase towards the hot spot (Eq. 2.13). ehs ¼ 2:52 e0:4t 2:24 e0:9t þ 0:72 e1:4t ð2:13Þ Precise positioning is not necessary if multi-grid strip gauges are used, since the results can be used to plot the stress distribution approaching the weld toe. The stresses at the required positions can then be read from the ﬁtted curve. Type “b” Hot Spots: Three gauges are attached to the plate edge at reference points 4, 8 and 12 mm distant from the weld toe. The hot spot strain is determined by quadratic extrapolation to the weld toe (Eq. 2.14): ehs ¼ 3 e4mm 3 e8 mm þ e12 mm ð2:14Þ Determination of Stress: If the stress state is close to uniaxial, the approximation to the structural hot spot stress is obtained approximately from Eq. (2.15). rhs ¼ E ehs ð2:15Þ For biaxial stress states, the actual stress may be up to 10 % higher than that obtained from Eq. (2.15). In this case, use of rosette strain gauges is recommended. If the ratio of longitudinal to transversal strains εy/εx is available, for example from FEA, the structural hot spot stress σhs can then be resolved from Eq. (2.16), assuming that this principal stress is approximately perpendicular to the weld toe. ey ex rhs ¼ E ex 1 m2 1þm ð2:16Þ The above equations also apply if strain ranges are measured, producing the range of structural hot spot stress Δσhs. 2.2.3.6 Tubular Joints Special recommendations exist for determining the structural hot spot stress in tubular joints [14]. In general these allow the use of linear extrapolation from the measured or calculated stresses at two reference points. The measurement of simple uni-axial stress is sufﬁcient. 2.2 Determination of Stresses and Stress Intensity Factors 27 Parametric formulae have been established for the stress concentration factor khs in many joints between circular and rectangular section tubes, see Ref. [14]. Hence the structural hot spot stress σhs becomes: rhs ¼ khs rnom ð2:17Þ where σnom is the nominal axial membrane or bending stress in the braces, calculated by elementary stress analysis or uni-axial measurement. 2.2.4 Effective Notch Stress 2.2.4.1 General Effective notch stress is the total stress at the root of a notch, obtained assuming linear-elastic material behaviour. To take account of the variation of the weld shape parameters, as well as of the non-linear material behaviour at the notch root, the actual weld contour is replaced by an effective one (Fig. 2.16). For structural steels and aluminium alloys an effective notch root radius of r = 1 mm has been veriﬁed to give consistent results. For fatigue assessment, the effective notch stress is compared with a single fatigue resistance curve, although, as with other assessment methods, it is necessary to check that the fatigue resistance curve for parent metal is not exceeded in the direct vicinity of the weld [17–21]. The method is restricted to the assessment of welded joints with respect to potential fatigue failures from the weld toe or weld root (Fig. 2.17). The fatigue assessment must be additionally performed at the weld toes for the parent material using structural hot-spot stress (see Sect. 2.2.3) and the associated fatigue class (FAT) for the base material. Other modes of fatigue failure, such as crack growth from surface roughness or embedded defects, are not covered. The method is also not applicable if there is a signiﬁcant stress component parallel to the weld. The method is also restricted to assessment of naturally formed as-welded weld toes and roots (Fig. 2.18). At weld toes, an effective notch stress of at least 1.6 times the structural hot-spot stress should be assumed. This condition is usually given at welde roots. More details for practical application can be found in reference [23]. Fig. 2.16 Fictitious rounding of weld toes and roots 28 2 Fatigue Actions (Loading) Fig. 2.17 Recommended rounding of weld toes and ﬁllet weld roots Fig. 2.18 Recommended rounding at Y-joint and backing bar roots The method is well suited to the comparison of alternative weld geometries. Unless otherwise speciﬁed, it is suggested that welds should be modelled with flank angles of 30° for butt welds and 45° for ﬁllet welds. The method is limited to thicknesses t ≥ 5 mm, since the method has not yet been veriﬁed for smaller wall thicknesses. Welds toes, machined or ground to a speciﬁed proﬁle, shall be assessed using the notch stress of the actual proﬁle in conjunction with the nominal stress based fatigue resistance curve for a butt weld ground flush to plate. 2.2.4.2 Calculation of Effective Notch Stress Effective notch stresses or stress concentration factors can be calculated by parametric formulae, taken from diagrams or calculated by ﬁnite element or boundary element models. The effective notch radius is introduced such that the tip of the 2.2 Determination of Stresses and Stress Intensity Factors 29 Fig. 2.19 Recommended meshing at weld toes and roots Table 2.4 Recommended sizes of elements on surface Element type Relative size Absolute size [mm] No. of elements in 45° arc No. of elements in 360° arc Quadratic with mid-side nodes Linear ≤r/4 ≤0.25 ≥3 ≥24 ≤r/6 ≤0.15 ≥5 ≥40 radius coincides with the root of the real notch, e.g. the end of an unwelded root gap. For the determination of effective notch stress by FEA, element sizes of not more that 1/6 of the radius are recommended in case of linear elements, and 1/4 of the radius in case of higher order elements (Fig. 2.19 and Table 2.4). These sizes have to be observed in the curved parts as well as in the beginning of the straight part of the notch surfaces in both directions, tangential and normal to the surface, see also Ref. [22]. Possible misalignment has to be considered explicitly in the calculations. The model may be simpliﬁed from a 3-dimensional to a 2-dimensional one under the following conditions: (a) The loading should be mainly perpendicular to the weld, i.e. normal and shear stress in direction of the weld are not existent or small and can be neglected. (b) The loading and the geometry of the weld should not vary in the area to be assessed. At an occurrence of multiaxial stress, the principles of Chap. 4 should be applied. If there is a proportional loading, i.e. all stress components are in a constant phase, then the maximum principle stress may be used, provided that the minimum principle stress has the same sign. Both should be either positive or negative. In all other cases the regulations of Sect. 4.3 should be applied. 2.2.4.3 Measurement of Effective Notch Stress Because the effective notch radius is an idealization, it cannot be measured directly in the welded component. In contrast, the simple deﬁnition of the effective notch can be used for photo-elastic stress measurements in resin models. 30 2 Fatigue Actions (Loading) 2.2.5 Stress Intensity Factors 2.2.5.1 General Fracture was developed to assess the behaviour of cracks or crack-like imperfections in components (Fig. 2.20). The methods are well established, but require an adequate level of knowledge and experience. It is recommended to perform the assessment procedures using the recommendations given here and consulting the actual compendia of the method [43, 53]. Fracture mechanics is used for several purposes as e.g.: (a) Assessment of fracture, especially brittle fracture, in a component containing cracks or crack-like details. (b) Assessment of fatigue properties in a component containing cracks or crack-like imperfection as e.g. in welded joints. (c) Predicting the fatigue properties of severely notched components with no or a relatively short crack initiation phase. Welded joints behave as being severely notched. Predictions are made assuming small initial defects. The fatigue assessment procedure as in (b) and (c) is performed by the calculation of the growth of an initial crack ai to a ﬁnal size af. Since crack initiation occupies only a small proportion of the lives of welded joints in structural metals, the method is suitable for assessment of fatigue life, inspection intervals, crack-like weld imperfections and the effect of variable amplitude loading. The ﬁnal crack af may be estimated as about one half wall thickness, since there is a rapid onset of crack propagation. Only a few and insigniﬁcant numbers of cycles are spent in that phase of fatigue. Fig. 2.20 Examples for different categories of cracks 2.2 Determination of Stresses and Stress Intensity Factors 2.2.5.2 31 Determination of Stress Intensity Factors The parameter which describes the fatigue action at a crack tip in terms of crack propagation is the stress intensity factor (SIF) range ΔK. The starting crack conﬁguration is the centre crack in an inﬁnite plate. The stress intensity factor K is pﬃﬃﬃﬃﬃﬃﬃﬃﬃ deﬁned by the formula K ¼ r p a. Where σ is the remote stress in the plate and a is the crack parameter, here the half distance from tip to tip. 2.2.5.2.1 Standard Conﬁgurations In existing components, there are various crack conﬁgurations and geometrical shapes. So, corrections are needed for the deviation from the centre cracked plate. The formula for the stress intensity factor has to be expanded by a correction function Yu(a). These corrections take into account the following parameters and crack locations: (a) (b) (c) (d) (e) Free surface of a surface crack. Embedded crack located inside of a plate. Limited width or wall thickness. Shape of a crack, mostly taken as being elliptic. Distance to an edge. For a variety of crack conﬁgurations, parametric formulae for the correction function Yu(a) have been developed (see Appendix 6.2 and references [25, 53]). These correction functions are based on different applied stress types (e.g. membrane, bending, structural hot spot stress, nominal stress). The one used must correspond to the stress type under consideration. 2.2.5.2.2 Stress Intensity Factor for Weld Toes Fracture mechanics calculations related to welded joints are generally based on the total stress at the notch root, e.g. at the weld toe. The universal correction function Yu(a) may be separated into the correction of a standard conﬁguration Y(a) and an additional correction for the local notch of the weld toe Mk(a). A further separation into membrane stress and shell bending stress was done at most of the parametric formulae for the functions Y(a) and Mk(a) [32, 34]. K ¼r pﬃﬃﬃﬃﬃﬃﬃﬃﬃ p a Yu ðaÞ ð2:18Þ In practical application, ﬁrst the relevant applied stress (usually the local nominal or the structural hot spot stress) at the location of the crack is determined, assuming that no crack is present. If required, the stress should be separated into membrane and shell bending stress components. The stress intensity factor (SIF) K then results as a superposition of the effects of both stress components. The effects of the crack 32 2 Fatigue Actions (Loading) shape and size are covered by the correction function Y. The effects of the any remaining stress raising discontinuity or notch from the weld toe (non-linear peak stress) can to be covered by additional factors Mk, while K¼ where K σm σb Ym Yb Mk, m Mk, b pﬃﬃﬃﬃﬃﬃﬃﬃﬃ p a ðrm Ym ðaÞ Mk; m ðaÞ þ rb ðaÞ Yb ðaÞ Mk; b ðaÞÞ ð2:18aÞ stress intensity factor membrane stress shell bending stress correction function for membrane stress intensity factor correction function for shell bending stress intensity factor correction for non-linear stress peak in terms of membrane action Correction for non-linear stress peak in terms of shell bending The correction functions Ym and Yb can be found in the literature. The solutions in Ref. [25–30] are particularly recommended. For most cases, the formulae for stress intensity factors given in Appendix 6.2 are adequate. Mk-factors may be found in references [31, 32]. 2.2.5.2.3 Weight Function Approach The weight function approach is based on the idea that a given stress distribution can discretized into differential pairs of split forces which open a crack. The action of each differential force on a crack can be described by a function, the so called weight function h(x, a). The determination of the stress intensity factor is thus reduced into an integration over the crack length. By this method, arbitrary stress distributions can be assessed. The basic formulation of the weight function approach is Zx¼a K¼ rðxÞ hðx; aÞ dx ð2:19Þ x¼0 Weight functions have been developed for 2-dimensional (Fett and Munz Ref. [39]) and 3-dimensional problems (Glinka et al., see Appendix 6.2 and Ref. [40]). More weight functions may be found in literature (Ref. [43]). The application of weight functions requires an integration process to obtain the stress intensity factor. Here it must be observed that several weight functions lead to improper integrals, i.e. integrals with inﬁnite boundaries but ﬁnite solutions. There are two ways to overcome. Firstly to use very ﬁne steps near the singularity, or secondly to integrate analytically, if possible, and to calculate small stripes, which are later summed up for the number of cycles. 2.2 Determination of Stresses and Stress Intensity Factors 33 For transverse loaded welds, parametric formulae for the stress distribution in the plate have been developed. In these cases a ﬁnite element calculation may not be necessary (Hall et al. Ref. [41]) 2.2.5.2.4 Finite Element Programs The determination of stresses and stress distributions ﬁnite element programs may be used. It must be made sure that the reﬁnement of the meshing corresponds to method, which is used for deriving the stress intensity factors. For the use of standard solutions and existing Mk formulae, a coarse meshing may be sufﬁcient to determine the membrane and the shell bending stress. If a weight function approach is used, a ﬁne meshing is needed for a full information about the stress distribution at the weld toe or root, whichever is considered. Several program systems exist which provide a direct determination of stress intensity factors. The meshing should be made according to the method used and to the recommendations of the program manual. 2.2.5.2.5 Aspect Ratio The aspect ratio a:c is a signiﬁcant parameter for the stress intensity factor (Fig. 2.21). It has to be taken into consideration at fracture mechanics calculations. This consideration can be done in different ways: (a) Direct determination and calculation of crack growth in c-direction, e.g. by 3-dimensional weight functions or Mk-formulae. These formulae give the stress intensity factor at the surface, which governs the crack propagation in c-direction. (b) Application of formulae and values which have been derived from toes of ﬁllet welds by ﬁtting of experimental data, a possible example is given by Engesvik [44]. 2 c ¼ 0:27 þ 6:34 a if a [ 0:1\a\3 mm a=ð2 cÞ ¼ 0 if a [ 3 mm Fig. 2.21 Crack parameters ð2:20Þ 34 2 Fatigue Actions (Loading) (c) If only 2-dimensional Mk values are given, then the crack depth of a = 0.15 or 0.1 mm may be used to calculate the effective stress intensity factor at the surface for the crack propagation in “c”-direction [53]. (d) A constant aspect ratio of a:c = 0.1 may be taken as a conservative approach. 2.2.5.2.6 Assessment of Welded Joints Without Detected Imperfections Fracture mechanics may be used to assess the fatigue properties of welded joints in which no imperfections have been detected. In such cases it is necessary to assume the presence of an initial crack, for example based on prior metallurgical evidence, the detection limit of the used inspection method or ﬁtting from fatigue data, and then to calculate the stress intensity factor as above. In case of post-weld treatment there is a possibly larger number of cycles for crack initiation. That shall be assessed and/or considered by a appropriate calculation procedure, which might be taken from the relevant literature. For cracks starting from a weld toe, in absences of other evidence, it is recommended that an initial crack depth of at a = 0.1 mm and an aspect ratio as given above might be taken considering that there might be multiple spots for crack initiation. The initial cracks have been derived from ﬁtting the assessment procedure to experimental data, disregarding possible fracture mechanics short crack effects. If possible, the calculations should be compared or calibrated at similar joint details with known fatigue properties. If no weld toe radius ρ was speciﬁed or determined by measuring, it is recommended to assume a sharp corner i.e. a toe radius of ρ = 0 to ρ = 0.2 mm. For root gaps in load-carrying ﬁllet welded cruciform joints, the actual root gap should be taken as the initial crack. It is convenient to disregard the threshold properties. Later the obtained fatigue cycles may be converted into a FAT class and to proceed using that S-N curve. rﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ N m FAT ¼ Drapplied 2 106 2.3 2.3.1 ð2:21Þ Stress History General The fatigue design data presented in Chap. 3 were obtained from tests performed under constant amplitude loading. However, loads and the resulting fatigue actions (i.e. stresses) in real structures usually fluctuate in an irregular manner and give rise to variable amplitude loading. The stress range may vary in both magnitude and period from cycle to cycle. 2.3 Stress History 35 Fig. 2.22 Stress time history illustration The stress history is a record and/or a representation of the fluctuations of the fatigue actions in the anticipated service time of the component. It is described in terms of successive maxima and minima of the stress caused by the fatigue actions (Fig. 2.22). It should aim to cover all loading events and the corresponding induced dynamic response in a conservative way. In most cases, the stress-time history is stationary and ergodic, which allows the deﬁnition of a mean range and its variance, a statistical histogram and distribution, an energy spectrum and a maximum values probabilistic distribution from a representation covering a limited period of operation. Therefore, the data needed to perform a fatigue analysis can be determined from service load measurements or observations conducted over a limited time, as long as it is reasonably representative of the loading to be experienced during the whole fatigue life. A stress history may be given as (a) a record of successive maxima and minima of stress measured in a comparable structure for comparable loading and service life, or a typical sequence of load events. (b) a two dimensional transition matrix of the stress history derived from a). (c) a one- or two-dimensional stress range histogram (stress range occurrences) obtained from a) by a speciﬁed counting method. (d) a one-dimensional stress range histogram (stress range exceedences, stress range spectrum) speciﬁed by a design code. The representations (a) and (b) may be used for component testing, while (c) and (d) are most useful for fatigue assessment by calculation. 2.3.2 Cycle Counting Methods Cycle counting is the process of converting a variable amplitude stress sequence into a series of constant amplitude stress range cycles that are equivalent in terms of damage to the original sequence. Various methods are available including zero crossing counting, peak counting, range pair counting and rainflow counting. For 36 2 Fatigue Actions (Loading) welded components, the ‘rainflow’ or similar ‘reservoir’ methods are recommended for counting stress ranges [58, 59]. 2.3.3 Cumulative Frequency Diagram (Stress Spectrum) The cumulative frequency diagram (stress spectrum) corresponds to the cumulative probability of stress range expressed in terms of stress range level exceedences versus the number of cycles. The curve is therefore continuous. It is usually more convenient to represent the spectrum by a table of discrete blocks of cycles of constant amplitude stress range, typically up to 20 different stress levels. The assumed magnitude of the stress range in a given block would then depend on the conservatism required. Typical values would be the maximum or the mean of the stress range in the block. Besides the representation in probabilities, a presentation of the number of occurrences or exceedances in a given number of cycles, e.g. 1 million, is used. An example showing a Gaussian normal distribution is given below (Table 2.5 and Fig. 2.23): Table 2.5 Example of a stress range occurrence table (stress histogram or frequency) Fig. 2.23 Example of a cumulative frequency diagram (stress spectrum) Block No. Relative stress range Occurrence (frequency) 1 2 3 4 5 6 7 8 1.000 0.950 0.850 0.725 0.575 0.425 0.275 0.125 2 16 280 2720 20000 92000 280000 605000 Chapter 3 Fatigue Resistance 3.1 Basic Principles Fatigue resistance is usually derived from constant or variable amplitude tests. The fatigue resistance data given here are based on published results from constant amplitude tests. Guidance on the direct use of fatigue test data is given in Sects. 3.7 and 4.5. As generally required, the fatigue resistance data presented here are expressed in terms of the same type of stress as that, used to determine the test data upon which they are based. The present fatigue endurance resistance data for welded joints are expressed as S-N curves. However, there are different deﬁnitions of failure in conventional fatigue endurance testing. In general, small welded specimens are tested to complete rupture, which is usually very close to through-thickness cracking. In large components or vessels, the observation of a larger or through-wall crack is usually taken as a failure. The fatigue failure according to the present S-N curves effectively corresponds to through-section cracking. The S-N curves are of the form: N¼ C Drm or N¼ C Dsm ð3:1Þ where the slope m may adopt different values over the range of possible fatigue lives, from the low endurance to the high cycle regime (see Sect. 3.2). For fracture mechanics analyses, the fatigue resistance data are in the form of relationships between ΔK and the rate of fatigue crack propagation (da/dN). The fatigue crack growth rate data are derived by monitoring crack propagation in tests. All fatigue resistance data are given as characteristic values, which are assumed to represent a survival probability of at least 95 %, calculated from the mean value on the basis of two-sided 75 % tolerance limits of the mean, unless otherwise stated (see Sect. 3.7). Other existing deﬁnitions as e.g. a survival probability of 95 % on the basis of 95 % one-sided limit of the mean or mean minus two standard © Springer International Publishing Switzerland 2016 A.F. Hobbacher, Recommendations for Fatigue Design of Welded Joints and Components, IIW Collection, DOI 10.1007/978-3-319-23757-2_3 37 38 3 Fatigue Resistance deviations corresponding to a survival probability of 97.7 % are practically equal for engineering applications. The (nominal) stress range should be within the limits of the elastic properties of the material. The range of the design values of the stress range shall not exceed 1.5 · fy for nominal normal stresses or 1.5 · fy/√3 for nominal shear stresses. The fatigue resistance of a welded joint is also limited by the fatigue resistance of the parent material. 3.2 Fatigue Resistance of Classiﬁed Structural Details The fatigue assessment of classiﬁed structural details and welded joints is based on the nominal stress range. In most cases, structural details are assessed on the basis of the maximum principal stress range in the section where potential fatigue cracking is considered. However, guidance is also given for the assessment of shear loaded details, based on the maximum shear stress range. Separate S-N curves are provided for consideration of normal or shear stress ranges, as illustrated in Figs. 3.1, 3.2 and 3.3 respectively. Care must be taken to ensure that the stress used for the fatigue assessment is the same as that given in the tables of the classiﬁed structural details. Macro-structural hot spot stress concentrations not covered by the structural detail of the joint itself, e.g. large cut-outs in the vicinity of the joint, have to be accounted for by the use of a detailed stress analysis, e.g. ﬁnite element analysis, or appropriate stress concentration factors (see Sect. 2.2.2). Fig. 3.1 Fatigue resistance S-N curves for steel, normal stress, standard applications 3.2 Fatigue Resistance of Classiﬁed Structural Details Fig. 3.2 Fatigue resistance S-N curves for steel, normal stress, very high cycles applications Fig. 3.3 Fatigue resistance S-N curves for aluminium, normal stress 39 40 3 Fatigue Resistance The fatigue curves are based on representative experimental investigations and thus include the effects of: • • • • • • • • • structural hot spot stress concentrations due to the detail shown local stress concentrations due to the weld geometry weld imperfections consistent with normal fabrication standards direction of loading high residual stresses metallurgical conditions welding process (fusion welding, unless otherwise stated) inspection procedure (NDT), if speciﬁed post weld treatment, if speciﬁed Furthermore, within the limits imposed by static strength considerations, the fatigue curves of welded joints are independent of the tensile strength of the material. Each fatigue strength S-N curve is identiﬁed by the characteristic fatigue strength of the detail in MPa at 2 million cycles. This value is the fatigue class (FAT). The slope of the fatigue strength S-N curves for details assessed on the basis of normal stresses (Fig. 3.1) is m = 3.00 if not stated expressly otherwise. The constant amplitude knee point is assumed to correspond to N = 107 cycles. The slope of the fatigue strength curves for details assessed on the basis of shear stresses (Figs. 3.2, 3.4, 3.5 and 3.6) is m = 5.00, but in this case the knee point is assumed to correspond to N = 108 cycles. The conventional assumption is that the S-N curves terminate at a fatigue limit, below which failure will not occur, or in which case the S-N curve becomes a horizontal line. Traditionally, this constant amplitude fatigue limit (CAFL), also referred as ‘knee point’, is deﬁned in terms of the corresponding fatigue endurance on the S-N curve, N = 107 being the most common assumption (see Fig. 3.1). However, new experimental data indicate that a CAFL does not exist and the S-N curve should continue on the basis of a further decline in stress range of about 10 % per decade in terms of cycles, which corresponds to a slope of m = 22. This issue is only relevant if a design is expected to withstand very large numbers of stress cycles, such as for example at rotating welded machine parts. The matter is still under development and users should consult the latest relevant literature. Meanwhile, the nominal stress-based characteristic S-N curves are presented with the extrapolation beyond 107 cycles at a slope of m = 22 in Figs. 3.2 and 3.3. The descriptions of the structural details only partially include information about the weld size, shape and quality. The data refer to a standard quality as given in codes and standard welding procedures. For higher or lower qualities, conditions of welding may be speciﬁed and veriﬁed by test (Sect. 3.7). 3.2 Fatigue Resistance of Classiﬁed Structural Details Fig. 3.4 Fatigue resistance S-N curve for shear at steel, standard applications Fig. 3.5 Fatigue resistance S-N curves for shear at steel, very high cycle applications 41 42 3 Fatigue Resistance Fig. 3.6 Fatigue resistance S-N curve for shear at aluminium As appropriate, the fatigue classes given in Table 3.1 shall be modiﬁed according to Sect. 3.5. The limitations on weld imperfections shall be considered (Sect. 3.8). All butt weld joints shall be fully fused and have full penetration welds, unless otherwise stated. All the S-N curves for weld details are limited by the S-N curve for the parent metal, which may vary with material tensile strength. It is recommended that a higher fatigue class for the material than stated (i.e. FAT 160 for steel or FAT 71 for aluminium alloys) should only be assumed if veriﬁed by test. The S-N curves for weld details refer to speciﬁc failure modes, generally fatigue crack growth from the weld toe through the base material, from the weld root trough the weld throat, or from the weld surface through the weld and then into the base material. In an assessment of a given weld detail it is important to consider all possible potential failure modes for the direction of loading. E.g. at cruciform joints with ﬁllet welds, both potential failure modes, such as toe crack through plate and root crack through weld throat, have to be assessed. 125 100 80 Machine thermally cut edges, corners removed, no cracks by inspection m=3 Manually thermally cut edges, free from cracks and severe notches m = 3 Manually thermally cut edges, uncontrolled, no notch deeper than 0.5 mm m=3 123 124 140 160 FAT St. 122 121 Unwelded parts of a component Rolled or extruded products, components with machined edges, seamless hollow sections m=5 Steel: A higher FAT class may be used if veriﬁed by test or speciﬁed by applicable code Al.: AA 5000/6000 alloys AA 7000 alloys Machine gas cut or sheared material with subsequent dressing, no cracks by inspection, no visible imperfections m=3 100 111 Description (St. = steel; Al. = aluminium) Structural Detail No. Notch effects due to shape of edges shall be considered – (continued) Notch effects due to shape of edges shall be considered All visible signs of edge imperfections to be removed. The cut surfaces to be machined or ground, all burrs to be removed No repair by welding reﬁll Notch effects due to shape of edges shall be considered Notch effects due to shape of edges shall be considered No fatigue resistance of any detail to be higher at any number of cycles Sharp edges, surface and rolling flaws to be removed by grinding. Any machining lines or grooves to be parallel to stresses Requirements and remarks – 40 71 80 — FAT Al. Table 3.1 Fatigue resistance values for structural details in steel and aluminium assessed on the basis of nominal stresses 3.2 Fatigue Resistance of Classiﬁed Structural Details 43 71 71 63 36 Transverse butt welds welded from one side without backing bar, full penetration Root checked by appropriate NDT including visual inspection NDT without visual inspection No NDT 28 20 12 25 80 216 215 214 32 25 28 80 213 36 45 FAT Al. Transverse butt weld not satisfying conditions of 212, NDT Al.: Butt weld with toe angle ≤ 50° Butt welds with toe angle > 50° Transverse butt weld, welded on non-fusible temporary backing, root crack Transverse butt weld on permanent backing bar 90 Transverse butt weld made in shop in flat position, NDT weld reinforcement <0.1 Α thickness 112 FAT St. 212 Butt welds, transverse loaded Transverse loaded butt weld (X-groove or V-groove) ground flush to plate, 100 % NDT 200 211 Description (St. = steel; Al. = aluminium) Structural Detail No. Table 3.1 (continued) Misalignment <10 % of plate thickness (continued) All welds ground flush to surface, grinding parallel to direction of stress. Weld run-on and run-off pieces to be used and subsequently removed. Plate edges ground flush in direction of stress. Welded from both sides. Misalignment <5 % of plate thickness Proved free from signiﬁcant defects by appropriate NDT Weld run-on and run-off pieces to be used and subsequently removed. Plate edges ground flush in direction of stress. Welded from both sides. Misalignment <5 % of plate thickness Weld run-on and run-off pieces to be used and subsequently removed. Plate edges ground flush in direction of stress. Welded from both sides. Misalignment <10 % of plate thickness Backing removed, root visually inspected Misalignment <10 % of plate thickness Misalignment <10 % of plate thickness Requirements and remarks 44 3 Fatigue Resistance Transverse butt weld ground flush, NDT, with transition in thickness and width Slope 1:5 Slope 1:3 Slope 1:2 Transverse butt weld made in shop, welded in flat position, weld proﬁle controlled, NDT, with transition in thickness and width: Slope 1:5 Slope 1:3 Slope 1:2 Transverse butt weld, NDT, with transition on thickness and width Slope 1:5 Slope 1:3 Slope 1:2 221 222 223 Description (St. = steel; Al. = aluminium) Transverse partial penetration butt weld, analysis based on stress in weld throat sectional area, weld overﬁll not to be taken into account Structural Detail 217 No. Table 3.1 (continued) 80 71 63 90 80 72 112 100 90 36 FAT St. 25 22 20 32 28 25 45 40 32 12 FAT Al. The detail is not recommended for fatigue loaded members Assessment by notch stress or fracture mechanics is preferred All welds ground flush to surface, grinding parallel to direction of loading. Weld run-on and run-off pieces to be used and subsequently removed. Plate edges to be ground flush in direction of stress Misalignment due to deliberate thickness step to be considered, see Sect. 3.8.2. Additional misalignment due to fabrication imperfection < 5 % of plate thickness Weld run-on and run-off pieces to be used and subsequently removed. Plate edges ground flush in direction of stress Misalignment due to deliberate thickness step to be considered, see Sect. 3.8.2. Additional misalignment due to fabrication imperfection < 5 % of plate thickness Weld run-on and run-off pieces to be used and subsequently removed. Plate edges ground flush in direction of stress Misalignment due to deliberate thickness step to be considered, see Sect. 3.8.2. Additional misalignment due to fabrication imperfection < 10 % of plate thickness (continued) Requirements and remarks 3.2 Fatigue Resistance of Classiﬁed Structural Details 45 234 233 Transverse butt weld splice in rectangular hollow section, welded from one side, full penetration, root crack root inspected by NDT, t >=8 mm root inspected by NDT, t < 8 mm no NDT Transverse butt weld splice in circular hollow section, welded from one side, full penetration, potential failure from root root inspected by NDT no NDT Tubular joint with permanent backing 232 71 56 36 71 36 71 80 Transverse butt weld splice in rolled section or bar besides flats, ground flush, NDT 231 22 71 28 25 12 28 12 28 28 40 22 FAT Al. 71 FAT St. 100 Transverse butt weld, different thicknesses without transition, centres aligned In cases, where weld proﬁle is equivalent to a moderate slope transition, see no. 222 Three plate connection, potential cracking from root Description (St. = steel; Al. = aluminium) Transverse butt weld flange splice in built-up section welded prior to the assembly, ground flush, with radius transition, NDT Structural Detail 226 225 224 No. Table 3.1 (continued) Welded in flat position Full peneration weld (continued) Welded in flat position Axial misalignment < 5 % of wall thickness All welds ground flush to surface, grinding parallel to direction of stress. Weld run-on and run-off pieces to be used and subsequently removed. Plate edges ground flush in direction of stress All welds ground flush to surface, grinding parallel to direction of stress. Weld run-on and run-off pieces to be used and subsequently removed. Plate edges ground flush in direction of stress Misalignment < 10 % of plate thickness Misalignment < 10 % of plate thickness If centers are deliberately misaligned, this misalignment has to be considered, see Sect. 3.8.2 Requirements and remarks 46 3 Fatigue Resistance 28 20 80 71 50 Transverse butt weld at intersecting flange, weld ground flush, NDT, at crossing flanges with welded triangular transition plates, weld ends ground Crack starting at butt weld For crack of continuous flange see details 525 and 526 Transverse butt weld at intersecting flange, NDT, at crossing flanges, with welded triangular transition plates, weld ends ground Crack starting at butt weld For crack of continuous flange see details 525 and 526 Transverse butt weld at intersecting flange Crack starting at butt weld For crack of continuous flange see details 525 and 526 243 245 244 32 90 Transverse butt weld made in shop at flat position, weld proﬁle controlled, NDT, at crossing flanges, radius transition 242 36 40 100 Transverse butt weld ground flush, weld ends and radius ground, 100 % NDT at crossing flanges, radius transition 241 FAT Al. FAT St. Structural Detail Description (St. = steel; Al. = aluminium) No. Table 3.1 (continued) (continued) Welded from both sides. Misalignment < 10 % of plate thickness Plate edges ground flush in direction of stress Welded from both sides. Misalignment < 10 % of plate thickness All welds ground flush to surface, grinding parallel to direction of stress. Weld run-on and run-off pieces to be used and subsequently removed. Plate edges ground flush in direction of stress Welded from both sides. No misalignment Weld run-on and run-off pieces to be used and subsequently removed. Plate edges ground flush in direction of stress Welded from both sides.Misalignment < 5 % of plate thickness All welds ground flush to surface, grinding parallel to direction of stress. Plate edges ground flush in direction of stress Welded from both sides. Misalignment < 10 % of plate thickness Requirements and remarks 3.2 Fatigue Resistance of Classiﬁed Structural Details 47 112 90 Continuous automatic longitudinal double sided ﬁllet weld without stop/start positions (based on stress range in flange) Continuous manual longitudinal ﬁllet or butt weld (based on stress range in flange) 322 323 36 90 36 45 50 45 112 125 36 50 90 125 Continuous automatic longitudinal fully penetrated K-butt weld without stop/start positions (based on stress range in flange) NDT 50 FAT Al. 125 FAT St. 321 313 312 Longitudinal load-carrying welds Automatic longitudinal seam welds without stop/start positions in hollow sections with stop/start positions Longitudinal butt weld, both sides ground flush parallel to load direction, or continuous automatic longitudinal butt weld without start/stop positions proved free from signiﬁcant defects by appropriate NDT Longitudinal butt weld, without stop/start positions, NDT with stop/start positions 300 311 Description (St. = steel; Al. = aluminium) Structural Detail No. Table 3.1 (continued) (continued) No stop-start position is permitted except when the repair is performed by a specialist and inspection is carried out to verify the proper execution of the weld Requirements and remarks 48 3 Fatigue Resistance 325 324 No. Structural Detail Table 3.1 (continued) Intermittent longitudinal ﬁllet weld (based on normal stress in flange σ and shear stress in web τ at weld ends) τ/σ = 0 0.0–0.2 0.2–0.3 0.3–0.4 0.4–0.5 0.5–0.6 0.6–0.7 >0.7 Longitudinal butt weld, ﬁllet weld or intermittent weld with cope holes (based on normal stress in flange σ and shear stress in web τ at weld ends), cope holes not higher than 40 % of web τ/σ = 0 0.0–0.2 0.2–0.3 0.3–0.4 0.4–0.5 0.5–0.6 >0.6 Description (St. = steel; Al. = aluminium) 71 63 56 50 45 40 36 80 71 63 56 50 45 40 36 FAT St. 28 25 22 20 18 16 14 32 28 25 22 20 18 16 14 FAT Al. (continued) Analysis based on normal stress in flange and shear stress in web at weld ends Representation by formula: Steel: FAT = 71 · (1 − Δτ/Δσ) but not lower than 36 Alum.: FAT = 28 . (1 − Δτ/Δσ) but not lower than 14 Analysis based on normal stress in flange and shear stress in web at weld ends Representation by formula: Steel: FAT = 80 · (1 - Δτ/Δσ) but not lower than 36 Alum.: FAT = 32 · (1 - Δτ/Δσ) but not lower than 14 Requirements and remarks 3.2 Fatigue Resistance of Classiﬁed Structural Details 49 400 411 332 Joint at stiffened knuckle of a flange to be assessed according to no. 411–414, depending on type of joint Stress in stiffener plate: Af 2 sin a r ¼ rf P Ast Af = area of flange Ast = area of stiffener Af Stress in weld throat: r ¼ rf P 2 sin a Aw Aw = area of weld throat Unstiffened curved flange to web joint, to be assessed according to no. 411–414, depending on type of joint Stress in web plate: Ff r¼ r t Stress in weld throat: Ff r¼ r Ra Ff axial force in flange t thickness of web plate a weld throat Cruciform joints and/or T-joints Cruciform joint or T-joint, K-butt welds, full penetration, weld toes ground, potential failure from weld toe Single sided T-joints 331 Description (St. = steel; Al. = aluminium) Structural Detail No. Table 3.1 (continued) 32 90 — — 28 — — 80 FAT Al. FAT St. (continued) Advisable to ensure that intermediate plate was checked against susceptibility to lamellar tearing Misalignment < 15 % of primary plate thickness in cruciform joints The resulting force of Ff-left and Ff-right will bend the flange perpendicular to the plane of main loading. In order to minimize this additional stressing of the welds, it is recommended to minimize the width and to maximize the thickness of the flange Stress parallel to the weld is to be considered. For additional shear, principal stress in web is to be consired (see 321–323) Requirements and remarks 50 3 Fatigue Resistance Cruciform joint or T-joint, ﬁllet welds or partial penetration K-butt welds including toe ground joints, potential failure from weld root For a/t <=1/3 Cruciform joint or T-joint, single-sided arc or laser beam welded V-butt weld, full penetration, potential failure from weld toe. Full penetration checked by inspection of root If root is not inspected, then root crack Cruciform joint or T-joint, single-sided arc welded ﬁllet or partial penetration Y-butt weld, no lamellar tearing, misalignment of plates e < 0.15 · t, stress at weld root. Penetration veriﬁed Attention: Bending by excenricity e must be consired! 414 415 416 Cruciform joint or T-joint, ﬁllet welds or partial penetration K-butt welds, potential failure from weld toe Single sided T-joints 413 Description (St. = steel; Al. = aluminium) Cruciform joint or T-joint, K-butt welds, full penetration, potential failure from weld toe Single sided T-joints Structural Detail 412 No. Table 3.1 (continued) 12 25 36 71 14 25 40 71 12 25 71 36 22 28 80 63 25 FAT Al. 71 FAT St. Analysis based on axial and bending stress in weld throat. Excentricity e to be considered in analysis. Stress at weld root: Δσ w, root = Δσ w, nom · (1 + 6e/a) e = excentricity between midpoints plate and weld throat a (inclusive penetration), rotated into vertical leg plane using root tip as pivot An analysis by effective notch stress procedure is recommended (continued) Advisable to ensure that intermediate plate was checked against susceptibility to lamellar tearing Misalignment < 15 % of primary plate thickness in cruciform joints Advisable to ensure that intermediate plate was checked against susceptibility to lamellar tearing Misalignment < 15 % of primary plate thickness in cruciform joints Also to be assessed as 414 Analysis P based on stress in weld throat rw ¼ F= ðaw lÞ l = length of weld, aw = load carrying weld throat. Also to be assessed as 413 Advisable to ensure that intermediate plate was checked against susceptibility to lamellar tearing Misalignment < 15 % of primary plate thickness in cruciform joints Requirements and remarks 3.2 Fatigue Resistance of Classiﬁed Structural Details 51 425 424 423 Splice of rectangular hollow section with intermediate plate, ﬁllet welds, potential failure from root wall thickness > 8 mm wall thickness < 8 mm Splice of circular hollow section with intermediate plate, singlesided butt weld, potential failure from toe wall thickness > 8 mm wall thickness < 8 mm Splice of circular hollow section with intermediate plate, ﬁllet weld, potential failure from root. Analysis based on stress in weld throat wall thickness >8 mm wall thickness <8 mm Splice of rectangular hollow section, single-sided butt weld, potential fairure from toe wall thickness > 8 mm wall thickness < 8 mm 422 Description (St. = steel; Al. = aluminium) Splice of rolled section with intermediate plate, ﬁllet welds, potential failure from weld root Structural Detail 421 No. Table 3.1 (continued) 40 36 50 45 45 40 56 50 36 FAT St. 16 14 20 18 16 14 22 20 12 FAT Al. (continued) NDT of welds in order to ensure full root penetration NDT of welds in order to ensure full root penetration Analysis based on stress in weld throat Requirements and remarks 52 3 Fatigue Resistance 514 513 512 500 511 Trapezoidal stiffener to deck plate, full penetration butt weld, calculated on basis of stiffener thickness, out of plane bending Weld connecting web and flange, loaded by a concentrated force in web plane perpendicular to weld. Force distributed on width b = 2 · h + 50 mm Assessment according to no. 411–414. A local bending due to eccentric load should be considered Non-load-carrying attachments Transverse non-load-carrying attachment, not thicker than main plate K-butt weld, toe ground Two sided ﬁllets, toe ground Fillet weld(s), as welded thicker than main plate Transverse stiffener welded on girder web or flange, not thicker than main plate K-butt weld, toe ground Two-sided ﬁllets, toe ground ﬁllet weld(s): as welded thicker than main plate Non-loadcarrying rectangular or circular flat studs, pads or plates L ≤ 50 mm L > 50 and ≤ 150 mm L > 150 and ≤ 300 mm L > 300 mm 431 Description (St. = steel; Al. = aluminium) Structural Detail No. Table 3.1 (continued) 71 80 71 63 50 100 100 80 71 100 100 80 71 – FAT St. 25 28 25 20 18 36 36 28 25 36 36 28 25 – FAT Al. (continued) Grinding marks normal to weld toe An angular misalignment corresponding to km = 1.2 is already covered Requirements and remarks 3.2 Fatigue Resistance of Classiﬁed Structural Details 53 Longitudinal ﬁllet welded gusset of length l. Fillet weld around end l < 50 mm l < 150 mm l < 300 mm l > 300 mm Longitudinal ﬁllet welded gusset with radius transition, ﬁllet weld around end and toe ground, c < 2 t, max 25 mm r > 150 mm Longitudinal ﬁllet welded gusset with smooth transition (sniped end or radius) welded on beam flange or plate, ﬁllet weld around end. c < 2 t, max 25 mm r > 0.5 h r < 0.5 h or ϕ > 20̊ Longitudinal flat side gusset welded on plate edge or beam flange edge, with smooth transition (sniped end or radius), ﬁllet weld around end. c < 2t2, max. 25 mm r > 0.5 h r < 0.5 h or ϕ > 20̊ 521 523 524 522 71 Trapezoidal stiffener to deck plate, ﬁllet or partial penetration weld, out of plane bending 515 50 45 71 63 80 71 63 50 90 FAT St. Structural Detail Description (St. = steel; Al. = aluminium) No. Table 3.1 (continued) 18 16 25 20 28 25 20 18 32 25 FAT Al. (continued) t = thickness of attachment If attachement thickness < 1/2 of base plat thickness, then one step higher allowed (not for welded on proﬁles!) Particularly suitable for assessment on the basis of structural hot spot stress approach t = thickness of attachment For t2 < 0.7 t1, FAT rises 12 % Particularly suitable for assessment on the basis of structural hot spot stress approach t = thickness of attachment Particularly suitable for assessment on the basis of structural hot spot stress approach For gusset on edge: see detail 525 Particularly suitable for assessment on the basis of structural hot spot stress approach Calculation based on maximum out-of-plane bending stress range in weld throat or stiffener Requirements and remarks 54 3 Fatigue Resistance 612 600 611 531 526 525 No. Lap joints Structural Detail Table 3.1 (continued) Transverse loaded lap joint with ﬁllet welds Fatigue of parent metal Fatigue of weld throat Longitudinally loaded lap joint with side ﬁllet welds Fatigue of parent metal Fatigue of weld (calc. on max. weld length of 40 times the throat of the weld) In-plane or out-of-plane longitudinal gusset welded to plate or beam flange edge, gusset length l: l < 150 mm l < 300 mm l > 300 mm Longitudinal flat side gusset welded on edge of plate or beam flange, radius transition ground r > 150 or r/w > 1/3 1/6 < r/w < 1/3 r/w < 1/6 Circular or rectangular hollow section, ﬁllet welded to another section. Section width parallel to stress direction < 100 mm, else like longitudinal attachment Description (St. = steel; Al. = aluminium) 50 50 63 45 90 71 50 71 50 45 40 FAT St. 18 18 22 16 36 28 22 28 18 16 14 FAT Al. (continued) Stresses to be calculated in the main plate using a plate width equal to the weld length Buckling avoided by loading or design! Buckling avoided by loading or design For veriﬁcation of parent metal, the higher stresses of the two members must be taken Non load-carrying welds. Width parallel to stress direction < 100 mm Smooth transition radius formed by grinding the weld area in transition in order to remove the weld toe completely. Grinding parallel to stress For t2 < 0.7 t1, FAT rises 12 % t1 is main plate thkcness t2 is gusset thickness Requirements and remarks 3.2 Fatigue Resistance of Classiﬁed Structural Details 55 721 712 700 711 614 613 No. Reinforcements Structural Detail Table 3.1 (continued) End of long doubling plate on beam, reinforced welded ends ground (based on stress range in flange at weld toe) tD ≤ 0.8 t 0.8 t < tD ≤ 1.5 t tD > 1.5 t End of reinforcement plate on rectangular hollow section wall thickness: t < 25 mm End of long doubling plate on I-beam, welded ends (based on stress range in flange at weld toe) tD ≤ 0.8 t 0.8 t < tD ≤ 1.5 t tD > 1.5 t Lap joint gusset, ﬁllet welded, non-load-carrying, with smooth transition (sniped end with ϕ < 20̊ or radius), welded to loaded element c < 2Αt, but c <= 25 mm to flat bar to bulb section to angle section Transverse loaded overlap joint with ﬁllet welds Stress in plate at weld toe (toe crack) Stress in weld throat (root crack) Description (St. = steel; Al. = aluminium) 71 63 56 50 56 50 45 63 36 63 56 50 FAT St. 28 25 22 20 20 18 16 22 12 22 20 18 FAT Al. No undercut at transverse weld! Grinding parallel to stress direction (continued) End zones of single or multiple welded cover plates, with or without transverse welds If the cover plate is wider than the flange, a transverse weld is needed. No undercut at transverse welds Stresses to be calculated using a plate width equalling the weld length For stress in plate, eccenticity to be considered, as given in chapters 3.8.2 and 6.3 Both failure modes have to be assessed separately t = thickness of gusset plate Requirements and remarks 56 3 Fatigue Resistance Fillet welded reinforcements Toe ground As welded Description (St. = steel; Al. = aluminium) 25 12 63 80 71 36 Fillet welded pipe to flat flange joint. Potential fatigue failure from weld toe in pipe Tubular branch or pipe penetrating a plate, K-butt welds Tubular branch or pipe penetrating a plate, ﬁllet welds. Toe cracks Root cracks (analysis based on stress in weld throat) 822 831 832 28 22 25 71 Flat flange with > 80 % full penetration butt welds, modiﬁed nominal stress in pipe, toe crack 22 12 25 32 25 FAT Al. 821 63 36 71 80 71 FAT St. Stiff block flange, partial penetration or ﬁllet weld toe crack in plate root crack in weld throat Flanges, branches and nozzles Stiff block flange, full penetration weld Structural Detail 812 800 811 731 No. Table 3.1 (continued) If diameter > 50 mm, stress concentration of cutout has to be considered Analysis based on modiﬁed nominal stress. However, structural hot spot stress recommended If diameter > 50 mm, stress concentration of cutout has to be considered Analysis based on modiﬁed nominal stress. However, structural hot spot stress recommended (continued) Analysis based on modiﬁed nominal stress. However, structural hot spot stress recommended Assessment by structural hot spot is recommended Grinding in direction of stress! Analysis based on modiﬁed nominal stress, however, structural hot spot stress approach recommended Requirements and remarks 3.2 Fatigue Resistance of Classiﬁed Structural Details 57 Fillet or partial penetration welded joint between circular tube or pipe and flange. Potential fatigue failure from weld root 913 But welded circular tube or pipe to solid bar joint. Potential fatigue failure from weld toe or root in tube or pipe Butt welded joint between circular tube or pipe and flange with integral backing. Potential fatigue failure fromweld root Tubular joints 912 900 911 50 63 63 63 Nozzle welded on pipe, root pass as welded 842 FAT St. 71 Description (St. = steel; Al. = aluminium) Nozzle welded on plate, root pass removed by drilling Structural Detail 841 No. Table 3.1 (continued) 18 22 22 22 25 FAT Al. (continued) Impairment of inspection of root cracks by NDT may be compensated by adequate safety considerations (see Sect. 3.5) or by downgrading by two FAT classes Analysis based on stress in tube or pipe Full penetration of weld to solid bas is required Analysis based on stress in tube or pipe Full penetration of weld to solid bas is required If diameter >50 mm, stress concentration of cutout has to be considered Analysis based on modiﬁed nominal stress. However, structural hot spot stress recommended If diameter > 50 mm, stress concentration of cutout has to be considered Analysis based on modiﬁed nominal stress. However, structural hot spot stress recommended Requirements and remarks 58 3 Fatigue Resistance 932 931 921 No. Structural Detail Table 3.1 (continued) Tube-plate joint, tube slitted and welded to plate tube diameter < 200 mm and plate thickness < 20 mm tube diameter > 200 mm or plate thickness > 20 mm Circular hollow section with welded on disc, potential fatigue failure from toe in hollow section K-butt weld, toe ground Fillet weld, toe ground Fillet welds, as welded Tube-plate joint, tubes flattened, butt weld (X-groove) Tube diameter < 200 mm and plate thickness < 20 mm Description (St. = steel; Al. = aluminium) 18 14 45 32 32 25 18 FAT Al. 63 90 90 71 63 FAT St. Requirements and remarks 3.2 Fatigue Resistance of Classiﬁed Structural Details 59 60 3 Fatigue Resistance Table 3.2 Fatigue resistance values for structural details on the basis of shear stress No Description (St. = steel; Al. = aluminium) FAT St. FAT Al. 1 2 Parent metal or full penetration butt weld; m = 5 down to 1E8 cycles Fillet weld or partial penetration butt weld; m = 5 down to 1E8 cycles 100 80 36 28 3.3 3.3.1 Fatigue Resistance Assessed on the Basis of Structural Hot Spot Stress Fatigue Resistance Using Reference S-N Curve The S-N curves for assessing the fatigue resistance of a detail on the basis of structural hot spot stress (Sect. 2.2.3) are given in the Table 3.2 for steel and aluminium, where the deﬁnition of the FAT class is given in Sect. 3.2. The resistance values refer to the as-welded condition unless stated otherwise. The effects of high tensile residual stress are included. Only small effects of misalignment are included, see also Sect. 3.8.2. The weld shape should be similar to that shown below (Table 3.3). The design value of the structural hot spot stress range Δσhs shall not exceed 2 · fy. The fatigue resistance of a welded joint is limited by the fatigue resistance of the base material. For hollow section joints, special hot-spot stress design S-N curves have been recommended by the IIW [14]. These tubular joint design curves should not be applied to other types of structure. 3.3.2 Fatigue Resistance Using a Reference Detail The tables of the fatigue resistance of structural details given in Sect. 3.2, or fatigue data from other sources which refer to a comparable detail, may be used. The reference detail should be chosen to be as similar as possible to the detail to be assessed. Thus, the procedure will be: (a) Select a reference detail with known fatigue resistance, which is as similar as possible to the detail being assessed with respect to geometric and loading parameters. (b) Identify the type of stress in which the fatigue resistance is expressed. This is usually the nominal stress (as in the tables in Sect. 3.2). (c) Establish a FEA model of the reference detail and the detail to be assessed with the same type of meshing and elements following the recommendations given in Sect. 2.2.3. 3.3 Fatigue Resistance Assessed on the Basis of Structural Hot Spot Stress 61 Table 3.3 Fatigue resistance against structural hot spot stress No. Structural detail Description Requirements FAT Steel FAT Alu. 1 Butt joint As welded, NDT 100 40 2 Cruciform or T-joint with full penetration K-butt welds K-butt welds, no lamellar tearing 100 40 3 Non load-carrying ﬁllet welds 100 40 4 Bracket ends, ends of longitudinal stiffeners Transverse non-load carrying attachment, not thicker than main plate, as welded Fillet welds welded around or not, as welded 100 40 5 Cover plate ends and similar joints As welded 100 40 6 Cruciform joints with load-carrying ﬁllet welds Fillet welds, as welded 90 36 7 Lap joint with load carrying ﬁllt welds Fillet welds, as welded 90 36 8 Type “b” joint with short attachment Fillet or full penetration weld, as welded 100 40 9 Type “b” joint with long attachment Fillet or full penetration weld, as welded 90 36 Note 1 Table does not cover larger effects of misalignment than those speciﬁed in Sect. 3.8.2. They have to be considered explicitly in the determination of the hot spot stress range Note 2 The nominally non- or partially load-carrying ﬁllet welds shown under no. 3 and 5 in Table 3.3 may actually be load-carrying, in certain cases, e.g. for very large attachments or if the bending of the base plate is restrained. In these cases load-carrying ﬁllet welds should be assumed with FAT classes given under no. 6 and 7 in Table 3.3. This may also apply to no. 4 without soft bracket end Note 3 A further reduction by one FAT class is recommended for ﬁllet welds having throat thicknesses of less than one third of the thickness of the base plate 62 3 Fatigue Resistance (d) Load the reference detail and the detail to be assessed with the stress identiﬁed in b). (e) Determine the structural hot spot stress σhs, ref of the reference detail and the structural hot spot stress σhs, assess of the detail to be assessed. (f) The fatigue resistance for 2 million cycles of the detail to be assessed FATassess is then calculated from fatigue class of the reference detail FATref by: FATassess ¼ 3.4 3.4.1 rhs; ref FATref rhs; assess ð3:2Þ Fatigue Resistance Assessed on the Basis of the Effective Notch Stress Steel The effective notch stress fatigue resistance against fatigue actions, as determined in Sect. 2.2.4 for steel [24], is given in Table 3.4. The deﬁnition of the FAT class is given in Sect. 3.2. The fatigue resistance value refers to the as-welded condition. The effect of high tensile residual stresses is included. The effect of possible misalignment is not included. The fatigue resistance of a weld toe is additionally limited by the fatigue resistance of the parent material, which is determined by the use of the structural hot-spot stress and the FAT class of the non-welded parent material. This additional check shall be performed according to Sect. 2.2.3. 3.4.2 Aluminium The same regulations apply as for steel (Table 3.5). Table 3.4 Effective notch fatigue resistance for steel No. Quality of weld notch Description FAT 1 Effective notch radius equal to 1 mm replacing weld toe and weld root notch Notch as-welded, normal welding quality m=3 225 Table 3.5 Effective notch fatigue resistance for aluminium No. Quality of weld notch Description FAT 1 Effective notch radius equal to 1 mm replacing weld toe and weld root notch Notch as-welded, normal welding quality m=3 71 3.5 Fatigue Strength Modiﬁcations 3.5 63 Fatigue Strength Modiﬁcations 3.5.1 Stress Ratio 3.5.1.1 Steel For effective stress ratios, based on consideration of both applied and residual stresses, R < 0.5 a fatigue enhancement factor f(R) may be considered by multiplying the fatigue class of classiﬁed details by f(R). This factor depends on the level and direction of residual stresses. Here, all types of stress which are not considered in fatigue analysis and which are effective during service loading of the structure are regarded as residual stress. The ranking in categories I, II or III should be documented by the design ofﬁce. If no reliable information on residual stress is available, an enhancement factor f(R) = 1 is recommended. Other factors should only be used if reliable information or estimations of the residual stress level are available [47]. The following cases are to be distinguished (Fig. 3.7): I. Unwelded base material and wrought products with negligible residual stresses (<0.2 · fy), stress relieved welded components, in which the effects of constraints or secondary stresses have been considered in analysis. No constraints in assembly f ðRÞ ¼ 1:6 f ðRÞ ¼ 0:4 R þ 1:2 f ðRÞ ¼ 1 Fig. 3.7 Enhancement factor f(R) for R\ 1 or completely in compression for 1 R 0:5 ð3:3Þ for R [ 0:5 64 3 Fatigue Resistance II. Small-scale thin-walled simple structural elements containing short welds. Parts or components containing thermally cut edges. No constraints in assembly. f ðRÞ ¼ 1:3 f ðRÞ ¼ 0:4 R þ 0:9 f ðRÞ ¼ 1 for R\ 1 or completely in compression for 1 R 0:25 ð3:4Þ for R [ 0:25 III. Complex two- or three-dimensional welded components, components with global residual stresses, thick-walled components. The normal case for welded components and structures. f ðRÞ ¼ 1 no enhancement ð3:5Þ It should be noted that stress relief in welded joints is unlikely to be fully effective, and additional residual stresses may be introduced by lack of ﬁt during assembly of prefabricated welded components, by displacements of abutments or for other reasons. Consequently, it is recommended that values of f(R) > 1 should only be adopted for welded components in very special circumstances. In several cases, stress relieving might reduce the fatigue properties as e.g. at TMCP steels by reduction of mechanical properties, or at weld roots in single sided butt welds or at ﬁllet welds, by reduction of beneﬁcial residual compressive stress. Note: For unwelded or stress relieved steel structures, a simpliﬁed approach may be used, which consists in considering only 60 % of the stresses in compression. 3.5.1.2 Aluminium The same regulations as for steel are recommended. 3.5.2 Wall Thickness Fatigue resistance modiﬁcations are required at the nominal stress method (see Sect. 3.2) and the hot spot structural stress method of type “a” at surface extrapolation as described in Sect. 3.3. It is not required at the effective notch stress method and at the fracture mechanics method (see Sects. 3.4 and 3.6). 3.5 Fatigue Strength Modiﬁcations 3.5.2.1 65 Steel The influence of plate thickness on fatigue strength should be taken into account in cases where the site for potential fatigue cracking is the weld toe. The fatigue resistance values given here for steel refer to a wall thickness up to 25 mm. The lower fatigue strength for thicker members is taken into consideration by multiplying the FAT class of the structural detail by the thickness reduction factor f(t): f ðtÞ ¼ n tref teff ð3:6Þ where the reference thickness tref = 25 mm. The thickness correction exponent n is dependent on the effective thickness teff and the joint category (see Table 3.6) [45]. In the same way a benign thinness effect might be considered, but this should be veriﬁed by component test. The plate thickness correction factor is not required in the case of assessment based on effective notch stress procedure or fracture mechanics. For the determination of teff, the following cases have to be distinguished (Fig. 3.8): if if L=t 2 then L=t\2 then teff ¼ t ð3:6aÞ teff ¼ 0:5 L or teff ¼ t which ever is the larger Table 3.6 Thickness correction exponents Joint category Condition n Cruciform joints, transverse T-joints, plates with transverse attachments, ends of longitudinal stiffeners Cruciform joints, transverse T-joints, plates with transverse attachments, ends of longitudinal stiffeners Transverse butt welds Butt welds ground flush, base material, longitudinal welds or attachments to plate edges as-welded 0.3 toe ground as-welded any 0.2 Fig. 3.8 Deﬁnition of toe distance L 0.2 0.1 66 3 Fatigue Resistance 3.5.2.2 Aluminium The same rules as for steel are recommended. 3.5.3 Improvement Techniques 3.5.3.1 General Post weld improvement techniques may increase the fatigue resistance, generally as a result of an improvement in the weld proﬁle, the residual stress conditions or the environmental conditions of the welded joint. They may be used to increase the fatigue strength of new structures, notably if a weld detail is found to be critical, or as a part of repair or upgrading of an existing structure. The main improvements techniques are: (a) Methods for improvement of weld proﬁle: Machining or grinding of but weld flush to the surface Machining or grinding of the weld transition at the toe Remelting of the weld toe by TIG-, plasma or laser dressing (b) Methods for improvement of residual stress conditions: Peening (hammer-, needle-, shot-, brush-peening or ultrasonic treatment) Overstressing (proof testing) Stress relief (c) Methods for improvement of environmental conditions: Painting Resin coating The effects of all improvement techniques are sensitive to the method of application and the applied loading, being most effective in the low stress high cycle regime. They may also depend on the material, the structural detail, the applied stress ratio and the dimensions of the welded joint. Consequently, fatigue tests for the veriﬁcation of the procedure in the endurance range of interest are recommended (Sects. 3.7 and 2.2.2). Recommendations are given below for the following post-welding weld toe improvement methods: grinding, TIG dressing, hammer and needle peening. 3.5.3.2 Applicability of Improvement Methods The recommendations apply to all arc welded steel or aluminium components subjected to fluctuating or cyclic stress and designed to a fatigue limit state 3.5 Fatigue Strength Modiﬁcations 67 criterion. They are limited to structural steels with speciﬁed yield strengths up to 900 MPa and to weldable structural aluminium alloys commonly used in welded structures, primarily of the AA 5000 and AA 6000 series but including weldable Al-Zn-Mg alloys. The recommendations apply to welded joints in plates, sections built up of plates or similar rolled or extruded shapes, and hollow sections. Unless otherwise speciﬁed, the plate thickness range for steel is 6 to 150 mm, while that for aluminium is 4 to 50 mm. The recommended levels of improvement in fatigue strength only apply when used in conjunction with the nominal stress or structural hot spot stress method. They do not apply to the effective notch stress or fracture mechanics method. The application is limited to joints operating at temperatures below the creep range. In general, the recommendations do not apply for low cycle fatigue conditions, so the nominal stress range is limited to Dr 1:5 fy . Additional restrictions may apply for speciﬁc improvement procedures. It is important to note that the fatigue resistance of an improved weld is limited by the fatigue resistance S-N curve of the base material. The improvement procedures described below, apply solely to the weld toe and hence to a potential fatigue crack growth starting from this point. Thus, weld details of the type illustrated in Fig. 3.9 are suitable for treatment. However, the beneﬁt of an improvement technique could be reduced as a result of intervention of fatigue cracking from the weld root. Thus, details of the kind shown in Fig. 3.10 are less suitable. In general, all potential alternative sites for fatigue crack initiation (e.g. weld root or imperfections) in treated welded joints should be assessed in order to establish the fatigue life of the weld detail under consideration. The beneﬁt factors due to the improvement techniques are presented as upgrades to the FAT class that applies to the as-welded joint. Alternative factors, including a possible change to a shallower, more favourable, slope of S-N curve for the improved weld, may be derived on the basis of special fatigue tests (see Sect. 4.5). A proﬁle improvement can sometimes assist in the application of a residual stress technique and vice versa (e.g. grinding before peening in the case of a poor Fig. 3.9 Examples of joints suitable for improvement 68 3 Fatigue Resistance Fig. 3.10 Examples of joints, in which an improvement might be limited by a possible root crack weld proﬁle or shot peening a dirty surface before TIG dressing). However, a higher beneﬁt factor than that applicable for the second technique alone can only be justiﬁed on the basis of special fatigue tests. 3.5.3.3 Grinding Weld toe fatigue cracks initiate at undercut, cold laps or the sharp crack-like imperfections, just a few tenths of a millimetre deep, which are an inherent feature of most arc welds. The aim of grinding is ﬁrstly to remove these imperfections and secondly to create a smooth transition between weld and plate, thus, reducing the stress concentration. All embedded imperfections revealed by grinding must be repaired. For the details of the grinding procedure see Ref. [46]. The beneﬁt of grinding is given as a factor on the stress range of the fatigue class of the non-improved joint, see Tables 3.7 and 3.8. The thickness correction exponent according to Sect. 3.5.2 Table 3.6 is n = 0.2. Table 3.7 FAT classes for use with nominal stress at joints improved by grinding Area of application and maximum possible claim Steel Aluminium Beneﬁt at details classiﬁed in as-welded condition as FAT ≤ 90 for steel or FAT ≤ 32 for aluminium Max possible FAT class after improvement 1.3 1.3 FAT 112 FAT 45 Table 3.8 FAT classes for use with structural hot-spot stress at joints improved by grinding Material Load-carrying ﬁllet welds Non-load-carrying ﬁllet welds and butt welds Mild steel, fy < 355 MPa Higher strength steel, fy ≥ 355 MPa Aluminium alloys 112 112 125 125 45 50 3.5 Fatigue Strength Modiﬁcations 3.5.3.4 69 TIG Dressing By TIG (tungsten inert gas) dressing, the weld toe is remolten in order to remove the weld toe imperfections and to produce a smooth transition from the weld to plate surface, thus reducing the stress concentration. The recommendations (Tables 3.9 and 3.10) apply to partial or full penetration arc welded in steels with a speciﬁed yield strength up to 900 MPa and to wall thicknesses ≥ 10 mm operating in a non-corrosive environment or under conditions of corrosion protection. The details of the procedure are described in Ref. [46]. The thickness correction exponent according to chapter 3.5.2 Table 3.6 is n = 0.2. A possible interaction between heat treatment and TIG dressing at aluminium alloys should be considered. 3.5.3.5 Hammer Peening By hammer peening, the material is plastically deformed at the weld toe in order to introduce beneﬁcial compressive residual stresses. The recommendations are restricted to steels with speciﬁed yield strengths up to 900 MPa and structural aluminium alloys, both operating in non-corrosive environments or under conditions of corrosion protection. The recommendations apply for plate thicknesses from 10 to 50 mm in steel and 5 to 25 mm in aluminium and to arc welded ﬁllet welds with a minimum weld leg length of 0.1 × t, where t is the thickness of the stressed plate (Tables 3.11 and 3.12). The details of the procedure are described in Ref. [46]. Special requirements apply when establishing the beneﬁt of hammer peening: Table 3.9 FAT classes for use with nominal stress at joints improved by TIG dressing Area of application and maximum possible claim Steel Aluminium Beneﬁt at details with FAT ≤ 90 at steel or FAT ≤ 32 at aluminium, as welded Max possible FAT class after improvement 1.3 1.3 FAT 112 FAT 45 Table 3.10 FAT classes for use with structural hot-spot stress at joints improved by TIG dressing Material Load-carrying ﬁllet welds Non-load-carrying ﬁllet welds and butt welds Mild steel, fy < 355 MPa Higher strength steel, fy > 355 MPa Aluminium alloys 112 112 45 125 125 50 70 3 Fatigue Resistance Table 3.11 FAT classes for use with nominal stress at joints improved by hammer peening Area of application and maximum possible claim Mild steel fy < 355 MPa Steel fy ≥ 355 MPa Aluminium Beneﬁt at details with FAT ≤ 90 at steel or FAT ≤ 32 at aluminium, as welded Max possible FAT after improvement 1.3 1.5 1.5 FAT 112 FAT 125 FAT 56 Table 3.12 FAT classes for use with structural hot-spot stress at joints improved by hammer peening Material Load-carrying ﬁllet welds Non-load-carrying ﬁllet welds Mild steel, fy < 355 MPa Higher strength steel, fy ≥ 355 MPa Aluminium alloys 112 125 50 125 140 56 (a) Maximum amount of nominal compressive stress in load spectrum including proof loading <0.25 fy (for aluminium, use fy of heat affected zone) (b) The S-N curve for the hammer peened weld is is used in conjunction with an effective stress range that depends on applied stress ratio R = minσ/maxσ as follows: if R < 0 The S-N resistance curve is used with full stress range Δσ if 0 < R ≤ 0.4 The S-N resistance curve is used with the maximum stress σmax if R > 0.4 Then there is no beneﬁt For wall thicknesses bigger than 25 mm, the thickness correction for as-welded joints still applies (see 3.5). 3.5.3.6 Needle Peening By needle peening, the material is plastically deformed at the weld toe in order to introduce beneﬁcial compressive residual stresses. The details of the procedure are described in [46]. Special requirements apply when establishing the beneﬁt of needle peening: (a) Maximum amount of nominal compressive stress in load spectrum including proof loading ≤ 0.25 fy (for aluminium, use fy of heat affected zone), see Tables 3.13 and 3.14. (b) The S-N curve for needle peened weld is expressed in terms of an effective stress range that depends on applied R ratio as follows: 3.5 Fatigue Strength Modiﬁcations 71 Table 3.13 FAT classes for use with nominal stress at joints improved by needle peening Area of application and maximum possible claim Mild steel fy < 355 MPa Steel fy ≥ 355 MPa Aluminium Beneﬁt at details with FAT ≤ 90 at steel or FAT ≤ 32 at aluminium, as welded Max possible FAT after improvement 1.3 1.5 1.5 FAT 112 FAT 125 FAT 56 Table 3.14 FAT classes for structural hot-spot stress at joints improved by needle peening Material Load-carrying ﬁllet welds Non-load-carrying ﬁllet welds Mild steel, fy < 355 MPa Higher strength steel, fy > 355 MPa Aluminium alloys 112 125 125 140 50 56 if R < 0 The S-N resistance curve is used with full stress range Δσ if 0 < R ≤ 0.4 The S-N resistance curve is used with the maximum stress σmax If R > 0.4 Then there is no beneﬁt For wall thicknesses bigger than 25 mm, the thickness correction for as-welded joints still applies (see 3.5). 3.5.4 Effect of Elevated Temperatures One of the main material parameters governing the fatigue resistance is the modulus of elasticity E which decreases with increase in temperature. So the fatigue resistance at elevated temperatures (HT) may be calculated as FATHT ¼ FAT20 C 3.5.4.1 EHT E20 C ð3:7Þ Steel For higher temperatures, the fatigue resistance data may be modiﬁed by the reduction factor given in Fig. 3.11. This fatigue reduction factor is a conservative approach and might be relaxed according to test evidence or applicable codes. Creep effects are not covered here. 72 3 Fatigue Resistance Fig. 3.11 Fatigue strength reduction factor for steel at elevated temperatures 3.5.4.2 Aluminium The fatigue data given here refer to operation temperatures lower than 70 °C. This value is a conservative approach. It may be raised according to test evidence or an applicable code. 3.5.5 Effect of Corrosion The fatigue resistance data given here refer to non-corrosive environments. Normal protection against atmospheric corrosion is assumed. A corrosive environment or unprotected exposure to atmospheric conditions may reduce the fatigue class. The position of the corresponding constant amplitude fatigue limit (CAFL or knee point) of the SN curve (traditionally the fatigue limit) may also be reduced considerably. The effect depends on the spectrum of fatigue actions and on the time of exposure. For steel, except stainless steel, in marine environment not more than 70 % of the fatigue resistance values in terms of stress range shall be applied and no fatigue limit or knee point of the S-N curve shall be considered. In fracture mechanics crack propagation calculations the constant C0 in the Paris power law shall be multiplied by a factor of 3.0. A threshold ΔΚ value shall not be considered. No further speciﬁc recommendations are given for corrosion fatigue assessment. If no service experience is available, monitoring of the structure in service is recommended. 3.6 Fatigue Resistance Assessed on the Basis of Crack Propagation Analysis 3.6 73 Fatigue Resistance Assessed on the Basis of Crack Propagation Analysis The resistance of a material against cyclic crack propagation is characterized by the material parameters of the “Paris” power law of crack propagation da ¼ C0 DK m dN where C0 m ΔK ΔKth R DK\Kth if else da ¼0 dN ð3:8Þ the material parameters are Constant of the power law Exponent of the power law Range of cyclic stress intensity factor Threshold value of stress intensity, under which no crack propagation is assumed Kmin/Kmax, taking all stresses including residual stresses into account (see Sect. 3.5.1) In the absence of speciﬁed or measured material parameters, the values given below are recommended. They are characteristic values. For elevated temperatures other than room temperature or for metallic materials other than steel, the crack propagation parameters vary with the modulus of elasticity E and may be determined accordingly. C ¼ C0; steel DKth ¼ DKth; steel 3.6.1 Esteel m E E Esteel ð3:9Þ ð3:10Þ Steel See Table 3.15 Table 3.15 Parameters of the Paris power law and threshold data for steel Units K [N · mm−3/2] da/dN [mm/cycle] K [MPa√m] da/dN [m/cycle] Paris power law parameters Threshold values ΔKth R ≥ 0.5 0 ≤ R≤0.5 R < 0 C0 = 5.21 · 10−13 m = 3.0 C0 = 1.65 · 10−11 m = 3.0 63 2.0 170– 214 · R 5.4– 6.8 · R Surface crack depth < 1 mm 170 ≤63 5.4 ≤2.0 74 3.6.2 3 Fatigue Resistance Aluminium See Table 3.16 Table 3.16 Parameters of the Paris power law and threshold data for aluminium Units K [N · mm−3/2] da/dN [mm/cycle] K [MPa√m] da/dN [m/cycle] 3.6.3 Paris power law parameters Threshold values ΔKth R ≥ 0.5 0 ≤ R≤0.5 R < 0 C0 = 1.41 · 10−11 m = 3.0 C0 = 4.46 · 10−10 m = 3.0 21 0.7 56.7– 72.3 · R 1.8– 2.3 · R Surface crack depth < 1 mm 56.7 ≤21 1.8 ≤0.7 Correlation of Fracture Mechanics to Other Veriﬁcation Methods The biggest portion of service life of welded joints is spent in crack propagation. So, estimates of fatigue life or the fatigue class FAT can be made by fracture mechanics calculations using appropriate parameters. The calculations should be veriﬁed at known structural details. A possible example of a set of parameters could be: ai = 0.1 mm Initial crack size parameter (ﬁtted value) ai:ci = 1 Initial aspect ratio (at butt welds ground flush ai:ci = 0.1) af = min(t/2; 12.5 mm) Final crack size parameter (t is wall thickness) r = t/25 Toe radius for most cases θ = 45° Weld angle for most cases, 30° for butt welds m = 3.0 Exponent of the Paris-Erdogan power law At cruciform joints or butt welds with partial penetration, the one half of the root gap shall be taken as the initial crack size parameter. Since the existence of a high stress concentration at the root gaps and a rapid growth in “c”-direction, a through-going crack or at least an initial aspect ratio ai:ci = 0.1 may be assumed and a two-dimensional analysis may be adequate. At butt welds ground flush, the point of a possible crack initiation may be located in the weld metal. Thus the constant for weld metal shall be taken, and ai: ci = 0.1 is recommended. For material parameters see Table 3.17. Misalignment shall be considered either in determination of the stress distribution by ﬁnite element analysis or by modiﬁcation of the results of fracture mechanics calculations. See chapter 3.8.2. 3.7 Fatigue Resistance Determination by Testing 75 Table 3.17 Constants Co of the power law for correlation (units in N and mm) Steel Aluminium 3.7 3.7.1 Weld metal (root cracks) Weld toes (base metal) 5.21 · 10−13 1.41 · 10−10 3.00 · 10−13 0.81 · 10−10 Fatigue Resistance Determination by Testing General Considerations Fatigue tests may be used to establish a fatigue resistance curve for a component or a structural detail, or the resistance of a material against (non critical) cyclic crack propagation. It is recommended that test results are obtained at constant stress ratios R. The S-N data should be presented in a graph showing log(endurance in cycles) as the abscissa and log(range of fatigue actions) as the ordinate. For crack propagation data, the log(stress intensity factor range) should be the abscissa and the log(crack propagation rate) the ordinate. Experimental fatigue data are scattered, with the extent of scatter tending to be greatest in the low stress/low crack propagation regime (e.g. see Fig. 3.12). For statistical evaluation, a Gaussian log-normal distribution should be assumed. If possible, at least 10 specimens should be tested. Many methods of statistical evaluation are available. However, the most common approach for analysing fatigue data is to ﬁt S-N or crack propagation curves by regression analysis, taking log(N) or log(da/dN) as the dependent variable. Test results should be analysed to produce characteristic values (subscript k). These are values that represent 95 % survival probability (i.e. 5 % failure probability) calculated from the mean on the basis of a two-sided conﬁdence of 75 %. More details on the use of the conﬁdence level and formulae are given below. Fig. 3.12 Scatter band in S-N curve 76 3 Fatigue Resistance At higher test cycles than about two or ten million cycles, the staircase method is recommended for testing and evaluation [70]. For a combined evaluation of failed and run-out specimens, maximum likelihood method is recommmended [71]. 3.7.2 Evaluation of Test Data Different methods for fatigue testing exist. For the derivation of S-N curves, testing at two stress range levels (Δσ) to give fatigue lives within the range of 5 × 104 to 106 cycles is preferred. For obtaining fracture mechanics crack propagation parameters, the range of stress intensity factor (ΔK) should be varied between the threshold and the critical level for fracture. For the evaluation of test data originating from a test series, the characteristic values are calculated by the following procedure: (a) Calculate log10 of all data: Stress range Δσ and number of cycles N, or stress intensity factor range ΔK and crack propagation rate da/dN. (b) Calculate exponents m and constant logC (or logC0 respectively) of the formulae: for S - N curve logN ¼ logC m logDr ð3:11Þ da ð3:12Þ ¼ logC0 þ m logDK for crack propagation log dN by linear regression taking stress or stress intensity factor range as the independent variable, i.e. logN = f(log Δσ) or log(da/dN) = f(log ΔK). The number and the spread of the data pairs should be critically assessed. If the number of pairs of test data n < 10, or if the data are not sufﬁciently evenly distributed to determine m accurately, a ﬁxed value of m should be taken, as derived from other tests under comparable conditions, e.g. m = 3 for steel and aluminium welded joints at stiff and thick-walled components. In all cases, the standard deviation of the exponent m shall be determined for a subsequent check if the pre-ﬁxed exponent, e.g. m = 3, is still reasonable. For other conditions other slopes might be also adequate. Values xi equal to logC or logC0 are calculated from the (N, Δσ)i or (da/dN, ΔK)i test results using the above equations. (c) Calculate mean xm and the standard deviation Stdv of logC (or logC0 respectively) using m obtained in b). P xm ¼ n xi sﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ P ðxm xi Þ2 Stdv ¼ n1 d) Calculate the characteristic values xk by the formulae The values of k are given in Table 3.18. ð3:13Þ 3.7 Fatigue Resistance Determination by Testing 77 Table 3.18 Values of k for the calculation of characteristic values 6 n 8 10 15 20 30 50 100 k 2.32 2.23 2.17 2.07 2.01 1.95 1.88 1.81 Note: In several areas of applications, the codes refer to mean minus two standard deviations, which corresponds to a survival probability of 97.7 %. Referring to survival probability of 95 % at two-sided conﬁdence level of the mean of 75 % (one-sided 87.5 %, sometimes also 95 %) and considering the usual scatter of fatigue tests as shown in Fig. 3.12, the difference in terms of stress is less than 2 % and thus may be neglected. The method proposed above is equal to about mean minus two standard deviations at about 20 specimens. S N data : Crack propagation rate : Values of k : xk ¼ xm k Stdv ð3:14Þ xk ¼ xm þ k Stdv 1 k ¼ 1:645 1 þ pﬃﬃﬃ n ð3:15Þ ð3:16Þ For more details and information, see Appendix 6.4 and Refs. [68–72, 75]. In the case of S-N data, proper account should be taken of the fact that residual stresses are usually low in small-scale specimens. The results should be corrected to allow for the greater effects of residual stresses in real components and structures. Examples of ways to achieve this are by testing at high R values, e.g. R = 0.5, or by testing at R = 0 and lowering the fatigue strength at 2 million cycles (FAT) by 20 %. 3.7.3 Evaluation of Data Collections Usually data collections do not originate from a single statistical population. These heterogeneous populations of data require a special consideration in order to avoid problems arising from the wide scatter. The evaluation procedure should consist of the following steps: 1. Calculate the constant log C of the S-N Wöhler curve for each data point (see Sect. 3.7.2.) using anticipated knowledge of the slope exponent from comparable test series, e.g. slope m = 3.00 for steel or aluminium. 2. Plot all values log C in a Gaussian probability chart, showing the values of log C on the abscissa and the cumulative survival probability on the ordinate. 3. Check the probability plot for heterogeneity of the population. If it is not heterogeneous, separate the portion of the population which is of interest (see illustration on Figs. 3.13 and 3.14). 4. Evaluate the interesting portion of population according to Sect. 3.7.2., which is the portion of the lowest values of log C. 78 Fig. 3.13 Example of scatter in data collections Fig. 3.14 Example of a heterogeneous population 3 Fatigue Resistance 3.8 Fatigue Resistance of Joints with Weld Imperfections 3.8 79 Fatigue Resistance of Joints with Weld Imperfections 3.8.1 General 3.8.1.1 Types of Imperfections The types of imperfections covered in this document are listed below. Other imperfections, not yet covered, may be assessed by assuming similar imperfections with comparable notch effect. Deﬁnitions are given in Ref. [48–50]. Imperfect shape All types of misalignment including centre-line mismatch (linear misalignment) and angular misalignment (angular distortion, rooﬁng, peaking). Undercut Volumetric discontinuities Gas pores and cavities of any shape. Solid inclusions, such as isolated slag, slag lines, flux, oxides and metallic inclusions. Planar discontinuities All types of cracks or crack-like imperfections, such as lack of fusion or lack of penetration (Note that for certain structural details intentional lack of penetration is already covered, e.g. partial penetration butt welds or ﬁllet welded cruciform joints. If a volumetric discontinuity is surface breaking or near the surface, or if there is any doubt about the type of an embedded discontinuity, it shall be assessed like a planar discontinuity. 3.8.1.2 Effects and Assessment of Imperfections Three effects of geometrical imperfections can be distinguished, as summarized in Table 3.19. Increase of general stress level This is the effect of all types of misalignment due to secondary bending. The additional stress magniﬁcation factor can be calculated by appropriate formulae. The fatigue resistance of the structural detail under consideration is to be lowered by division by this factor. Local notch effect Here, interaction with other notches present in the welded joint is decisive. Two cases are to be distinguished: Additive notch effect If the location of the notch due to the weld imperfection coincides with a structural discontinuity associated with the geometry of the weld shape (e.g. weld 80 3 Fatigue Resistance Table 3.19 Categorization and assessment procedure for weld imperfections Effect of imperfection Type of imperfection Assessment Increase of general stress level Misalignment Local notch effect Weld shape imperfections, undercut Porosity and inclusions not near the surface Cracks, lack of fusion and penetration, all types of imperfections other than given here Formulae for stress magniﬁcation factors Tables given Tables given additive competitive Crack-like imperfection Fracture mechanics toe), then the fatigue resistance of the welded joint is decreased by the additive notch effect. This may be the case at weld shape imperfections. Competitive notch effect If the location of the notch due to the weld imperfection does not coincide with a structural geometry associated with the shape geometry of the weld, the notches are in competition. Both notches are assessed separately. The notch giving the lowest fatigue resistance is governing. Crack-like imperfections Planar discontinuities, such as cracks or crack-like imperfections, which require only a short period for crack initiation, are assessed using fracture mechanics on the basis that their fatigue lives consist entirely of crack propagation. After inspection and detection of a weld imperfection, the ﬁrst step of the assessment procedure is to determine the type and the effect of the imperfection as given here. If a weld imperfection cannot be clearly identiﬁed as a type or an effect of the types listed here, it is recommended that it is assumed to be crack-like [54, 57]. 3.8.2 Misalignment Misalignment in axially loaded joints leads to an increase of stress in the welded joint due to the occurrence of secondary shell bending stresses [55, 56]. The resulting stress is calculated by stress analysis or by using the formulae for the stress magniﬁcation factor km given in Table (3.20) and in Appendix 6.3. Secondary shell bending stresses do not occur in continuous welds longitudinally loaded or in joints loaded in pure bending, and so misalignment will not reduce the fatigue resistance. However, misalignment in components, e.g. beams, subject to overall bending may cause secondary bending stresses in parts of the component, where the through-thickness stress gradient is small, e.g. in the flange of a beam, where the stress is effectively axial. Such cases should be assessed. 3.8 Fatigue Resistance of Joints with Weld Imperfections 81 Table 3.20 Consideration of stress magniﬁcation factors due to misalignment Type of km analysis Nominal stress approach Structural hot spot, effective notch and fracture mechanics appoach Type of welded joint km already covered in FAT class 1.15 km already covered in SN curves 1.05 Default value of effective km to be considered in stress 1.10* Butt joint made in shop in flat position Other butt joints 1.30 1.05 1.25* Cruciform joints 1.45 1.05 1.40* Fillet welds on one 1.25 1.05 1.20** plate surface Fillet welds on both 1.25 1.05 1.10*** plate surfaces * but not more than (1 + 2.5 · emax/t), where emax = permissible misalignment and t = wall thickness of loaded plate ** but not more than (1 + 0.2 · tref/t), where tref = reference wall thickness of fatigue resistance curves *** but not more than (1 + 0.1 · tref/t), where tref = reference wall thickness of fatigue resistance curves Some allowance for misalignment is already included in the tables of classiﬁed structural details (3.2). In particular, the data for transverse butt welds are directly applicable for misalignment which results in an increase of stress up to 30 %, while for the cruciform joints the increase can be up to 45 %. In the case of the structural hot spot stress and the effective notch stress assessment methods, a small but inevitable amount of misalignment corresponding to a stress magniﬁcation factor of km = 1.05 is already included in the fatigue resistance S-N curves (Table 3.20). Additional requirements apply for the joints listed in Table 3.20. The effect of a larger misalignment has to be additionally considered in the local stress (structural hot spot stress or effective notch stress). The misalignment effect may be present even in the vicinity of supporting structures. A corresponding stress increase must be taken into account also in crack propagation analyses. In all those cases where the stress magniﬁcation factor is calculated directly, use is made of an effective stress magniﬁcation factor km,eff. km; eff ¼ km; calculated km; alreadycovered ð3:17Þ For joints containing both linear and angular misalignment, both stress magniﬁcation factors should be applied using the formula: km ¼ 1 þ ðkm; axial 1Þ þ ðkm; angular 1Þ ð3:18Þ Since misalignment reduces the fatigue resistance, either the calculated applied stress is multiplied by km,eff or the allowable stress range obtained from the relevant resistance S-N curve is divided by km,eff. Table 3.20 tabulates the factors km which are already covered in the different veriﬁcation methods. Actual or speciﬁed fabrication tolerances may be assessed by the formulae given in Sect. 6.3. 82 3.8.3 3 Fatigue Resistance Undercut The basis for the assessment of undercut is the ratio u/t, i.e. depth of undercut to plate thickness. Though undercut is an additive notch, it is already considered to a limited extent in the tables of fatigue resistance of classiﬁed structural details (Sect. 3.2). Undercut does not reduce the fatigue resistance of welds which are only loaded in the longitudinal direction, i.e. parallel to the undercut. 3.8.3.1 Steel See Table 3.21 Table 3.21 Acceptance levels for weld toe undercut in steel Fatigue class Allowable undercut u/t Butt welds Fillet welds 100 0.025 Not applicable 90 0.05 Not applicable 80 0.075 0.05 71 0.10 0.075 63 0.10 0.10 56 and lower 0.10 0.10 Notes a Undercut deeper than 1 mm shall be assessed as a crack-like imperfection b The table is only applicable for plate thicknesses from 10–20 mm 3.8.3.2 Aluminium See Table 3.22 Table 3.22 Acceptance levels for weld toe undercut in aluminium Fatigue class Allowable undercut u/t Butt welds Fillet welds 50 0.025 Not applicable 45 0.05 Not applicable 40 0.075 0.05 36 0.10 0.075 32 0.10 0.10 28 and lower 0.10 0.10 Notes a Undercut deeper than 1 mm shall be assessed as a crack-like imperfection b The table is only applicable for plate thicknesses from 10–20 mm 3.8 Fatigue Resistance of Joints with Weld Imperfections 3.8.4 83 Porosity and Inclusions Embedded volumetric discontinuities, such as porosity and inclusions, are considered as competitive weld imperfections which can provide alternative sites for fatigue crack initiation to those covered by the fatigue resistance tables of classiﬁed structural details (Sect. 3.2). Before assessing the imperfections with respect to fatigue, it should be veriﬁed that the conditions apply for competitive notches, i.e. that the anticipated sites of crack initiation in the fatigue resistance tables do not coincide with the porosity or inclusions to be assessed and that there is no interaction between them. It is important to ensure that there is no interaction between multiple weld imperfections, be they of the same or different type. Combined porosity or inclusions shall be treated as a single large imperfection. The defect interaction criteria given in Sect. 3.8.5 for the assessment of cracks also apply for adjacent inclusions. Worm holes shall be assessed as slag inclusions. If there is any doubt about the coalescence of porosity or inclusions in the wall thickness direction or about the distance from the surface, the imperfections shall be assessed as cracks. It must be veriﬁed by NDT that the porosity or inclusions are embedded and volumetric. If there is any doubt, they are to be treated as cracks. The parameter for assessing porosity is the maximum percentage of projected area of porosity in the radiograph; for inclusions, it is the maximum length. Directly adjacent inclusions are regarded as a single one. 3.8.4.1 Steel See Table 3.23 Table 3.23 Acceptance levels for porosity and inclusions in welds in steel Fatigue class Max. length of an inclusion in mm As-welded Stress relieved + Limits of porosity in % of area * ** 100 1.5 7.5 3 90 2.5 19 3 80 4 58 3 71 10 no limit 5 63 35 no limit 5 56 and lower no limit no limit 5 * Area of radiograph used is length of weld affected by porosity multiplied by width of weld ** Maximum pore diameter or width of an inclusion less than 1/4 plate thickness or 6 mm + Stress relieved by post weld heat treatment 84 3 Fatigue Resistance Table 3.24 Acceptance levels for porosity and inclusions in welds in aluminium Fatigue class Max. length of an inclusion in mm ** As-welded Limits of porosity in % of area * ** 40 and 1.5 0 +) higher 36 2.5 3 32 4 3 28 10 5 25 35 5 15 and lower no limit 5 * Area of radiograph used is length of weld affected by porosity multiplied by width of weld ** Maximum pore diameter or width of an inclusion less than ¼ plate thickness or 6 mm + Single pores up to 1.5 mm allowed 3.8.4.2 Aluminium Tungsten inclusions have no effect on fatigue behaviour and therefore do not need to be assessed (Table 3.24). 3.8.5 Crack-like Imperfections 3.8.5.1 General Procedure Planar discontinuities, cracks or crack-like defects are identiﬁed by non-destructive testing and inspection. NDT indications are idealized as elliptical cracks (Fig. 3.15) for which the stress intensity factor is calculated according to Sect. 2.2.5. For embedded cracks, the shape is idealized by a circumscribing ellipse, which is measured by its two half-axes a and c. The crack parameter a (crack depth) is the half-axis of the ellipse in the direction of the crack growth to be assessed. The remaining perpendicular half-axis is the half length of the crack c. The wall thickness parameter t is the distance from the centre of the ellipse to the nearest surface (Fig. 3.16). If a/t > 0.75, the defect should be re-categorized as a surface crack. Surface cracks are described in terms of a circumscribing half-ellipse. The thickness parameter is wall thickness t. If a/t > 0.75, the defect is regarded as being fully penetrating and is to be re-categorized as a centre crack or an edge crack, whichever is applicable. For details of dimensions of cracks and re-categorization see Appendix 6.2. 3.8 Fatigue Resistance of Joints with Weld Imperfections 85 Fig. 3.15 Transformation of NDT indications into elliptic or semi-elliptic cracks Fig. 3.16 Crack dimensions for assessment 3.8.5.2 Simpliﬁed Procedure The simpliﬁed procedure makes use of the fatigue resistance at 2 · 106 cycles (analogous to FAT classes for the classiﬁed structural details) for ranges of crack types, sizes and shapes, of which the data are presented in Tables 3.25. These were obtained by integration of the crack propagation law for steel, given in Sect. 3.6.1, between the limits of an initial crack size ai and a ﬁnal crack size of 50 % of the wall thickness. In addition, use was made of the correction functions and the local weld geometry correction given in Sect. 6.2.4. (See Tables 6.1 and 6.3, also 6.14). In assessing a defect by the simpliﬁed procedure, the stress range Δσi corresponding to the initial crack size parameter ai and the stress range Δσc for the critical crack size parameter ac are identiﬁed. The stress range Δσ or the FAT class corresponding to a crack propagation from ai to ac in 2 · 106 cycles is then calculated by: Dr ¼ qﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ 3 Dr3i Dr3c ð3:19Þ The tables may be used for aluminium by dividing the resistance stress ranges at 2 · 106 cycles (FAT classes) for steel by 3. The tables have been calculated using Ref. [40, 42] with a constant of Co = 5.21e-13 [N; mm] and an exponent of m = 3.0 in order to cover the worst case under normal operation and environmental conditions. Corrosion is not considered. A possible misalignment has to be considered explicitly according to Table 3.20. Note: The different deﬁnition of t for surface and embedded cracks in Table 3.25 shall be considered according to Fig. 3.16. 86 3 Fatigue Resistance Table 3.25 Stress ranges at 2 · 106 cycles (FAT classes in N/mm2) of welds containing cracks for the simpliﬁed procedure (following 3 pages) Long crack at ﬁllet weld toe, L/t = 2.5, a:c = 0.1 a\ t 5 6 8 10 12 14 16 20 25 30 35 40 50 25 0 0 0 0 0 0 0 0 0 0 0 8 12 100 22 20 0 0 0 0 0 0 0 0 0 7 11 13 17 26 16 0 0 0 0 0 0 0 0 9 12 15 17 21 29 12 0 0 0 0 0 0 0 10 15 18 21 23 26 34 10 0 0 0 0 0 0 10 15 19 22 24 26 29 36 8 0 0 0 0 8 12 15 19 23 26 28 30 33 39 6 0 0 0 12 16 19 22 26 29 32 34 35 38 42 5 0 0 11 16 20 23 26 29 33 35 37 38 40 44 4 0 10 17 22 26 28 31 34 37 39 41 42 44 46 3 13 18 24 29 32 35 37 40 42 44 45 46 47 48 2 25 29 35 38 41 43 45 47 49 50 51 51 52 51 1 44 47 51 53 55 56 57 58 58 58 58 58 57 55 0.5 61 62 64 65 65 66 66 65 65 64 64 63 62 58 0.2 77 77 77 76 75 74 74 72 71 69 68 67 66 60 0.1 85 85 83 81 80 79 78 76 74 72 71 69 67 61 Short crack at ﬁllet weld toe, L/t = 2.5, a:c = 0.5 a\ t 5 6 8 10 12 14 16 20 25 30 35 40 50 100 25 0 0 0 0 0 0 0 0 0 0 0 17 22 31 20 0 0 0 0 0 0 0 0 0 15 20 23 27 35 16 0 0 0 0 0 0 0 0 17 22 26 28 31 37 12 0 0 0 0 0 0 0 20 26 29 32 34 36 41 10 0 0 0 0 0 0 19 26 30 33 35 37 39 43 8 0 0 0 0 17 23 27 31 35 37 39 40 42 45 6 0 0 0 23 28 32 34 38 41 42 44 45 46 48 5 0 0 22 29 33 36 38 41 44 45 46 47 48 50 4 0 19 30 35 39 41 43 45 47 48 49 50 51 52 3 26 32 38 42 45 47 48 50 51 52 53 53 54 54 2 40 44 48 51 53 54 55 56 57 57 58 58 58 56 1 58 60 62 63 64 65 65 65 66 65 64 64 63 58 0.5 72 73 74 74 74 74 73 72 71 69 68 67 65 60 0.2 86 86 84 82 81 80 78 76 74 72 71 70 68 61 0.1 93 91 88 86 84 82 81 78 76 74 72 71 69 62 (continued) 3.8 Fatigue Resistance of Joints with Weld Imperfections 87 Table 3.25 (continued) Long crack at butt weld toe, L/t = 1, a:c = 0.1 a\ t 5 25 20 0 6 8 10 12 14 16 20 25 30 35 40 50 0 0 0 0 0 0 0 0 0 0 8 12 100 22 0 0 0 0 0 0 0 0 7 11 13 17 26 16 0 0 0 0 0 0 0 0 9 12 15 17 21 29 12 0 0 0 0 0 0 0 10 15 18 21 23 26 33 10 0 0 0 0 0 0 10 15 19 22 24 26 29 36 8 0 0 0 0 8 12 15 19 23 26 28 30 33 39 6 0 0 0 12 16 19 22 26 29 32 34 35 38 42 5 0 0 11 16 20 23 26 29 33 35 37 38 40 44 4 0 10 17 22 26 28 31 34 37 39 41 42 44 46 3 13 18 24 29 32 35 37 40 42 44 45 46 47 49 2 25 29 35 38 41 43 45 47 49 50 51 51 52 52 1 44 47 51 53 55 56 57 58 59 59 59 59 58 56 0.5 61 63 65 66 66 66 66 66 65 65 64 64 63 58 0.2 77 78 77 77 76 75 75 73 72 70 69 68 67 61 0.1 86 85 84 83 81 80 79 77 75 73 72 71 68 62 Short crack at butt weld toe, L/t = 1, a:c = 0.5 a\ t 5 6 8 10 12 14 16 20 25 30 35 40 50 100 25 0 0 0 0 0 0 0 0 0 0 0 16 22 31 20 0 0 0 0 0 0 0 0 0 15 20 23 27 34 16 0 0 0 0 0 0 0 0 17 22 25 28 31 37 12 0 0 0 0 0 0 0 20 26 29 31 33 36 41 10 0 0 0 0 0 0 19 26 30 33 35 37 39 43 8 0 0 0 0 17 23 26 31 35 37 39 40 42 45 6 0 0 0 23 28 31 34 37 40 42 43 44 46 48 5 0 0 22 29 33 36 38 41 43 45 46 47 48 50 4 0 19 30 35 38 41 43 45 47 48 49 50 51 52 3 26 31 38 42 45 47 48 50 51 52 53 53 54 54 2 40 43 48 51 53 54 55 56 57 57 58 58 58 56 1 58 60 62 63 64 65 65 65 66 66 65 64 63 59 0.5 72 73 74 74 75 74 74 73 71 70 69 68 66 61 0.2 86 86 85 83 82 81 79 77 75 74 72 71 69 62 0.1 94 92 89 87 85 84 82 80 77 75 74 72 70 63 (continued) 88 3 Fatigue Resistance Table 3.25 (continued) Long surface crack at weld ground flush to surface, a:c = 0.1 a\ t 5 6 8 10 12 14 16 20 25 30 35 40 50 100 25.0 0 0 0 0 0 0 0 0 0 0 0 8 13 23 20.0 0 0 0 0 0 0 0 0 0 7 11 13 17 26 16.0 0 0 0 0 0 0 0 0 9 12 15 17 21 30 12.0 0 0 0 0 0 0 0 10 15 18 21 23 26 34 10.0 0 0 0 0 0 0 10 15 19 22 24 26 29 37 8.0 0 0 0 0 8 12 15 20 23 26 29 30 33 41 6.0 0 0 0 12 16 19 22 26 29 32 34 36 38 45 5.0 0 0 11 16 20 23 26 30 33 36 38 39 42 48 4.0 0 10 17 22 26 28 31 34 38 40 42 43 46 52 3.0 13 18 25 29 32 35 37 40 43 45 47 49 51 56 2.0 25 29 35 39 42 44 46 49 51 53 55 56 58 63 1.0 44 47 52 55 58 59 61 63 66 67 68 69 71 74 0.5 63 65 69 72 74 75 77 78 80 81 82 83 84 86 0.2 87 89 91 93 95 96 96 98 99 99 100 101 101 103 0.1 105 106 109 110 111 112 112 113 114 115 115 115 116 117 Short surface crack at weld ground flush to surface, a:c = 0.5 a\ t 5 6 8 10 12 14 16 20 25 30 35 40 50 100 25 0 0 0 0 0 0 0 0 0 0 0 17 23 95 20 0 0 0 0 0 0 0 0 0 15 20 24 29 39 16 0 0 0 0 0 0 0 0 17 23 27 30 34 43 12 0 0 0 0 0 0 0 21 27 31 35 37 40 48 10 0 0 0 0 0 0 20 27 32 36 39 41 44 51 8 0 0 0 0 17 24 28 34 38 42 44 46 49 55 6 0 0 0 23 29 34 37 41 45 48 50 52 54 59 5 0 0 22 30 35 39 42 46 50 52 54 55 58 62 4 0 20 31 38 42 45 48 52 55 57 58 60 62 66 3 27 33 41 47 50 53 55 58 61 63 64 65 67 71 2 43 48 54 58 61 63 65 67 69 71 72 73 74 77 1 66 69 73 76 78 79 80 82 84 85 86 86 87 90 0.5 86 88 91 93 94 95 96 98 99 99 100 100 101 103 0.2 111 112 114 115 116 117 117 118 119 119 120 120 121 122 0.1 129 130 132 133 133 134 134 135 136 136 136 137 137 138 (continued) 3.8 Fatigue Resistance of Joints with Weld Imperfections 89 Table 3.25 (continued) Long embedded crack, t = distance to nearest surface, a:c = 0.1 a\ t 3 4 5 6 8 10 12 14 16 20 25 30 35 40 50 25 0 0 0 0 0 0 0 0 0 0 0 0 0 4 7 20 0 0 0 0 0 0 0 0 0 0 0 3 5 7 11 16 0 0 0 0 0 0 0 0 0 0 4 6 9 11 14 12 0 0 0 0 0 0 0 0 0 5 8 11 14 16 19 10 0 0 0 0 0 0 0 0 4 8 12 15 17 19 23 8 0 0 0 0 0 0 3 6 8 12 16 19 22 24 27 6 0 0 0 0 0 5 9 12 14 18 22 25 27 29 32 5 0 0 0 0 5 9 12 15 18 22 26 28 31 32 35 4 0 0 0 4 9 14 17 20 23 26 30 33 35 37 39 3 0 0 6 10 16 20 24 27 29 32 36 38 40 42 45 2 4 10 15 19 25 30 33 36 38 41 44 46 48 50 52 1 22 29 33 37 42 46 49 51 53 56 59 61 63 64 67 0.5 42 47 52 55 60 63 66 68 69 72 75 77 79 80 82 0.2 68 73 77 80 84 87 90 92 93 96 98 100 101 103 105 0.1 90 94 98 101 105 107 110 111 113 115 117 119 120 122 124 Short embedded crack, t = distance to nearest surface, a:c = 0.5 a\ t 3 4 5 6 8 10 12 14 16 20 25 30 35 40 50 25 0 0 0 0 0 0 0 0 0 0 0 0 0 5 10 20 0 0 0 0 0 0 0 0 0 0 0 4 7 10 14 16 0 0 0 0 0 0 0 0 0 0 5 9 12 15 19 12 0 0 0 0 0 0 0 0 0 7 12 15 19 21 26 10 0 0 0 0 0 0 0 0 6 11 16 20 23 26 30 8 0 0 0 0 0 0 5 9 12 17 21 25 28 31 35 6 0 0 0 0 0 8 12 16 19 24 29 32 35 38 42 5 0 0 0 0 7 12 17 21 24 29 33 37 40 42 46 4 0 0 0 6 13 19 23 27 30 35 39 43 45 48 51 3 0 0 9 14 21 27 31 35 38 42 47 50 53 55 58 2 6 15 21 26 33 39 43 46 49 54 58 61 63 65 68 1 29 37 44 48 55 60 64 67 69 73 76 79 81 82 85 0.5 54 62 67 72 78 82 85 87 89 92 95 97 99 100 102 0.2 89 95 99 103 107 111 113 115 116 119 121 123 124 125 127 0.1 115 121 124 127 131 133 135 137 138 140 142 144 145 146 148 Chapter 4 Fatigue Assessment 4.1 General Principles In a fatigue assessment, the fatigue actions and the fatigue resistance are related by means of an appropriate assessment procedure. It must be ensured that all three elements (actions, resistance and assessment procedure) correspond. Three procedures may be distinguished: (a) Procedures based on S-N curves, such as – Nominal stress approach – Structural hot spot stress approach – Effective notch stress approach (b) Procedures based on fatigue crack propagation considerations (c) Direct experimental approach by the fatigue testing of components or entire structures. 4.2 Combination of Normal and Shear Stress If normal and shear stresses occur simultaneously, their combined effect shall be considered. Three cases may be distinguished: (a) If the nominal shear stress range is less than 15 % of the normal stress range or if the fatigue damage sum due to the shear stress range is lower than 10 % of that due to the normal stress range, the effect of shear stress may be neglected. (b) If the normal and shear stresses vary simultaneously in-phase, or if the plane of maximum principal stress does not change signiﬁcantly (<20°) during cycling, the maximum principal stress range should be used, otherwise the procedure as given in Sect. 4.3.1 is recommended. © Springer International Publishing Switzerland 2016 A.F. Hobbacher, Recommendations for Fatigue Design of Welded Joints and Components, IIW Collection, DOI 10.1007/978-3-319-23757-2_4 91 92 4 Fatigue Assessment (c) If the normal and shear stresses vary independently out-of-phase (i.e. non-proportional loading), the procedure given in Sect. 4.3.1 is recommended. Fracture mechanics fatigue crack propagation calculations should be based on the maximum principal stress range. 4.3 Fatigue Assessment Using S-N Curves The fatigue assessment is carried out using The design stress or spectrum of fatigue actions in terms of stress ranges Δσi,S,d, in which the stresses of the characteristic spectrum Δσi,S,k have been multiplied by the partial safety factor γF for fatigue actions. and The design resistance Wöhler S-N curve based on design resistance stresses ΔσR, in which the characteristic resistance stress range ΔσR,k has been divided by the partial safety factor γM for fatigue resistance. d, The characteristic resistance S-N curve is derived from an appropriate fatigue class FAT, which may be modiﬁed further according to stress ratio, wall thickness, post weld improvement etc., and to the requirements of the damage calculation procedure. Two types of veriﬁcation are distinguished, a veriﬁcation in terms of cycles and a veriﬁcation in terms of stress. Veriﬁcation in Terms of Cycles: An action as a constant amplitude design stress ΔσS,d a stress spectrum or a constant amplitude equivalent stress representing the spectrum Δσeq,S,d is given on the load side and a modiﬁed design fatigue resistance class FATd (ΔσR,d) is given on the resistance side. From both, the number of life cycles may be calculated as: Ncalc DrR;d m ¼ 2 10 or resp: DrS;d 6 Ncalc DrR;d ¼ 2 10 Dreq;S;d m 6 ð4:1Þ Ncalc Nspec where DrS;d design value of the constant amplitude stress range Dreq;S;d design value of an equivalent stress range, derived from a given load spectrum, which characterizes the loading, and a cumulative damage calculation DrR;d design value of the fatigue resistance at 2·106 cycles derived from the modiﬁed fatigue class FAT of the structural detail 4.3 Fatigue Assessment Using S-N Curves Ncalc Nspec 93 calculated number of life cycles speciﬁed number of life cycles Veriﬁcation in Terms of Stress: For constant amplitude loading, the design resistance stress range ΔσR,d shall be determined at the required or speciﬁed number of stress cycles Nspec. The following fatigue criterion should then be checked: DrS; d ¼ DrS; k cF DrR; d ¼ DrR; k cM ð4:2Þ For a constant amplitude loading which produces both normal and shear stresses, the maximum principal stress Δσcomp,S,d shall be used, provided its direction is within ±60° from the normal to the weld. Drcomp;S;d ¼ pﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ 1 DrS;d þ DrS;d þ 4 DsS;d 2 ð4:3Þ Otherwise the following criterion must be met, where the comparison value CV depends on the material and type of loading. See Table 4.1. DrS;d DrR;d 2 DsS;d þ DsR;d 2 CV ð4:4Þ For variable amplitude loading, a cumulative damage calculation procedure should be applied. Usually a modiﬁed “Palmgren-Miner” rule, as described in Table 4.1 Assessment procedures for combined normal and shear stress using S-N curves Type of load Normal and shear stress Constant amplitude Proportional Assessment procedure Assessment on the basis of the maximum principal stress or DrS;d 2 DsS;d 2 þ CV DrR;d DsR;d 2 2 Un-correlated DrS;d DsS;d þ CV DrR;d DsR;d Variable Proportional Assessment on the basis of maximum amplitude principal stress and Miner’s rule, or Dreq;S;d 2 Dseq;S;d 2 þ CV DrR;d DsR;d 2 2 Un-correlated Dreq;S;d Dseq;S;d þ CV DrR;d DsR;d Note: For fluctuating mean stress, a Palmgren-Miner sum of D = 0.2 is a For semi-ductile aluminium alloys CV = 1.0 is recommended [65] Speciﬁed damage sum D or comparison value CV CV = 1.0 CV = 0.5a D = 0.5 CV = 1.0 D = 0.5 CV = 0.5a recommended 94 4 Fatigue Assessment Sect. 4.3.1, is appropriate. Relevant data associated with their resistance S-N curves (Figs. 4.1 and 4.2), that are used to apply the rule, are given in Table 4.2. For load spectra which are sensitive to the position of the constant amplitude fatigue limit (CAFL) or knee point on the S-N curve, or in which the spectrum changes during the service life, an additional assessment using fracture mechanics, as described in Sect. 4.4 is recommended referring also to Sects. 2.2.5 and 3.6. Fig. 4.1 Modiﬁed resistance S-N curves of steel for Palmgren-Miner summation Fig. 4.2 Modiﬁed resistance S-N curves of aluminium for Palmgren-Miner summation 4.3 Fatigue Assessment Using S-N Curves 95 Table 4.2 FAT data, stress range at knee point of S-N curve, constants of S-N curves and constants for constant and variable amplitude loading (Palmgren-Miner summation) Stress ranges Values of constant C: N = C/Δσm or N = C/Δτm FAT class Stress range at For stress ranges above For stress ranges below knee [MPa] knee point knee point point Welded structural details under normal stress: Δσ at 2E + 6 cycles Δσ at 1E + 7 cycles m=3 125 112 100 90 80 71 63 56 50 45 40 36 32 28 25 22 20 18 16 14 12 Base material: Δσ at 2E + 6 cycles 73.1 65.5 58.5 52.7 46.8 41.5 36.9 32.8 29.3 26.3 23.4 21.1 18.7 16.4 14.6 12.9 11.7 10.5 9.4 8.2 7.0 3.906E 2.810E 2.000E 1.458E 1.024E 7.158E 5.001E 3.512E 2.500E 1.823E 1.280E 9.331E 6.554E 4.390E 3.125E 2.130E 1.600E 1.166E 8.192E 5.488E 3.456E 12 12 12 12 12 11 11 11 11 11 11 10 10 10 10 10 10 10 09 09 09 Constant amplitude m = 22 1.014E + 48 9.064E + 46 7.541E + 45 7.583E + 44 5.564E + 43 3.954E + 42 2.983E + 41 2.235E + 40 1.867E + 39 1.734E + 38 1.327E + 37 1.362E + 36 9.561E + 34 5.328E + 33 4.128E + 32 2.710E + 31 3.163E + 30 2.925E + 29 2.563E + 28 1.270E + 27 3.910E + 25 Variable amplitude m=5 2.091E + 16 1.207E + 16 6.581E + 15 4.046E + 15 2.245E + 15 1.236E + 15 6.800E + 14 3.773E + 14 2.141E + 14 1.264E + 14 7.016E + 13 4.143E + 13 2.299E + 13 1.179E + 13 6.691E + 12 3.531E + 12 2.192E + 12 1.295E + 12 7.184E + 11 3.685E + 11 1.705E + 11 Δσ at 1E + 7 cycles m=5 160 80 71 Shear stress: Δτ at 2E + 6 cycles 116.0 58.0 51.5 2.097E + 17 6.554E + 15 3.623E + 15 Constant amplitude m = 22 2.619E + 52 6.243E + 45 4.568E + 44 Variable amplitude m=9 3.803E + 25 7.428E + 22 2.548E + 22 Δτ at 1E + 8 cycles m=5 100 80 36 28 45.7 36.6 16.5 12.8 1.993E 3.277E 1.209E 3.442E Constant amplitude m = 22 3.297E + 44 2.492E + 42 6.090E + 34 2.284E + 32 Variable amplitude m=9 8.695E + 22 1.179E + 22 9.065E + 18 9.223E + 17 + + + + + + + + + + + + + + + + + + + + + + + + + 16 15 14 13 96 4 Fatigue Assessment In any ﬁeld of application, for which there are no test data, or no service experience exists and the shape of the stress spectrum is not close to constant amplitude, the assessment procedure as detailed in Sect. 4.3.1 is recommended. Veriﬁcation in Terms of Stress at 2 million Cycles: In the 2 million cycles equivalent procedure, the equally damaging stress range at 2 million cycles ΔσS,d,E2 is determined. It can be directly compared with the factored and modiﬁed fatigue class FAT. DrS;d;E2 FAT=cM ð4:5Þ The 2 million cycles equivalent ΔσS,d,E2 for constant amplitude fatigue action is calculated by sﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ m m n Dr S;d DrS;d;E2 ¼ ð4:6Þ 2 106 where n is the speciﬁed number of cycles corresponding to the total anticipated load history of the joint and ΔσS,d is the design stress range of the fatigue action. 4.3.1 Linear Damage Calculation by the “Palmgren-Miner” Rule First, the required number of cycles shall be speciﬁed, and the design resistance S-N curve shall be determined. If a fatigue limit is considered and if the maximum design stress range Δσmax,S,d in the load spectrum is lower than the assumed design fatigue limit ΔσL,R,d for the design fatigue resistance S-N curve, the life of the welded joint can be assumed to be inﬁnite and no further damage calculation is necessary. However, this procedure is not recommended for aluminium or for steels required to survive for very high numbers of load cycles (see Sect. 3.2) and [64, 66]. For other situations, the assumed constant amplitude fatigue limit (CAFL) or knee point is ignored. The S-N curve must be extrapolated beyond it at the shallower slope of m2 = 2 · m1-1 [62] as shown in Figs. 4.1 and 4.2. For fatigue veriﬁcation, it has to be shown that [60, 61]: Dcalc ¼ where Dcalc Dspec i ni Ni X ni Ni Dspec ¼ 0:5. . .1:0 ð4:7Þ calculated damage sum (note restrictions in Sects. 4.2 and 4.3) speciﬁed damage sum as in Table 4.1 index for block number in load spectrum of required design life number of cycles of design load stress range Δσi,S,d in load spectrum block i number of cycles to failure at design stress range Δσi,S,d obtained from the modiﬁed design fatigue resistance S-N curve. 4.3 Fatigue Assessment Using S-N Curves 97 The order of sequence of the blocks has no effect on the results of this calculation provided, that the size of the spectrum allows for about 20 repetitions in summing. It is accepted that the stresses below the assumed constant amplitude fatigue limit or below the knee point must be included in cumulative damage calculation relating to welded joints. There are currently different opinions about how this should be achieved. The method presented here (Figs. 4.1 and 4.2) appears in a number of codes. However, recent research indicates that assuming a speciﬁed damage sum or fatigue damage ratio of Dspec = 1 can be non-conservative. Here, this question is partially solved by recommending a value of Dspec = 0.5. Note: It has been observed that for spectra with high mean stress fluctuations, the damage sum may be even lower, possibly down to Dspec = 0.2. In some cases an equivalent constant amplitude stress range Δσeq,S,d may need to be determined and compared directly with the constant amplitude resistance S-N curve. Δσeq,S,d is calculated for Δσeq,S,d > ΔσL,d as follows: Dreq;S;d For Δσ eq,S,d Dreq;S;d where: Dspec Δσeq,S,d m1 m2 Δσi,S,d Δσj,S,d ΔσL,d ni nj vﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ u u 1 P ðni Drm1 Þ þ Drðm1 m2 Þ P ðnj Drm2 Þ t i;S;d j;S;d P L;d P ¼ Dspec nj ni þ m1 ð4:8aÞ < ΔσL,d: vﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ u u 1 Drðm2 m1 Þ P ðni Drm1 Þ þ P ðnj Drm2 Þ m2 t i;S;d j;S;d L;d P P ¼ Dspec nj ni þ ð4:8bÞ speciﬁed Miner sum (Dspec = 1, if values from Table 4.1 are used) design value of equivalent stress range (loads) for (Σni + Σnj) cycles slope above the knee point of the SN curve slope below the knee point of the SN curve design values of stress ranges (loads) above the knee point design values of stress ranges (loads) below the knee point design value of stress range (resistance) at the knee point of S-N curve (Table 4.2) number of cycles at applied stress range Δσi number of cycles at applied stress range Δσj For calculation of equivalent shear stress Δτeq,S,d, the same formula applies expressed in terms of the corresponding shear stress ranges. If Δσeq,S,d or Δτeq,S,d are below the knee points ΔσL,d or ΔτL,d, the corresponding constant amplitude fatigue 98 4 Fatigue Assessment lives are obtained from the S-N curves for the relevant FAT class extrapolated beyond the knee point at slope m2 (Eq. 4.8). If all stress ranges are all above or all below the knee point, the formula simpliﬁes to: all above : all below : Dreq;S;d Dreq;S;d sﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ P i Þ ðnj Drm 1 P i;S;d ¼ Dspec ni m1 vﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ u P m2 u Dr n j j;S;d t 1 P ¼ Dspec nj m2 ð4:9aÞ ð4:9bÞ The effects of combination of normal and shear stresses shall be assessed on the basis of the following criterion: Dreq;S;d 2 Dseq;S;d 2 þ CV DrR;d DsR;d ð4:10Þ where ΔσR,d and ΔτR,d are the design resistance normal and shear stress ranges derived from the speciﬁed number of cycles and the appropriate FAT class. CV is a comparison value, which is given in Table 4.1. In cases where the stresses are acting in different directions with respect to the weld, they are assessed by different methods, e.g. nominal stress, structural hot-spot stress or effective notch stress method, the veriﬁcation by the above given formulae must be performed with the fatigue resistance data for the corresponding method. In the 2 million cycles equivalent procedure, the same applied as for formula (4.8) with the difference that the equivalence is for 2 million cycles, where ni and nj refer to the total anticipated load history of the joint. Assuming the most damaging blocks or Δσeq,S,d being above the knee point of the S-N curve, then the 2 million cycles equivalent stress range ΔσS,d,E2 for constant amplitude fatigue action is calculated by DrS;d;E2 vﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ u u 1 P ðni Drm1 Þ þ Drðm1 m2 Þ P ðnj Drm2 Þ m1 t i;S;d j;S;d L;d ¼ Dspec 2 106 ð4:11Þ In cases where the most damaging blocks or Δσeq,S,d are below the knee point of the S-N curve, then calculate DrS;d;E2 vﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ u u 1 Drðm2 m1 Þ P ðni Drm1 Þ þ P ðnj Drm2 Þ m2 t i;S;d j;S;d L;d ¼ Dspec 2 106 ð4:12Þ 4.3 Fatigue Assessment Using S-N Curves 99 The assessment procedures for an interaction of fluctuating normal and shear stress are given in Table 4.1. If Table 4.1 is used for the 2 million cycles equivalent procedure, all fatigue action data are 2 million cycles equivalents. The fatigue resistance data are modiﬁed and factored fatigue class values FATmod/γM. Note: The veriﬁcation procedures for multi-axial and non-proportional loading are in development. The procedures given in Table 4.1 describe a conservative approach. In cases of special interest, the user may consult the relevant literature [67]. For the grid of fatigue resistance S-N curves with the initial slope of m = 3 predominantly used in Sect. 3.2, stepping down one class corresponds to a division of the stress range by 1.12. So, different levels of safety γM of an applied S-N curve may be considered (see Sect. 6.4.3). 4.3.2 Nonlinear Damage Calculation A nonlinear fracture mechanics damage calculation according to Sect. 4.4 is recommended in cases, where (a) The Palmgren-Miner summation is sensitive to the exact location of the knee point of the fatigue resistance S-N curve, (b) The spectrum of fatigue actions (loads) varies in service or is changed, and so the sequence of loads becomes signiﬁcant or (c) The resistance S-N curve of a pre-damaged component has to be estimated. Where the parameters for a fracture mechanics fatigue assessment are not known and only the resistance S-N curve is known, the S-N curve can be used to derive dimensionless fracture mechanics parameters, which allow a damage calculation [63]. The procedure is based on the “Paris” power law of crack propagation da ¼ C0 DK m dN but where a N ΔK ΔKth da ¼0 dN if DK [ DKth ð4:13Þ if DK DKth ð4:14Þ dimensionless crack parameter Number of cycles Stress intensity factor range Threshold stress intensity factor range below which no crack propagation is assumed C0, m material constants 100 4 Fatigue Assessment The characteristic stress intensity factor range ΔKS,k of the fatigue action is calculated with the stresses in the spectrum Δσi,S,k and the crack parameter a. DKS; k ¼ DrS; k pﬃﬃﬃ a ð4:15Þ The characteristic resistance parameters can be derived from the characteristic constant amplitude fatigue resistance S-N curve: The threshold value corresponds to the fatigue limit, ΔKth,k = ΔσL,R,k·√a, m equals the slope of the S-N curve, and the constant C0,k can be calculated from a data point (ΔσS-N and NS-N) on the S-N curve, preferably from the fatigue class at 2 · 106 cycles. C0; k ¼ 2 ðm 2Þ NSN Drm SN ð4:16Þ The fatigue assessment is carried out according to Sect. 4.4, using an initial crack parameter ai = 1 and a ﬁnal one af = ∞ or a large number e.g. af = 109. The restrictions on life cycles given in Sect. 4.3 are to be considered. The actual fatigue class FATact of a pre-damaged component thus becomes FATact. = FAT/√a. 4.4 Fatigue Assessment by Crack Propagation Calculation The fatigue action represented by the design spectrum of stress intensity factor ranges DKS; d ¼ DKS; k cF ð4:17Þ is veriﬁed by the material resistance design parameters against crack propagation C0; d ¼ C0; k cm M DKth; d ¼ ð4:18Þ Kth; k cM ð4:19Þ using the “Paris” power law da ¼ C0 DK m dN if where a Crack size N Number of cycles ΔK Stress intensity factor range DK [ DKth else da ¼0 dN ð4:20Þ 4.4 Fatigue Assessment by Crack Propagation Calculation 101 ΔKth Threshold value of stress intensity factor range below which no crack propagation is assumed C0, m material constants For applied stress intensity factors, which are high compared with the fracture toughness of the material, Kmat, an acceleration of crack propagation will occur. In these cases, the following extension of the “Paris” power law of crack propagation is recommended. In the absence of an accurate value of the fracture toughness, a conservative estimate should be made. da C0 DK m ¼ dN ð1 RÞ KDK mat ð4:21Þ where Kmat Fracture toughness of the material R Stress ratio The fatigue life N is determined by integration starting from an initial crack parameter ai to a ﬁnal one af [51–53]. The calculated number of life cycles N must be greater or equal to the required number of life cycles. The same formulae apply for a crack growth calculation in a c-direction, if that was required by the selected procedure. In general, the integration has to be carried out numerically. The increment for one cycle is Δa as given in Eq. 4.17. It is recommended that a continuous spectrum be subdivided into an adequate number of stress range blocks, e.g. 8 or 10 blocks, and that the integration be performed block-wise by summing the increments of a and the number of cycles of the blocks. The entire size of the spectrum in terms of cycles should be adjusted by multiplying the block cycles by an appropriate factor in order to ensure at least 20 loops over the whole spectrum in the integration procedure. If the sequence of loading is not known, the highest stresses in spectrum should be processed ﬁrst. m Da ¼ C0;d DKa;d 1 cycle Dc ¼ C0;d m DKc;d 1 cycle if DKa;d [ DKth;d else Da ¼ 0 if DKc;d [ DKth;d else Dc ¼ 0 ð4:22Þ When using weight functions, the integration of the power law of crack propagation has to be performed over the implicite integral of the weight function. x¼af Z N¼ x¼ai dx ¼ C0 DK m x¼af Z x¼ai C0 R x¼a x¼0 dx m Drð xÞ hðx; aÞ dx ð4:23Þ 102 4.5 4.5.1 4 Fatigue Assessment Fatigue Assessment on the Basis of Service Testing General An experimental fatigue assessment of components or structures may be required for different reasons: (a) Existence of a new design with no or insufﬁcient knowledge or experience of its fatigue behaviour. (b) Veriﬁcation of a component or structure for a speciﬁed survival probability under a special fatigue action (stress) history. (c) Optimization of design and/or fabrication with respect to weight, safety and economy after initial design. For example, the selected dimensions may be justiﬁed on the basis of higher fatigue resistance data than those presented here. Support for this might require component testing. A preliminary design may be done by assuming an about 50 % higher fatigue resistance than given by the FAT classes. Later the design has to be veriﬁed by component test. In production, an adequate quality assurance system has to be established to make sure that the quality in test and in production are always equal. In component testing, the statistical nature of fatigue must be considered. It might also be necessary to take into account differences in fabrication quality between the tested component and the actual structure. The system of quality assurance should be documented. The veriﬁcation or assessment might also depend on the safety strategy considered (see Sect. 5.2), with some distinction between safe-life, fail-safe and damage tolerant strategies. Ideally, the fatigue tests should be performed under loading conditions that represent the service fatigue action history (see Sect. 3.7), factored if necessary by the partial safety factors γF and γM (i.e., the stress levels of the action history have to be multiplied by γF γM for testing) (Table 4.3). The all failed approach is the normal way of testing a small sample of which each specimen represents the same weld details. The test data may be suitable for producing a S-N curve, in which case their statistical analysis considers only the data of the failed specimens disregarding the results from the non-failed ones. However, there are techniques for including those as well, if necessary (e.g. [75]). The ﬁrst to fail approach is usually used to save time when a large number of identical specimens are tested. The results could be used to establish a safe fatigue life for the component, but only at the level of the test. The p to fail approach is used in similar way to the “ﬁrst to fail” one. A common situation would be one, in which the test specimen contains many potential sites of fatigue cracking, and when repair of cracks allows to continue the test. Each time when a detail fails, the test is stopped and the failed detail is repaired. At the end, possibly all details have failed and thus the “all failed” approach could be applied. 4.5 Fatigue Assessment on the Basis of Service Testing 103 Table 4.3 Testing approaches No Testing procedure Approach 1 2 3 All specimens from the samples are tested to failure Testing is stopped at failure of ﬁrst specimen from the sample Testing is stopped when p specimens of the n samples have failed All failed First to fail p to fail If only p specimens out of the n possible ones failed, the “p to fail” approach may be used. This section considers the all failed and ﬁrst to fail approaches. Other approaches and details of statistical analysis are considered in Appendix 6.4. The following test result data should be documented according to the selected approach: • The mean of the log of number of cycles to failure of all n failed samples or details. • The number of cycles to failure of the ﬁrst failed detail within n tested details. • The number of cycles to failure of the ﬁrst p failed details within n tested details. The tests should be performed according to well established and appropriate procedures or standards [68]. In order to relate the results of the fatigue test to service operation, an estimate of the standard deviation of log N is required, possibly taking into account the fact that this can vary along the S-N curve, see Fig. 3.1. If the number of test results n < 10, or if the procedure of ﬁrst failure or p failures in n specimens approach is used, the standard deviation in terms of log cycles can be conservatively estimated as follows: 0.18 for geometrically simple structures at fatigue endurances between 104 and 105 cycles 0.25 for complex structures at fatigue endurances up to 106 cycles No estimate can be given for fatigue endurances approaching the endurance limit. Here, special veriﬁcation procedures are recommended, see Ref. [69] 4.5.2 Acceptance Criteria The required or usable fatigue life of the component or structure should be less than the minimum probable fatigue life estimated on the basis of the tests, such that Nd \ NT F ð4:24Þ 104 4 Fatigue Assessment Table 4.4 F-factors for failure of all test specimens Stdv.\n 2 4 6 8 10 0.18 0.250 3.93 6.86 2.64 3.90 2.45 3.52 2.36 3.32 2.30 3.18 Table 4.5 F-factors for the ﬁrst test specimen to fail Stdv.\n 2 4 6 8 10 0.18 0.25 2.72 4.07 2.07 2.77 1.83 2.34 1.69 2.09 1.55 1.85 where NT The log mean fatigue life in cycles of the test specimens, or the life of the ﬁrst test specimen to fail, whichever is applicable F Factor dependent of the number of test results available as deﬁned in Tables 4.4 and 4.5 as appropriate. The F-factors refer to a survival probability as decribed in Sect. 3.7 Nd Number of cycles, up to which the component or structure may be used in service If all components or test specimens are tested to failure, values of F from Table 4.4 shall be used. If the tests are carried out until failure of the ﬁrst test specimen, values of F from Table 4.5 shall be used. The factor F may be further modiﬁed according to safety requirements as given in Sect. 5.3. 4.5.3 Safe Life Assessment Safe life assessment considers each structural element and detail as independent. Each element should fulﬁll the acceptance criteria deﬁned in Sect. 4.5.2. The partial safety factors γF applied to fatigue actions (loads) and γM applied to fatigue resistance may be selected from Table 5.1. 4.5.4 Fail Safe Assessment Fatigue life assessment of fail safe structures depends largely on the design and service operation parameters of the structure. The effectiveness of statically over-determined (hyperstatic) behaviour or redundancy of structural components, the possibility of detection of failures in individual structural parts and the 4.5 Fatigue Assessment on the Basis of Service Testing 105 possibility of repair determine the level of safety required in the individual structural parts. Consequently, no general recommendation can be given. The factor F given in Sect. 4.5.2 can be used for general guidance and to establish agreement. The partial safety factors γF applied to fatigue actions (loads) and γM applied to fatigue resistance may be selected from Table 5.1. 4.5.5 Damage Tolerant Assessment The veriﬁcation that a structure is damage tolerant requires the demonstration that the structure can sustain fatigue cracking without failure until such time as the cracking is detected. When fatigue testing is employed as a part of the veriﬁcation procedure, the failure criterion of the tests should be chosen to reflect the influence of the type of loading and the operation conditions of the actual structure. The criteria for factoring the observed lives obtained in the tests depend of the application. It is recommended to establish agreement on the choice of the factor F between the relevant parties. The partial safety factors γF applied to fatigue actions (loads) and γM applied to fatigue resistance may be selected from Table 5.1. Chapter 5 Safety Considerations 5.1 Basic Principles A component has to be designed for an adequate survival probability. The required survival probability depends on the • Uncertainties and scatter in the fatigue assessment data • Safety strategy • Consequences of failure. Uncertainties in the fatigue assessment data may also origin from the fatigue actions, such as • Determination of loads and load history • Determination of stresses or stress intensity factors from the model used for analysis • Dynamic response problems. These uncertainties can be covered by an appropriate partial safety factor for the fatigue actions γF, which is not considered here. However, it is emphasized that assumptions made at the design stage should be conservative and ideally checked during early stages of service operation. Uncertainties in a fatigue assessment arising from the fatigue resistance data and damage calculation methods include: • Scatter in fatigue resistance data, • Scatter of veriﬁcation results from damage calculations. The last two sources of uncertainty are considered here. For normal applications, they are already covered in the fatigue resistance data given here. For special applications, the data may be modiﬁed by the selection of an adequate partial safety factor γM. © Springer International Publishing Switzerland 2016 A.F. Hobbacher, Recommendations for Fatigue Design of Welded Joints and Components, IIW Collection, DOI 10.1007/978-3-319-23757-2_5 107 108 5.2 5 Safety Considerations Fatigue Design Strategies Different service operation conditions require different fatigue design strategies. The deﬁnition of a fatigue design strategy refers predominantly to the method of fatigue analysis, inspection and monitoring in service. 5.2.1 Inﬁnite Life Design This strategy is based on keeping all fatigue actions under an assumed resistance fatigue limit or threshold value. If regular in-service monitoring is not speciﬁed, the survival probability must be high. This strategy is most suited to components that experience very high numbers of cycles, which are uniform or preferably close to constant amplitude. The strategy often relies on the assumption that there is always a fatigue limit below which inﬁnite life can be expected. However, there are increasing doubts that this is the case for welded components. It is recommended that due consideration should be given to the adoption of am S-N curve that does not become horizontal at the CAFL or ‘knee’ point, but continues at a very shallow slope, as indicated in Sect. 3.2. 5.2.2 Safe Life Design This design strategy is used in situations where regular inspection in service is not possible or the consequences of failure are very high. Consequently a very high survival probability is required. 5.2.3 Fail Safe Design This design strategy is based on the assumption that the component or structure can tolerate extensive fatigue cracking without failing, possibly because it is statically over-determined (hyper-static) or there is an adequate redundancy. Regular monitoring in service is not usually provided. It is relied on the redistribution of forces if cracking does occur, which can be readily detected and repaired. Welded joints in such structures can be designed for a normal survival probability. 5.2.4 Damage Tolerant Design This design strategy is based on the assumption that fatigue cracks will form but they will be readily detectable in service before they become critical. 5.2 Fatigue Design Strategies 109 Fracture mechanics can be used to calculate suitably inspection intervals. However, apart from fatigue considerations it may also be necessary to ensure that the material is sufﬁciently tough to tolerate the largest fatigue crack that could be present before it has been detected. A normal probability of survival is adequate. 5.3 Partial Safety Factors The requirement for a partial safety factor to be applied to the fatigue resistance data γM depends largely on such circumstances as • Fatigue design strategy • Consequences of failure • Practical experience in ﬁelds of application. Examples of possible values for partial safety factors are given in Table 5.1, but no general recommendations can be given. In most cases of the use of the conservative fatigue resistance data given in the present recommendations, γM = 1 should be adequate for design or assessment of components or structures of normal fabrication quality, which will be regularly inspected in service. The safety factors γM = 1 are given in terms of stress. If safety factors are needed in terms of cycles, ΓM may be calculated using the exponent m of the resistance S-N curve or Paris power law of crack propagation.It should be noted that the slope m of the S-N resistance curves may vary over the range of application (e.g. see Fig. 3.1). CM;cycles ¼ cm M ð5:1Þ where ΓM, cycles refers to a partial safety factor in terms of cycles and γM refers to stress. No general recommendations on partial safety factors can be given. For special ﬁelds of application, safety factors on load actions γF and on fatigue resistance γM may be established. Table 5.1 shows a possible example for γM which may be adjusted according to the special requirements of the individual application. Table 5.1 Possible examples of partial safety factors γM for fatigue resistance Partial safety factor γM → Consequence of failure Fail safe and damage tolerant strategy Safe life and inﬁnite life strategy Loss of secondary structural parts Loss of the entire structure Loss of human life 1.0 1.15 1.30 1.15 1.30 1.40 110 5.4 5 Safety Considerations Quality Assurance Weld quality assurance is based on adequate organization of work flow in design, fabrication, destructive and non-destructive inspection of materials and welds, and the individual acceptance levels for the different types of weld imperfections. Acceptable levels for different types of weld imperfections related speciﬁcally to fatigue resistance may be found in Sect. 3.8 or in other fatigue based weld quality codes [e.g. 53]. Since more general weld quality acceptance criteria are needed for practical shop fabrication, the standards ISO 5817 for steel and ISO 10042 for aluminium are widely used. However, it should be noted that these are based more on traditional perceptions of what constitutes good workmanship, than on objective criteria related specially to the influence of the imperfection on the strength, including fatigue strength of the welded joint. Consequently they can be irrelevant, over-conservative and even potentially unsafe from the fatigue viewpoint. Nevertheless, there is a growing tendency to relate them to strength requirements. For example, ISO 5817:2006 quality level D might be speciﬁed for statically loaded structures and B for fatigue or special requirements, even though these levels are not completely consistent in terms of their effect on fatigue properties. Besides regulations and quality codes, the general standards of good workmanship should to be maintained. For conservative reasons, an ISO 5817:2006 level B or even B+ may be speciﬁed or modiﬁed in conjunction with Sect. 3.8 or other weld quality codes with an adequate consideration to fatigue [e.g. see Ref. 53]. It is recommended to have a documentation or a drawing on which the required fatigue class for each weld is written. If an imperfection needs an assessment, it can be done on a basis of fatigue performance. A direct relation to quality groups of ISO 5817 and fatigue properties is given in Ref. [76], see also Appendix 6.4. 5.5 Repair of Components The most common cause of damage in welded structures and components is fatigue. Before the start of any repair of such damage, it is vitally important to establish the reasons for its occurrence since these will influence decisions to be made about the need for repair and for the repair method [77–80]. Possible reasons for fatigue damage include: • Under-estimation of service loading, number of cycles and shape of load spectrum • Unexpected sources of fatigue loading • Inadequate stress analysis • Inadequate structural design, especially of weld details • Unsuitable material e.g. regarding toughness, corrosion resistance or weldability 5.5 Repair of Components 111 • Poor workmanship (e.g. parts missing or not properly positioned, unsatisfactory application of thermal cutting, signiﬁcant weld imperfections such as poor penetration, severe undercut, severe misalignment, unauthorized welding of fabrication aids) • Unexpected dynamic response leading to vibrations not considered in design • Environmental influences detrimental to fatigue e.g. corrosion or elevated temperature • Faulty operation, e.g. overload • Accident, e.g. collision In most cases of damage, design, loads and imperfections are the governing parameters of the failure, material properties are often secondary. The actions to be taken should be based on the results of the investigations. Possible actions are: • • • • No repair Delayed repair Immediate repair More frequent or continuous crack monitoring, in-service inspection or vibration monitoring • Change in operating conditions A large variety of repair methods exist. They may generally include the following aspects: • • • • • • Removal of crack Modiﬁcation of detail design Modiﬁcation of service loading Selection of adequate material and repair welding procedure Application of a weld toe improvements technique (see Sect. 5.2) Quality control of the repair weld 6 Appendices The appendices are intended to give special guidance, background information and additional explanations. They are not normative. 6.1 6.1.1 Loading History Markov Transition Matrix A Markov transition matrix is a method for recording the numbers of half-cycles of each particular stress range in a fatigue loading stress-time history and the number of ‘transitions’ from one extreme level (peak or trough) to another. Its general form is illustrated in Fig. 6.1. The actual spectrum is broken down into a number of equally spaced stress levels a1, a2, a3… an 32 stress levels are sufﬁcient. The two axes deﬁne the starting and the ﬁnishing level of each half-cycle, and each individual cell ai,j of the matrix deﬁnes the number of transitions from a level i to a level j stress. Falling stress half-ranges (from the peak in the stress-time history) appear in the cells below the diagonal, while rising stress half-cycles (from troughs in the stress-time history) appear in those above it, as indicated in Fig. 6.1. The data for the transition matrix can be obtained by measurement or by time simulation computations. A time stress-time signal for fatigue tests or crack propagation simulations or a cumulative frequency diagram (stress spectrum) for a damage calculation can be generated from the transition matrix by a Markov random draw (Table 6.1). 6.1.2 ‘Rainflow’ or ‘Reservoir’ Counting Method The algorithm of reservoir counting method is well explained by using the analogy of the flow of water from a reservoir, the boundary of which is the stress-time © Springer International Publishing Switzerland 2016 A.F. Hobbacher, Recommendations for Fatigue Design of Welded Joints and Components, IIW Collection, DOI 10.1007/978-3-319-23757-2_6 113 114 6 Appendices a(1,1) stress i a(1,j) a(1,n) stress j transition from min to max i<j a(i,1) transition from max to min i>j stress j stress i a(n,1) a(n,n) Fig. 6.1 Principle of the transition matrix Table 6.1 Illustration of a transition matrix 1 2 2 3 4 5 x 6 7 8 9 10 11 12 13 14 ↓ 30 31 32 3 x — — 4 # # x 4 # # # 5 x 6 — 7 — 8 9 — # # # 20 10 11 12 13 14 → 30 31 32 20 transitions from level 5 trough to level 9 peak x x x Rising ranges # x — — 45 x 45 transitions from level 4 peak to level 10 trough x x x Falling ranges x x x x x history, as illustrated in Fig. 6.2. Water is drained from the troughs in the stress-time history and the stress range is the largest drop before emptying that part of the reservoir. 6.1 Loading History 115 Fig. 6.2 Illustration of reservoir counting Rainflow counting is similar but in this case, the stress-time history is visualized as a pagoda roof and stress cycles are deﬁned in terms of the distances travelled by water flowing down the roof [58, 59]. The same results are obtained from each method. 6.2 6.2.1 Fracture Mechanics Rapid Calculation of Stress Intensity Factors A simpliﬁed method may be used to determine Mk-factors [31]. Here, the Mkfactors are derived from the non-linear total stress distribution σnl(x) along the anticipated crack path x assuming no crack being present. Hence, the function of the stress concentration factor kt,nl(x) can be calculated [33]. The integration for a certain crack length a yields: 2 Mk ¼ p Zx¼a x¼0 kt ; nlðxÞ pﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ dx a2 x 2 ð6:1Þ For different crack lengths a, a function Mk(a) can be established, which is preferably presented in the form: Mk ðaÞ ¼ const=aexp 6.2.2 Dimensions of Cracks See Table 6.2 Mk ðaÞ 1 ð6:2Þ 116 6 Appendices Table 6.2 Dimensions for assessment of crack-like imperfections (example) Idealizations and dimensions of crack-like imperfection for fracture mechanics assessment procedure (t = wall thickness). 6.2.3 Interaction of Cracks Adjacent cracks may interact and behave like a single large one. The interaction between adjacent cracks should be checked according to an interaction criterion. There are different interaction criteria, and in consequence no strict recommendation can be given. It is recommended to proceed according to an accepted codes and compilations, e.g. [53]. 6.2 Fracture Mechanics 6.2.4 117 Formulae for Stress Intensity Factors Stress intensity factor formulae may be taken from literature, see references [25– 32]. The formulae given below address most of the cases relevant to welded joints. 6.2.4.1 Standard Solutions See Table 6.3 Table 6.3 Stress intensity factors at welds Surface cracks under membrane stress The formula for the stress intensity factor K1 is valid for a/c < 1, for more details see Ref. [26] p K1 ¼ r ðp a = QÞ Fs Q ¼ 1 þ 1:464 ða=cÞ1:65 h i Fs ¼ M1 þ M2 ða=tÞ2 þ M3 ða=tÞ4 g f f w M1 ¼ 1:13 0:09 ða=cÞ M2 ¼ 0:54 þ 0:89= ð0:2 þ a=cÞ M3 ¼ 0:5 1= ð0:65 þ a=cÞ þ 14ð1 a=cÞ24 p f w ¼ ½secðp c ða=tÞ =ð2 bÞÞ1=2 g and f are dependent to direction ''a''direction : g ¼ 1 f ¼ 1 h i ''c''direction : g ¼ 1 þ 0:1 þ 0:35 ða=tÞ2 p f ¼ ða=cÞ Embedded cracks under membrane stress The formula for the stress intensity factor K1 is valid for a/c < 1, for more details see Ref. [27], where D is the diameter in mm and P is the internal pressure in N/mm2. (continued) 118 6 Appendices Table 6.3 (continued) K1, Q, Fs, fw as given before for surface cracks, but: M1 ¼ 1 M2 ¼ 0:05= 0:11 þ ða=cÞ3=2 M3 ¼ 0:29= 0:23 þ ða=cÞ3=2 g and f are dependent to direction ''a'' direction:g ¼ 1 f ¼ 1 ''c'' direction:g ¼ 1 ða=tÞ4 = ð1 þ 4a=cÞf ¼ p ða=cÞ Surface cracks under shell bending and membrane stress The formula for the stress intensity factor K1 is valid for a/c < 1, for more details see Ref. [26]. K1 ¼ ðrmem þ H rben Þ p ðp a = QÞ Fs 1:65 Q ¼ 1 þ 1:464ða=cÞ h i Fs ¼ M1 þ M2 ða=tÞ2 þ M3 ða=tÞ4 g f f w M1 ¼ 1:13 0:09 ða=cÞ M2 ¼ 0:54 þ 0:89= ð0:2 þ a=cÞ M3 ¼ 0:5 1= ð0:65 þ a=cÞ þ 14ð1 a=cÞ24 p f w ¼ ½secðp c ða=tÞ =ð2 bÞÞ1=2 g and f are dependent to direction ''a'' direction:g ¼ 1 f ¼ 1 h i p ''c'' direction:g ¼ 1 þ 0:1 þ 0:35ða=tÞ2 f ¼ ða=cÞ The function H is given by the formulae: ''a'' direction:H ¼ 1 þ G1 ða=tÞ þ G2 ða=tÞ2 where G1 ¼ 1:22 0:12 ða=cÞ G2 ¼ 0:55 1:05 ða=cÞ0:75 þ 0:47ða=cÞ1:5 ''c'' direction: H ¼ 1 0:34ða=tÞ 0:11ða=cÞ ða=tÞ Surface cracks under internal pressure The formula for the stress intensity factor K1 is valid for a/c < 1, for more details see Ref. [27], where D is the diameter in mm and P is the internal pressure in N/mm2. (continued) 6.2 Fracture Mechanics 119 Table 6.3 (continued) p K1 ¼ r ðp a = QÞ Fs S ¼ p Dinner = ð2tÞ Q ¼ 1 þ 1:464ða=cÞ1:65 h i Fs ¼ 0:97 M1 þ M2 ða=tÞ2 þ M3 ða=tÞ4 C g f f w M1 ¼ 1:13 0:09 ða=cÞ M2 ¼ 0:54 þ 0:89= ð0:2 þ a=cÞ M3 ¼ 0:5 1= ð0:65 þ a=cÞ þ 14ð1 a=cÞ24 p f w ¼ ½secðp c ða=tÞ =ð2 bÞÞ1=2 2 p C ¼ Dout þ D2in = D2out D2in þ 1 0:5 a=t 2t=Din g and f are dependent to direction ''a'' direction : g ¼ 1 f ¼ 1 h i p ''c'' direction : g ¼ 1 þ 0:1 þ 0:35ða=tÞ2 f ¼ ða=cÞ Through the wall cracks under internal pressure In sphere and longitudinal cracks in cylinder loaded by internal pressure. Mk covers increase of stress concentration factor due to bulging effect of shell. For details see Ref. [27, 30] pﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ K ¼ rmem ðp aÞ Mk where Mk = 1.0 for x < 0.8 and pﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ Mk ¼ ð0:95 þ 0:65 x 0:035 x1:6 Þ for x [ 0:8 and x < 50 pﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ with x ¼ a = ðr tÞ a half distance between crack tips of through the wall crack r radius of curvature perpendicular to the crack plane t wall thickness Root gap in a ﬁllet welded cruciform joint The formula for the stress intensity factor K is valid for H/t from 0.2 to 1.2 and for a/w from 0.0 to 0.7. For more details see Ref. [29]. K= rðA1 þ A2 a=wÞðpa secðpa=2wÞÞ 1 þ 2H=t where w ¼ H þ t=2 σ = nominal stress range in the longitudinal plates and with x ¼ H=t A1 ¼ 0:528 þ 3:287 x 4:361 x2 þ 3:696 x3 1:875 x4 þ 0:415 x5 A2 ¼ 0:218 þ 2:717 x 10:171 x2 þ 13:122 x3 7:755 x4 þ 1:783 x5 Parametric formulae for Mk functions have been established for a variety of types of welded joints [31, 32] (Table 6.4). 120 6 Appendices Table 6.4 Formulae for Mk values for different welded joints Transverse non-loadcarrying attachment Dim: H=T W=T h A=T t=T Mk ¼ C a k T min 0:2 0:2 15 0:175 0:125 max 1 1 60 0:72 2 Mk ¼ 1 C ¼ 0:8068 0:1554 k ¼ 0:1993 0:8139 H H þ 0:0429 T T 2 H H þ 0:0495 T T 2 þ 0:0794 W T þ 0:0815 H T (1) Cruciform joint K-butt weld Dim: H=T W=T h A=T t=T Mk ¼ C a k T min 0:2 0:2 15 0:175 0:5 max 1 1 60 1:3 20 Mk 1 C ¼ 0:7061 0:4091 k ¼ 0:2434 0:3939 H H þ 0:1596 T T H H þ 0:1536 T T 2 þ 0:3739 2 þ 0:3004 W T W T 0:1329 0:0995 W T W T 2 (2) 2 Cruciform joint ﬁllet welds Dim: H=T W=T h A=T t=T Mk ¼ C min 0:2 0:2 15 0:175 0:5 max 1 1 60 0:8 10 a k Mk 1 T If 0.2 < H/T < 0.5 and 0.2 < W/T <0.5 and a/T < 0.07 then: H W C ¼ 2:0175 0:8056 1:2856 T T H W k ¼ 0:3586 0:4062 þ 0:3004 T T If 0.2 < H/T < 0.5 and 0.2 < W/T <0.5 and a/T > 0.07 then: H W þ 0:69421 C ¼ 2:2916 0:0620 T T H W k ¼ 1:1146 0:213224062 þ 1:4319 T T If 0.5 < H/T < 1.5 and 0.5 < W/T <1.5 (3) (4) (continued) 6.2 Fracture Mechanics 121 Table 6.4 (continued) 2 H H þ 0:1753 T T C ¼ 0:9055 0:4369 þ 0:0665 H H þ 0:2167 T T k ¼ 0:2307 0:5470 2 W T 2 (5) W T þ 0:2223 Lap joint Mk ¼ C Dim: H=T W=T U=T h A=T t=T a k min 0:25 0:25 0 15 0:175 0:5 max 1 2 1:5 60 0:8 10 Mk 1 (6) T H H þ 0:1844 T T C ¼ 1:0210 0:3772 k ¼ 0:4535 0:1121 2 þ 0:0187 H W þ 0:3409 T T 0:0824 W T W T 2 0:1856 2 þ 0:0877 U U þ 0:1362 T T U T 0:0417 2 U T 2 Longitudinal non-loadcarrying attachment Mk ¼ C a k T Dim. min Dim: L=T B=T h=45 t=T A ¼ 0:7 max min 5 2:5 0:670 0:25 t max 40 40 1:33 2 Mk ¼ 1 (7) C ¼ 0:9089 0:2357 t k ¼ 0:02285 þ 0:0167 þ 0:0249 T t T 0:3863 L L 0:00038 T T 2 H H þ 0:1230 45 45 þ 0:0186 B H 0:1414 T 45 2 An example of a 3-dimensional Mk-solution was published by Bowness and Lee [35–37] (Fig. 6.3): The ﬁtted formulae are valid for membrane stress and a weld toe angle of 45° and: 0:005\ a=t \1:0 0:1\ a=c \1:0 0:5\ L=t \2:75 if L=t [ 2:75 then L=t ¼ 2:75 122 6 Appendices Fig. 6.3 Relevant dimensions for different joint types Membrane stress: Deepest point g1 ¼ 1:0343 ða/cÞ2 0:15657 ða/cÞ þ 1:3409 g2 ¼ 1:3218 ða/cÞ0:61153 g3 ¼ 0:87238 ða/cÞ þ 1:2788 g4 ¼ 0:46190 ða/cÞ3 þ 0:6709 ða/cÞ2 0:37571 ða/cÞ þ 4:6511 g3 f1 ¼ 0:43358 ða/tÞðg1 þ ðg2 ða=tÞÞ Þ þ 0:93163 expðða/tÞ0:050966 Þ f2 ¼ 0:21521 ð1 ða/tÞÞ176:4199 þ 2:8141 ða/tÞð0:1074ða=tÞÞ g5 ¼ 0:015647 ðL/tÞ3 þ 0:09089 ðL/tÞ2 0:17180 ðL/tÞ 0:24587 g6 ¼ 0:20136 ðL/tÞ2 þ 0:93311 ðL/tÞ 0:41496 g7 ¼ 0:20188 ðL/tÞ2 0:97857 ðL/tÞ þ 0:068225 g8 ¼ 0:027338 ðL/tÞ2 þ 0:12551 ðL/tÞ 11:218 f3 ¼ 0:33994 ða/tÞg5 þ 1:9493 ða/tÞ0 :23003 þ ðg6 ða/tÞ2 þ g7 ða/tÞ þ g8Þ Mka ¼ f1 þ f2 þ f3 if Mka\1 then Mka ¼ 1 surface point g1 ¼ 0:0078157 ðc/aÞ2 0:070664 ðc/aÞ þ 1:8508 g2 ¼ 0:000054546 ðL/tÞ2 þ 0:00013651 ðL/tÞ 0:00047844 g3 ¼ 0:00049192 ðL/tÞ2 0:0013595 ðL/tÞ þ 0:011400 g4 ¼ 0:0071654 ðL/tÞ2 0:033399 ðL/tÞ 0:25064 g5 ¼ 0:018640 ðc/aÞ2 þ 0:24311 ðc/aÞ 1:7644 g6 ¼ 0:0016713 ðL/tÞ2 þ 0:0090620 ðL/tÞ 0:016479 g7 ¼ 0:0031615 ðL/tÞ2 0:010944 ðL/tÞ þ 0:13967 g8 ¼ 0:045206 ðL/tÞ3 þ 0:32380 ðL/tÞ2 0:68935 ðL/tÞ þ 1:4954 2 2 f1 ¼ g1 (a/t)ðg2ðc=aÞ þ g3ðc=aÞ þ g4Þ þ g5 ð1 (a/t)Þðg6ðc=aÞ þ g7ðc=aÞ þ g8Þ þ g9 6.2 Fracture Mechanics 123 g9 = 0:25473 ða/c)2 þ 0:40928 ða/c) + 0:0021892 g10 = 37:423 ða/c)2 15:741 ða/c) + 64:903 f2 ¼ 0:28639 (a/c)2 þ 0:35411 (a/c) þ 1:643 (a/t)g9 þ 0:27449 ð1 (a/t)Þg10 g11 ¼ 0:10553 ðL/t)3 þ 0:59894 ðL/t)2 1:0942 ðL/t) 1:2650 g12 = 0:043891 ðL/t)3 0:24898 ðL/t)2 þ 0:44732 ðL/t) + 0:60136 g13 ¼ 0:011411 ða/c)2 þ 0:004369 ða/c) + 0:51732 f3 ¼ g11 (a/t)0:75429 þ g12 expð(a/t)g13 Þ Mkc ¼ f1 f2 f3 if Mkc\1 then Mkc ¼ 1 Bending stress: Deepest point g1 ¼ 0:014992 ða/c)2 0:02401 ða/c) 0:23851 g2 = 0:61775 ða/c)ð1:0278Þ g3 = 0:00013242 ða/cÞ1:4744 g4 = - 0:28783 ða/c)3 þ 0:58706 ða/c)2 0:37198 ða/c) 0:89887 fx ¼ ðg1 þ ðg2 (a/t)g3 Þ if fx [ 10 then fx ¼ 10 else f1 ¼ 0:065916 (a/t)fx þ 0:52086 expð(a/t)0:10364 Þ þ g4 g5 ¼ 17:195 ða/tÞ2 þ 12:468 ða/tÞ 0:51662 f2 ¼ 0:021995 ð1 a/tÞ2:8086 þ 0:021403 ða/tÞg5 g6 ¼ 0:059798 ðL/tÞ3 þ 0:38091 ðL/tÞ2 0:8022020 ðL/tÞ þ 0:31906 g7 ¼ 0:358 ðL/tÞ2 þ 1:3975 ðL/tÞ 1:7535 g8 ¼ 0:31288 ðL/tÞ2 1:3599 ðL/tÞ þ 1:6611 g9 ¼ 0:001470 ðL/tÞ2 0:0025074 ðL/tÞ 0:0089846 f3 ¼ 0:23344 (a/t)g6 0:14827 (a/t)0:20077 þ ðg7 (a/t)2 þ g8 (a/t) þ g9Þ Mka ¼ f1 þ f2 þ f3 if Mka\1 then Mka ¼ 1 124 6 Appendices Surface point g1 ¼ 0:0023232 (c/a)2 0:000371 (c/a) þ 4:5985 g2 ¼ 0:000044010 ðL/tÞ2 þ 0:00014425 ðL/tÞ þ 0:00086706 g3 ¼ 0:00039951 ðL/tÞ2 0:0013715 ðL/tÞ þ 0:014251 g4 ¼ 0:0046169 ðL/tÞ2 0:017917 ðL/tÞ 0:16335 g5 ¼ 0:018524 ðc/aÞ2 þ 0:27810 ðc/aÞ 5:4253 g6 ¼ 0:00037981 ðL/tÞ2 þ 0:0025078 ðL/tÞ þ 0:00014693 g7 ¼ 0:0038508 ðL/tÞ2 þ 0:023212 ðL/tÞ 0:026862 g8 ¼ 0:011911 ðL/tÞ3 þ 0:082625 ðL/tÞ2 0:16086 ðL/tÞ þ 1:2302 g9 ¼ 0:27798 ða/tÞ3 1:2144 ða/tÞ2 2:4680 ða/tÞ þ 0:099981 g10 ¼ 0:25922 ða/cÞ2 þ 0:39566 ða/cÞ þ 0:011759 fy ¼ ðg2 ðc/aÞ2 þ g3 ðc/aÞ þ g4Þ if fy [ 10 then f1 ¼ 0 else f1 ¼ g1 (a/t)fy þ g5 ð1 (a/t)Þðg6ðc=aÞ 2 þ g7ðc=aÞ þ g8Þ þ g9 2 g11 ¼ 6:5964 ða/cÞ þ 55:787 ða/cÞ þ 37:053 f2 ¼ ð0:35006 ða/cÞ2 þ 0:40768 ða/cÞ þ 1:7053Þ ða/tÞg 10 þ 0:24988 ð1 ða/tÞÞg11 g12 ¼ 0:14895 ðL/tÞ3 þ 0:815 ðL/tÞ2 1:4795 ðL/tÞ 0:89808 g13 ¼ 0:055459 ðL/tÞ3 0:30180 ðL/tÞ2 þ 0:54154 ðL/tÞ þ 0:53433 g14 ¼ 0:01343 ða/cÞ3 þ 0:0066702 ða/cÞ 0:75939 f3 ¼ g12 (a/t)0:94761 þ g13 exp (a/t)g14 Mkc ¼ f1 þ f2 þ f3 if Mkc\1 then Mkc ¼ 1 More detailed formulae containing the effect of the weld angle may be found in Ref. [37]. 6.2.4.2 Weight Function for a Surface Crack Here, an example of a 3-dimensional weight function for a given distribution of stress [40] is given: Za Ka ¼ Za rðxÞ Ma ðx; aÞ dx 0 Kc ¼ rðxÞ Mc ðx; aÞ dx 0 6.2 Fracture Mechanics 125 The weight functions for the stress intensity factors at the deepest point (a) and the surface (c) are: 2 x 12 x x 32 Ma ðx; aÞ ¼ pﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ 1 þ M1;a 1 þ M2;a 1 þ M3;a 1 a a a 2pða xÞ 1 3 2 x 2 x x 2 Mc ðx; aÞ ¼ pﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ 1 þ M1;c þ M2;c þ M3;c a a a p xÞ The coefﬁcients for the functions are: A0 ¼ 0:456128 0:114206 ða/cÞ 0:046523 ða/cÞ2 A1 ¼ 3:022 10:8679 ða/cÞ þ 14:94 ða/cÞ2 6:8537 ða/cÞ3 A2 ¼ 2:28655 þ 7:88771 ða/cÞ 11:0675 ða/cÞ2 þ 5:16354 ða/cÞ3 B0 ¼ 1:1019 0:019863 ða/cÞ 0:043588 ða/cÞ2 B1 ¼ 4:32489 14:9372 ða/cÞ þ 19:4389 ða/cÞ2 8:52318 ða/cÞ3 B2 ¼ 3:03329 þ 9:96083 ða/cÞ 12:582 ða/cÞ2 þ 5:3462 ða/c)3 a ¼ 1:14326 þ 0:0175996 ða/tÞ þ 0:501001 ða/tÞ2 b ¼ 0:45832 0:102985 ða/tÞ 0:398175 ða/tÞ2 c ¼ 0:97677 0:131975 ða/tÞ þ 0:484875 ða/tÞ2 d ¼ 0:448863 0:173295 ða/tÞ 0:267775 ða/tÞ2 Q ¼ 1 þ 1:464 ða/cÞ1:65 Y0 ¼ B0 þ B1 ða/tÞ2 þ B2 ða/tÞ4 Y1 ¼ A0 þ A1 ða/tÞ2 þ A2 ða/tÞ4 pﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ M1a ¼ 3:1415 ð4 Y0 6 Y1Þ= 2 Q 24=5 M2a ¼ 3 pﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ M3a ¼ 2 ð3:1415 Y0= 2 Q M1a 4Þ F1 ¼ a ða/cÞb F2 ¼ c ða/cÞd pﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ 4Q8 pﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ M2c ¼ 3:1415 ð60 F1 90 F2Þ= 4 Q 15 M1c ¼ 3:1415 ð30 F2 18 F1Þ= M3c ¼ 1 ð1 þ M1c þ M2cÞ The formulae are valid for 0 < a/t < 0.8 and for 0.2 < a/c < 1. 126 6.2.5 6 Appendices Stress Distribution at a Weld Toe Several parametric formulae exist, which may be useful for the weight function approach. An example is given here [42]. The formulae are valid for p p a 6 3 and 1 q 1 50 t 15 For membrane stress, the stress distribution is # 3 1 x 1 2 1 þ þ 2 q 2 Gm q0:454 qq m where kt;0 ¼ 1 þ 0:388 a0:37 ; Em ¼ 1:05 a0:18 t t x q q ¼ 0:12 a0:62 ; Tm ¼ 0:3 t t 0:94 expðEm Tm Þ x if Gm ¼ 0:06 þ [ 0:3 else Gm ¼ 1 3 0:8 1:1 q 1 þ Em Tm exp Em Tm m kt;0 r0 rm ðxÞ ¼ pﬃﬃﬃ 2 2 " x 1 þ q 2 12 For bending stress: Where b kt;0 r0 rb ðxÞ ¼ pﬃﬃﬃ 2 2 " x 1 þ q 2 12 1 x 1 þ þ 2 q 2 q0:469 b where kt;0 ¼ 1 þ 0:512 a0:573 ; t x q Tb ¼ 0:4 t t 0:93 expðEb Tbm Þ Gb ¼ 0:07 þ 1 þ Eb3 Tb0:6 exp Eb Tb1:2 32 # 1 Gb Eb ¼ 0:9 if qð0:0026 þ 0:0825=aÞ t x [ 0:4 q else Gb ¼ 1 where σ0 reference stress at the surface, structural stress at the toe k t,0 (x) geometrical stress concentration factor at the surface, m indicates membrane, b indicates bending x coordinate from surface down α weld angle in radians t wall thickness ρ weld toe radius σm(x) stress distribution for membrane stress σb(x) stress distribution for bending stress 6.3 Formulae for Misalignment 6.3 127 Formulae for Misalignment See Table 6.5 Table 6.5 Formulae for assessment of misalignment No Type of misalignment 1 Axial misalignment between flat plates km ¼ 1 þ k e l1 t ðl1 þ l2 Þ 2 λ is dependent on restraint, λ=6 for unrestrained joints. For remotely loaded joints assume l1=l2. Axial misalignment between flat plates of differing thickness 6e tn km ¼ 1 þ n 1 n t1 t1 þ t2 3 Relates to remotely loaded unrestraint joints. The use of n=1.5 is supported by tests. Axial misalignment at joints in cylindrical shells with thickness change 6e tn 1 km ¼ 1 þ t1 ð1 m2 Þ t1n þ t2n 4 n=1.5 in circumferential joints and joints in spheres. n=0.6 for longitudinal joints. Angular misalignment between flat plates Assuming ﬁxed ends: rﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ with b ¼ 2 l 3 rm t E 3 y tanhðb=2Þ km ¼ 1 þ t b=2 3 a l tanhðb=2Þ alternat.: km ¼ 1 þ 2t b=2 Assuming pinned ends: 6 y tanhðbÞ km ¼ 1 þ t b 3 a l tanhðbÞ alternat.: km ¼ 1 þ t b The tanh correction allows for reduction of angular misalignment due to the straightening of the joint under tensile loading. It is always ≤1 and it is conservative to ignore it. σm is membrane stress range. (continued) 128 6 Appendices Table 6.5 (continued) No Type of misalignment 5 Angular misalignment at longitudinal joints in cylindrical shells Assuming ﬁxed ends: rﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ 2 with b ¼ 2 l 3 ð1 m Þ rm t E 3d tanhðb=2Þ km ¼ 1 þ t ð1 m2 Þ b=2 assuming pinned ends: 6d tanhðbÞ km ¼ 1 þ t ð1 m2 Þ b d is the deviation from the idealized geometry Ovality in pressurized cylindrical pipes and shells 1:5 ðDmax Dmin Þ cos / km ¼ 1 þ " 0:5 pmax ð1 m2 Þ D t 1þ E t 6 7 3 # Axial misalignment of cruciform joints (toe cracks) e l1 t ðl1 þ l2 Þ λ is dependent on restraint km ¼ 1 þ k 8 9 λ varies from λ=3 (fully restrained) to λ=6 (unrestraint). For unrestrained remotely loaded joints assume: l1=l2 and λ=6 Angular misalignment of cruciform joints (toe cracks) l1 l2 km ¼ 1 þ k a t ðl1 þ l2 Þ λ is dependent on restraint If the in-plane displacement of the transverse plate is restricted, λ varies from λ=0.02 to λ=0.04. If not, λ varies from λ=3 to λ=6. Axial misalignment in ﬁllet welded cruciform joints (root cracks) e km ¼ 1 þ k tþh km refers to the stress range in weld throat. 6.4 Statistical Considerations on Safety 6.4 6.4.1 129 Statistical Considerations on Safety Statistical Evaluation of Fatigue Test Data The methods for evaluation of fatigue test data as described in Sect. 3.7 consider different statistical effects, when evaluating a set of fatigue data. Ideally, all the following effects should be considered, e.g. • • • • Variance of data Probability distribution of the mean value by its conﬁdence interval Probability distribution of the variance by its conﬁdence interval Difference of the distribution of the whole set of data (population) and the distribution of the sample (Gaussian versus t-distribution) • Deviation from the assumed Gaussian distribution which can be evaluated by a likelihood or χ2 testing For design, a safety margin is considered, which is applied to the mean values. The values used for design are the so called characteristic values (index k). These characteristic values are, in principle, values at a α = 95 % survival probability (5 % probability of failure) calculated from the mean value xm on the basis of two sided tolerance limits of the 75 % conﬁdence level of the mean xm, for details see Sect. 3.7. xk ¼ xm k Stdv ð6:3Þ The factor ki considers the ﬁrst four (as described above) and corresponds to: ∙ the minimum value of the mean conﬁdence interval ∙ the maximum value of the variance conﬁdence interval Taking into account that the probability distribution of the mean corresponds to a Student’s law (t-distribution) and the probability distribution of the variance corresponds to a Chi-square law (χ2), the general formula for ki is given by: tðp; n1Þ k1 ¼ pﬃﬃﬃ þ /1 ðaÞ n sﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ n1 2 v 1þb ð 2 ð6:4Þ ; n1Þ where t value of the two sided t-distribution (Student’s law) for p = β = 0.75, or of the one sided t-distribution for a probability of p = (1 + β)/2 = 0.875 at n-1 degrees of freedom n number of test results φ distribution function of the Gaussian normal distribution probability of exceedence of α = 95 % (superscript -1 indicates inverse function) χ2 Chi-square for a probability of (1 + β)/2 = 0.875 at n-1 degrees of freedom 130 6 Appendices Table 6.6 k-values for the different methods n t χ2 k1 k2 2 3 4 5 10 15 20 25 30 40 50 100 2.51 1.61 1.44 1.36 1.24 1.21 1.20 1.19 1.18 1.18 1.17 1.16 0.028 0.27 0.69 1.21 4.47 8.21 12.17 16.26 20.45 29.07 37.84 83.02 11.61 5.41 4.15 3.6 2.73 2.46 2.32 2.24 2.17 2.09 2.04 1.91 3.41 2.57 2.36 2.25 2.04 1.96 1.91 1.88 1.86 1.83 1.81 1.76 If the variance is ﬁxed from other tests or standard values, no conﬁdence interval has to be considered and so the factor is given by (Table 6.6): k2 ¼ 6.4.2 tð0:875; n1Þ tð0:875; n1Þ pﬃﬃﬃ pﬃﬃﬃ þ /1 þ 1:645 ð0:95Þ ¼ n n ð6:5Þ Statistical Evaluation of Results from Component Testing Testing All Test Specimens to Failure When all specimens are tested to failure, the procedure is to estimate the mean log NT of the S-N curve and the associated standard deviation. Starting from the formula in Sect. 4.5.2, there is Nd ¼ NT F ð6:6Þ which deﬁnes the safety factor F by: logðNT Þ logðFÞ [ logðNd Þ ð6:7Þ Taking the acceptance criterion xm − k·Stdv > xk from Sect. 3.7 the factor F can be deduced: 6.4 Statistical Considerations on Safety 131 logðFÞ ¼ k Stdv ð6:8Þ With the formula for k the different values of F can be calculated, depending on the number of test results n and on the assumed standard deviation Stdv of logN for those results. k¼ tð0:875; n1Þ tð0:875; n1Þ pﬃﬃﬃ pﬃﬃﬃ þ U1 þ 1:645 ð0:95Þ ¼ n n ð6:9Þ Testing All Test Specimens Simultaneously Until First Failure When all test specimens are tested simultaneously until the ﬁrst to fail, only one value of log NT is obtained and the standard deviation cannot be derived from test results (Table 6.7). Starting from the formula in Sect. 4.5.2, there is Nd ¼ NT F ð6:10Þ which deﬁnes the safety factor F by: logðNT Þ logðFÞ [ logðNd Þ ð6:11Þ When considering statistical evaluation, account must be taken of additional effects as illustrated in Fig. 6.4: • Distribution of the 1/n-th extreme value • Distribution of the sample between 1/n-th extreme and mean • Safety margin for the characteristic value Table 6.7 Values k testing until all failed n 2 4 6 8 10 100 k 3.34 2.37 2.19 2.10 2.04 1.76 Fig. 6.4 Distribution of action and resistance 132 6 Appendices Table 6.8 Values k for testing until ﬁrst failure n 2 4 k 2.44 1.77 For more details see Ref. [73, 74]. 6 8 10 1.48 1.28 1.07 where NT Life of ﬁrst specimen to fail xm Mean of the sample Nd Design value log NT is considered as the probable maximum (safe side) of the distribution of the minimum value of the log N distribution. The mean of the sample xm is therefore given by: xk ¼ xm ka a Stdv þ kb Stdv ð6:12Þ with Stdv standard deviation of the sample α from table of variance order statistics ka, kb from table of expected values of normal order statistics Taking the acceptance criterion xm − k1 Stdv > xk from Sect. 3.7, the factor F can be deduced: logðFÞ ¼ ðka a kb þ k1 Þ Stdv ð6:13Þ The different values of F can be calculated, depending on number of test results n and the assumed standard deviation Stdv of the test specimens in terms of log N (Table 6.8). Testing All Specimens Simultaneously Until p Failures Amongst n Specimens Values of k may be taken from the relevant literature or from Ref. [75]. 6.4.3 Statistical Considerations for Partial Safety Factors No general recommendations on partial safety factors are given. For special ﬁelds of application, safety factors on load actions γF and on fatigue resistance γM may be established. Table 6.9 shows a possible example for γM which may be adjusted according to the special requirements of the individual application. 6.5 Fatigue Resistance of ISO 5817 Quality 133 Table 6.9 Possible examples of partial safety factors γM for fatigue resistance Partial safety factor γM → consequence of failure Fail safe and damage tolerant strategy Safe life and inﬁnite life strategy Loss of secondary structural parts Loss of the entire structure Loss of human life 1.0 1.15 1.30 1.15 1.30 1.40 6.5 Fatigue Resistance of ISO 5817 Quality The quality groups B, C and D as deﬁned in ISO 5817 are not completely consistent in terms of fatigue properties of the welded joints. A correlation between the fatigue properties and the individual types of weld imperfections is given in Table 6.6. For more details, see Ref. [76] (Table 6.10). Note: The dimensions of acceptable weld imperfections within a quality group are partially dependent of the wall thickness and partially absolute values. So a wall thickness of 10 mm was chosen for the table. Absolute dimensions are less harmful for thicker walls and thus conservative. The limitations of fatigue resistance due to bigger wall thicknesses still apply. No. ISO 6520-1 1998 4021 5011 5012 1.6 1.7 502 401 1.5 5013 2025 1.4 1.9 Non-continuous undercut 2017 1.3 1.8 Continuous undercut 104 1.2 Excessive weld overﬁll Root notch Butt weld >3 >3 >3 Fillet weld (Toe crack) Butt weld >3 >3 Fillet weld (Toe crack) Butt weld >3 >6 >6 >6 >6 t mm Butt weld Veriﬁcation of net section! Fillet weld (Root crack) Fitness for purpose assessment by fracture mechanics recommended. Butt weld Micro lack of fusion Insufﬁcient root penetration Fitness for purpose assessment by fracture mechanics recommended Fillet weld (Root crack) Butt weld Fillet weld (Root crack) Butt weld Fitness for purpose assessment by fracture mechanics recommended Fitness for purpose assessment by fracture mechanics recommended Remarks Lack of fusion Open end crater cavity Surface pore End crater crack 100 Crack Type of imperfection 1.1 1 Surface imperfections No ISO 5817 2006 Table 6.10 Fatigue resistance of weld imperfections as deﬁned by ISO 5817-2006 for steel FAT 80 FAT 40 FAT 63 FAT 71 FAT 63 FAT 71 FAT 63 FAT 40 FAT 63 Not allowed FAT 40 FAT 40 FAT 40 FAT 40 Not allowed Not allowed D FAT 80 FAT 71 FAT 80 FAT 90 FAT 80 FAT 90 Not allowed FAT 40 FAT 80 Not allowed FAT 40 FAT 71 FAT 40 FAT 71 Not allowed Not allowed C (continued) FAT 90 FAT 90 FAT 80 FAT 90 FAT 80 FAT 90 Not allowed Not allowed Not allowed Not allowed Not allowed Not allowed Not allowed B Maximum usable fatigue class FAT in assessment by nominal stress method for the different quality groups 134 6 Appendices 510 512 515 516 517 5213 5214 601 1.15 1.16 1.17 1.18 1.19 1.20 1.21 1.22 Arc strikes Excessive throat thickness Insufﬁcient throat thickness Insufﬁcient weld start Root porosity Root concavity Excessive asymmetry Blowholes FAT 90 FAT 63 Fillet weld (Toe crack) FAT 40 FAT 40 Butt weld Root crack Root crack, veriﬁcation of net section! FAT 71 FAT 40 FAT 40 FAT 71 FAT 63 Fillet weld (Root crack) >6 >6 >6 FAT 80 Not allowed FAT 40 FAT 40 FAT 80 FAT 63 FAT 80 FAT 80 FAT 63 D Not allowed FAT 40 FAT 40 Not allowed Not allowed FAT 71 FAT 80 Not allowed FAT 71 FAT 71 Not allowed FAT 71 FAT 80 FAT 80 FAT 71 C (continued) Not allowed FAT 40 Not allowed Not allowed Not allowed FAT 90 FAT 80 Not allowed FAT 90 FAT 90 Not allowed FAT 80 FAT 90 FAT 90 FAT 80 B Maximum usable fatigue class FAT in assessment by nominal stress method for the different quality groups Butt weld Fillet weld (Root crack) Butt weld Fillet weld (Toe crack) >3 Root sagging >3 Fillet weld (Toe crack) 511 1.14 >3 Butt weld >6 >3 >3 506 1.13 Incorrect weld toe Fillet weld Sagging, incomplete ﬁlled groove 505 1.12 Excessive root overﬁll Excessive convexity t mm 509 504 1.11 Remarks >3 503 1.10 Type of imperfection Overlap No. ISO 6520-1 1998 No ISO 5817 2006 Table 6.10 (continued) 6.5 Fatigue Resistance of ISO 5817 Quality 135 602 1.23 2014 2015 2016 202 2.5 2.6 2.7 Porosity 2012 2013 2011 2.3 2.4 Pore 1001 2.2 Cavity Wormhole Pore line Pore net clustered porosity Micro-crack 100 Crack Sputter Type of imperfection 2.1 2. Inner imperfections No. ISO 6520-1 1998 No ISO 5817 2006 Table 6.10 (continued) Fillet weld (Root crack) Butt weld Fillet weld (Root crack) Butt weld Fillet weld (Root crack) Butt weld Fillet weld (Root crack) Without a special assessment, or at an additional limitation of projected area. Butt weld Fillet weld (Root crack) Butt weld Fillet weld (Root crack) Fitness for purpose assessment by fracture mechanics recommended Fitness for purpose assessment by fracture mechanics recommended >6 >6 >6 >6 >6 >6 FAT 40 FAT 71 FAT 40 FAT 71 FAT 40 FAT 71 FAT 40 FAT 50 ≤5 % : FAT 71 FAT 40 FAT 80 FAT 40 FAT 63 Not allowed FAT 63 Fillet weld (Toe crack) D Not allowed FAT 40 FAT 80 FAT 40 FAT 80 FAT 40 (continued) Not allowed FAT 40 FAT 90 FAT 40 FAT 90 FAT 40 FAT 40 FAT 71 ≤3 %: FAT 90 FAT 40 FAT 125 Not allowed Not allowed FAT 63 FAT 90 B FAT 63 ≤4 % : FAT 80 FAT 100 Not allowed Not allowed FAT 63 FAT 90 C Maximum usable fatigue class FAT in assessment by nominal stress method for the different quality groups FAT 90 t mm Depending on surface quality. Butt weld Remarks 136 6 Appendices No. ISO 6520-1 1998 2024 300 301 302 303 304 3042 401 4011 4012 4013 402 No ISO 5817 2006 2.8 2.9 2.10 2.11 2.12 2.13 Table 6.10 (continued) Lack of penetration (At longer imperfection veriﬁcation of net section!) Lack of penetration Flank LOP Interpass LOP Root LOP Copper inclusion Metallic inclusion except copper Solid inclusion Slag inclusion Flux inclusion Oxide inclusion End crater cavity Type of imperfection FAT 40 FAT 36 Fillet weld (Root crack) FAT 36 Fillet weld (Root crack) FAT 36 FAT 40 Butt weld HV-Weld FAT 40 Fillet weld (Root crack) Butt weld FAT 100 Butt weld FAT 100 FAT 40 Fillet weld (Root crack) FAT 36 Fillet weld (height of inclusion < 1/4- a), Root crack Butt weld FAT 56 L ≤ 10 mm: FAT 71 Butt weld (height of inclusion < 1/4-t) or at additional limitation of length L FAT 71 D Not allowed Not allowed Not allowed Not allowed FAT 40 FAT 100 FAT 40 FAT 100 FAT 40 FAT 63 L ≤ 4 mm: FAT 80 Not allowed C (continued) Not allowed Not allowed Not allowed Not allowed FAT 40 FAT 125 FAT 40 FAT 125 FAT 40 FAT 80 L ≤ 2,5 mm: FAT 90 Not allowed B Maximum usable fatigue class FAT in assessment by nominal stress method for the different quality groups FAT 40 >6 t mm Fillet weld (Root crack) Butt weld Remarks 6.5 Fatigue Resistance of ISO 5817 Quality 137 Type of imperfection 508 617 (3.2)a 3.2 none none 4.1 4.2 4. Multiple imperfections 507 3.1 Multiple imperfection in longitudinal direction of weld Engineering assessment of interactionb Engineering assessment of interactionb Without influence Lack of ﬁt at ﬁllet welds Multiple imperfections in arbitrary section calculative veriﬁcation recommended, if necessary calculative veriﬁcation recommended, if necessary Angular misalignment Angular misalignment Remarks >6 t mm FAT 36 FAT 45 D FAT 56 FAT 63 C FAT 90 FAT 90 B Maximum usable fatigue class FAT in assessment by nominal stress method for the different quality groups b This item is no longer part of ISO 5817:2006, but it was contained in ISO 5817:2003. Nevertheless, this item is relevant for fatigue Only general remarks can be given for engineering assessment. It may be done by veriﬁcation of the net section using FAT 36, by the effective notch stress method or by fracture mechanics considerations a No. ISO 6520-1 1998 3. Imperfecions of weld geometry No ISO 5817 2006 Table 6.10 (continued) 138 6 Appendices References General 1. ISO 2394 General principles on reliability for structures. Second edition 1986-10-14 2. Niemi E (1995) Recommendations concerning stress determination for fatigue analysis of welded components. IIW doc. XIII-1458-92/XV-797-92 Abington Publishing, Cambridge 3. Gurney TR (1978) Fatigue of welded structures. Cambridge University Press, Cambridge 4. Maddox SJ (1991) Fatigue strength of welded structures. Abington Publishing, Abington 5. Radaj D (1990) Design and analysis of fatigue resistent welded structures. Abington Publishing, Cambridge 6. Hobbacher A et al (1982) Design recommendations for cyclic loaded welded steel structures IIW doc. XIII-998-81/XV-494-81. Weld World 20:153–165 7. Radaj D, Sonsino CM, Fricke W (2006) Fatigue assessment of welded joints by local approaches, 2nd ed. Woodhead Publishing, Cambridge, UK 8. Gurney TR (2006) Cumulative damage of welded joints. Woodhead Publishing Ltd., Cambridge, UK. ISBN-13:978-1-85573-938-3 Structural Hot Spot Stress Procedure: 9. Huther M, Henry J Recommendations for hot spot stress deﬁnition in welded joints. IIW doc. XIII-1416-91 10. Huther M, Parmentier G, Henry J Hot spot stress in cyclic fatigue for linear welded joints. IIW doc. XIII-1466-92/XV-796-92 11. Niemi E, Fricke W, Maddox SJ (2006) Fatigue analysis of welded components—designer’s guide to structural hot-spot stress approach. IIW doc. XIII-1819-00/XV-1090-01, update June 2003. Woodhead Publishing, Cambridge, UK 12. Dong P, Hong JK (2002) Assessment of ASME’s FSRF rules for vessel and piping welds using a new structural stress method (Master S-N Curve Approach). IIW doc. XIII-1929-02/XV-1182-02. Weld World 48:28–36 13. Doerk O, Fricke W, Weissenborn Ch Comparison of different calculation methods for structural stresses at weld joints. IIW doc. XIII-1919-02/XV-1124-02 14. Zhao X-L, Packer JA (2000) Recommended fatigue design procedure for welded hollow section joints. IIW doc. XIII-1772-99 / XV-1021-99. Abington Publishing, Abington, Cambridge © Springer International Publishing Switzerland 2016 A.F. Hobbacher, Recommendations for Fatigue Design of Welded Joints and Components, IIW Collection, DOI 10.1007/978-3-319-23757-2 139 140 References 15. Haibach E (1968) Die Schwingfestigkeit von Schweissverbindungen aus der Sicht einer örtlichen Beanspruchungsmessung (The fatigue strength of welded joints considered on the basis of a local stress measurement). LBF Report FB77, Fraunhofer-Inst. f Betriebsfestigkeit Darmstadt Germany 16. Xiao Z-G, Yamada K (2004) A method of determining geometric stress for fatigue strength evaluation of steel welded joints. Int J Fatigue 26:1277–1293 and IIWdoc. XIII-2022-04/ XV-1175-04 Effective Notch Stress Procedure 17. Petershagen H (1986) A comparison of approaches to the fatigue strength assessment of welded components IIW document XIII-1208-86 18. Petershagen H (1989) Experiences with the notch stress concept according to Radaj (transl.) 15. Vortragsveranstaltung des DVM Arbeitskreises Betriebsfestigkeit, Ingolstadt 18.-19.10 19. Olivier R, Köttgen VB, Seeger T (1989) Welded connections I: Fatigue assessment of welded connections based on local stresses (transl.) Forschungskuratorium Maschinenbau, Bericht No. 143, Frankfurt 1989 (143 pages) 20. Köttgen VB, Olivier R, Seeger T (1991) Fatigue analysis of welded connections based on local stresses IIW document XIII-1408-91 21. Morgenstern C, Sonsino CM, Hobbacher A (2004) Fatigue design of aluminium welded joints by local stress concept with the ﬁctitious notch radius of rf = 1 mm. IIW-Doc. No. XIII–2009–04 22. Fricke W (2006) Round robin study on stress analysis for the effective notch stress approach. IIW document XIII-2129-06/XV-1223-06 23. Fricke W (2008) Guideline for the fatigue assessment by notch stress analysis for welded structures. IIW document XIII-2240-08/XV-1289-08 24. Hobbacher. A. Database for the Effective Notch Stress Method at Steel. IIW Joint Working Group Doc. JWG-XIII-XV-197-08, International Institute of Welding (2008) Fracture Mechanics 25. Murakami Y (1987) Stress intensity factors handbook. Pergamon Press, Oxford 26. Newman JC, Raju IS (1983) Stress intensity factor equations for cracks in three-dimensional ﬁnite bodies. ASTM STP 791:I-238–I-265. 27. Newman JC, Raju IS (1980) Stress intensity factors for internal surface cracks in cylindrical pressure vessels. J Press Vessel Technol 102:342–346 28. Newman JC, Raju IS (1981) An empirical stress intensity factor equation for the surface crack. Eng Fract Mech 15(1–2):185–192 29. Frank KH, Fisher JW (1979) Fatigue strength of ﬁllet welded cruciform joints. J Struct Div Proc ASCE 105:1727–1740 30. Folias ES (1965) Axial crack in pressurized cylindrical shell. Int J Fract Mech 1(2):104 31. Hobbacher A (1993) Stress intensity factors of welded joints. Eng Fract Mech 46(2):173–182; (1994) 49(2):323 32. Maddox SJ, Andrews RM (1990) Stress intensity factors for weld toe cracks, in ‘Localized Damage Computer Aided Assessment and Control’. In: Aliabadi MH, Brebbia CA, Cartwright DJ (eds) Computational Mechanics Publications, Southamton. ISBN 1 853 12 070 7; co-published with Springer-Verlag, Heidelberg, ISBN 3 540 527 17 6 33. Albrecht P, Yamada K (1977) Rapid calculation of stress intensity factors. J Struct Div ASCE 103(ST2):377–389 References 141 34. Pang HLJ (1990) A review of stress intensity factors for semi-elliptical surface crack in a plate and ﬁllet welded joint. The Welding Institute, Abington, Cambridge, UK, TWI Report 426/1990 IIW doc. XIII-1433-91 35. Bowness D, Lee MMK (1996) Stress intensity factor solutions for semi-elliptical weld-toe cracks in T-butt geometries. Fatigue Fract Eng Mater Struct 19(6):787–797 36. Bowness D, Lee MMK (2000) Prediction of weld toe magniﬁcation factors for semi-elliptical cracks in T-but joints. Int J Fatigue 22(5):389–396 37. Bowness D, Lee MMK (2002) Fracture mechanics assessment of fatigue cracks in offshore tubular structures. University of Swansea, Swansea, UK. ISBN 0 7176 23289 38. Nykänen T, Marquis G, Björk T Simpliﬁed assessment of weld quality for fatigue loaded cruciform joints. IIW document XIII-2177-07. 39. Fett T, Munz D (1997) Stress intensity factors and weight functions. Computational Mechanics Publications, Southampton 40. Shen G, Plumtree A, Glinka G (1991) Weight function for the surface point of semi elliptical surface crack in a ﬁnite thicknedd plate. Eng Fract Mech 40(1):167–176 41. Moftakhar AA, Glinka G (1992) Calculation of stress intensity factors by efﬁcient integration of weight functions. Eng Fract Mech 43(5):749–756 42. Hall MS, Topp DA, Dover WD (1995) Parametric equations for stress intensity factors in weldments. Project Report TSC/MSH/0244, Technical Software Consultants Ltd., Milton Keynes, U.K. 1990 taken from: Mohanan CC (ed) Early Fatigue Crack Growth at Welds, Computational Mechanics Publications, Southampton UK 1995. 43. Fracture Mechanics Proof of strength for engineering components. VDMA-Verlag Frankfurt-M, Germany (2009) 44. Engesvik KM (1981) Analysis of uncertainties in the fatigue capacity of welded joints. Doctoral thesis, Division of Marine Structures, University of Trondheim, Norwegian Institute of Technology, Trondheim Norway Fatigue Strength Modiﬁcations 45. Ørjasæter O (1995) Effect of plate thickness on fatigue of welded components. IIW doc. XIII-1582-95/XV-890-95 46. Haagensen PJ, Maddox SJ (2006) IIW Recommendations for weld toe improvement by grinding, TIG dressing and hammer peening for steel and aluminium structures. IIW doc. XIII-1815-00 (rev. 24 Feb. 2006). (See more references listed in document!) 47. Krebs J, Kassner M (2006) Influence of welding residual stresses on fatigue design of welded joints and components. IIW doc. XIII-2126-06/XV-1220-06 Weld Imperfections 48. ISO 6520:1982: Weld irregularities 49. ISO 5817:2006: Welding—fusion-welded joints in steel, nickel, titanium and their alloys— quality levels for imperfections 50. ISO 10042: Welding—arc-welded joints in aluminium and its alloys—quality levels for imperfections 51. IIW guidance on assessment of the ﬁtness for purpose of welded structures. IIW doc. SST-1157-90 (1990) 52. Hobbacher A et al (1988) Recommendations for assessment of weld imperfections in respect of fatigue. IIW doc. XIII-1266-88/XV-659-88 142 References 53. BS 7910:2005: Guidance on methods for assessing the acceptability of flaws in metallic structures British Standard Institution, London 54. Ogle MH (1991) Weld quality speciﬁcations for steel and aluminium structures. IIW doc. XV-776-91. Weld World 29(11/12):341–362 55. Berge S, Myhre H (1977) Fatigue strength of misaligned cruciform and butt joints. IIW doc. XIII-863-77. Norw Marit Res 5(1) 56. Maddox SJ (1985) Fitness for purpose assessment of misalignment in transverse butt welds subject to fatigue loading. IIW doc. XIII-1180-85 (more references in the document) 57. Hobbacher A (2006) Problems of effect of weld imperfections on fatigue and their consideration in design codes. Int J Steel Struct 6:289–298 Stress Spectrum 58. Endo T et al (1974) Fatigue of metals subjected to varying stress - prediction of fatigue lives (transl.) Kyushu District Meeting of the JSME, Nov. 1967. also: Rain flow method—the proposal and the applications. Memoir Kyushu Institute of Technical Engineering 59. Standard Practice for Cycle Counting in Fatigue Analysis. ASTM E 1049-85 Damage Calculation 60. Palmgren A (1924) On life duration of ball bearings (transl.). VDI-Z 68:339–341 61. Miner AM (1945) Cumulative damage in fatigue. J Appl Mech 151–164 62. Haibach E (1970) Modiﬁed linear damage accumulation hypothesis considering the decline of the fatigue limit due to progressive damage (transl.) Laboratorium für Betriebsfestigkeit, Darmstadt, Germany, Techn. Mitt. TM 50/70 63. Hobbacher A (1977) Cumulative fatigue by fracture mechanics. Trans ASME Ser E J Appl Mech 44:769–771 64. Sonsino CM, Maddox SJ, Hobbacher A (2004) Fatigue life assessment of welded joints under variable amplitude loading—state of present knowledge and recommendations for fatigue design regulations. In: Proceedings of the annual IIW-assembly and international conference, July 15–16, 2004 Osaka/Japan, S. 87–102 65. Sonsino CM, Wiebesiek J (2007) Assessment of multiaxial spectrum loading of welded steel and aluminium joints by modiﬁed equivalent stress and Gough-Pollard algorithms. IIW doc. XIII-2158r1-07/XV-1250r1-07 66. Sonsino CM, Maddox SJ, Haagensen P (2005) A short study on the form of the S-N curves for weld details in the high-cycle-fatigue regime. IIW doc. XIII-2045-05 67. Bäckström M (2000) Multiaxial fatigue life assessment of welds based on nominal and hot spot stresses. Doctoral Thesis Lappeenranta Univ. of Technology Lappeenranta Finland 2003. VTT Publications 502/1235-0621, VTT Information Service, POB 2000, FIN-02044 VTT. ISBN 951-38-6233-X Fatigue Testing 68. Lieurade HP, Huther M, Maddox SJ (2006) Recommendations on fatigue testing of welded joints IIW doc. XIII-2114-06 (ISO proposal) 69. Sonsino CM (2007) Fatigue testing under variable amplitude loading. Int J Fatigue 29:1080– 1089 References 143 70. Dixon WJ, Mood AM (1948) A method for obtaining and analyzing sensitivity data. J Am Stat Assoc 43:108–126 71. Spindel JE, Haibach E (1979) The method of maximum likelihood applied to the statistical analysis of fatigue data including run-outs. Int J Fatigue 1(2):81–88 72. Sonsino CM, Bruder Th, Baumgartner JS-N (2010) Lines for welded thin joints—suggested slopes and FAT values for applying the notch stress concept with various reference radii. Weld Worls 54(11/12) Quality and Safety Considerations 73. Huther M (1990) Uncertainties, conﬁdence intervals and design criteria IIW doc. XIII-1371-90 74. Schneider CRA, Maddox SJ (2006) Best practise guide on statistical analysis of fatigue data obtained from specimens containing many welds. IIW doc. XIII-2138-06 75. Marquis G, Mikkola T (2000) Analysis of welded structures with failed and non-failed welds, based on maximum likelihood. IIW document XIII-1822-00 76. Hobbacher A, Kassner M (2012) On relation between fatigue properties of welded joints vs. quality criteria and groups in ISO 5817. IIW doc. XIII-2323r1-10. Weld World 11–12 Fatigue Failure and Repair 77. Anon (1973/1979) Fatigue fractures in welded constructions. Publication de la Soudure Autogène, vols. 1, II 78. Anon (1990) IIW Guidance on assessment of ﬁtness-for-purpose of welded structures. IIW SST-1157-90 79. Petershagen H (1996) IIW Recommendations on the Repair of Fatigue-Loaded Welded Structures. IIW doc. XIII-1632-96 80. Miki C, Goto K, Itoh Y Database of repair cases for fatigue failure on the internet. IIW doc. XIII-1830-00. http://www.wg5.cv.titech.ac.jp